thesis final

Upload
sjoerdsmit 
Category
Documents

view
47 
download
1
Embed Size (px)
Transcript of thesis final
Passivating selective contacts for siliconphotovoltaics
Solar cells designed by physics
PROEFSCHRIFT
ter verkrijging van de graad van doctor aan deTechnische Universiteit Eindhoven, op gezag van de
rector magnificus prof.dr.ir. F.P.T. Baaijens, voor eencommissie aangewezen door het College voor
Promoties, in het openbaar te verdedigenop dinsdag 14 juni 2016 om 16:00 uur
door
Sjoerd Smit
geboren te Waalwijk
Dit proefschrift is goedgekeurd door de promotoren en de samenstellingvan de promotiecommissie is als volgt:
voorzitter: prof.dr. H.J.H. Clercx1e promotor: prof.dr.ir. W.M.M. Kessels2e promotor: prof.dr. M. Zeman (TUD)leden: prof.dr.ir. P.P.A.M. van der Schoot
prof.dr. J. Gomez RivasProf.Dr. K. Lips (Freie Universitat Berlin)Dr.rer.nat. P.P. Altermatt (Trina Solar Ltd.)
adviseur: dr. P.C.P. Bronsveld (ECN Solar Energy)
Het onderzoek dat in dit proefschrift wordt beschreven is uitgevoerd inovereenstemming met de TU/e Gedragscode Wetenschapsbeoefening.
Funding information
This research is supported by the Dutch Technology Foundation STW,which is part of the Netherlands Organisation for Scientific Research(NWO) and partly funded by the Ministry of Economic Affairs (FLASHproject 1.4: Advanced Interface Engineering for Si Heterojunction SolarCells; STW project number 12167).
Contents
1 Introduction 7
2 The physics of solar cells: semiconductor physics enhanced bythermodynamics 23
2.1 The theory of nonequilibrium thermodynamics . . . . . . . . . 27
2.1.1 Literature discussion . . . . . . . . . . . . . . . . . . . . 29
2.2 Overview of NETPV . . . . . . . . . . . . . . . . . . . . . . . . 29
2.3 The thermodynamic formulation of solar cellphysics step 1: Equilibrium and thermodynamic variables . . . 31
2.3.1 Entropy . . . . . . . . . . . . . . . . . . . . . . . . . . . 40
2.3.2 Generalisation to nonequilibrium . . . . . . . . . . . . . 43
2.4 The thermodynamic formulation of solar cellphysics step 2: Interaction with the environment . . . . . . . . 47
2.5 The thermodynamic formulation of solar cellphysics step 3: Continuity equations . . . . . . . . . . . . . . . 50
2.5.1 The entropy source term qs . . . . . . . . . . . . . . . . 53
2.5.2 Loss processes in the bulk of a solar cell and the entropygeneration rate . . . . . . . . . . . . . . . . . . . . . . . 54
2.6 The thermodynamic formulation of solar cellphysics step 4: Onsager theory . . . . . . . . . . . . . . . . . . 57
2.7 The thermodynamic formulation of solar cellphysics step 5: Symmetry, the Onsager reciprocal relations andthe Curie principle . . . . . . . . . . . . . . . . . . . . . . . . . 64
2.7.1 The Onsager reciprocal relations . . . . . . . . . . . . . 64
2.7.2 The Curie principle . . . . . . . . . . . . . . . . . . . . 65
2.8 Wrap up: what does thermodynamics tell us? . . . . . . . . . . 71
3 The physics of solar cells: semiconductor physics enhanced bythermodynamics 77
3.1 The thermodynamics of the selective membrane model . . . . . 77
3.2 The selective membrane model . . . . . . . . . . . . . . . . . . 78
3.2.1 What is selectivity? . . . . . . . . . . . . . . . . . . . . 89
4
3.3 The selectivity of Schottkytype junctions . . . . . . . . . . . . 92
3.4 The selectivity of homojunctions . . . . . . . . . . . . . . . . . 97
3.5 The selectivity of heterojunctions . . . . . . . . . . . . . . . . . 99
3.6 Generation and recombination in selective membranes . . . . . 105
3.7 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 109
4 Variational method for the minimisation of entropy generationin solar cells 115
4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 115
4.2 Entropy production in solar cells . . . . . . . . . . . . . . . . . 117
4.3 Variational solar cell optimisation . . . . . . . . . . . . . . . . . 123
Appendices 127
4.A Boundary conditions for the VEGM method . . . . . . . . . . . 127
5 Metaloxidebased holeselective tunnelling contacts for crystalline silicon solar cells 133
5.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 133
5.2 Materials and methods . . . . . . . . . . . . . . . . . . . . . . . 135
5.3 Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 138
5.3.1 The ZnO/Al2O3/cSi system as a selective contact . . . 138
5.3.2 Modeling of the tunnelling currents . . . . . . . . . . . . 138
5.3.3 Considerations for improving the contact resistance andsurface passivation . . . . . . . . . . . . . . . . . . . . . 140
5.4 Results and discussion . . . . . . . . . . . . . . . . . . . . . . . 143
5.4.1 Passivation of cSi by Al2O3/ZnO stacks . . . . . . . . . 143
5.4.2 Charge transport through Al2O3/ZnO stacks . . . . . . 147
5.4.3 Improved cSi passivation by aSi:H/Al2O3/ZnO stacks 147
5.5 Conclusions and outlook . . . . . . . . . . . . . . . . . . . . . . 149
6 Properties of graphene and its potential applications in siliconsolar cells 155
6.1 The electrical and optical properties of graphene . . . . . . . . 156
6.1.1 The graphene dispersion relation and density of states . 156
6.1.2 Conduction and photon absorption in graphene . . . . . 162
6.2 Junctions of graphene and silicon . . . . . . . . . . . . . . . . . 170
6.2.1 Equilibrium conditions . . . . . . . . . . . . . . . . . . . 171
6.2.2 Nonequilibrium conditions . . . . . . . . . . . . . . . . 173
6.2.3 Graphene as a carrier selective contact . . . . . . . . . . 181
6.3 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 182
Appendices 185
6.A Approximate expressions for the graphene carrier densities . . . 185
5
A Mathematical formulation of the charge transport in solarcells 195A.1 The driftdiffusion equations . . . . . . . . . . . . . . . . . . . . 195A.2 The PoissonBoltzmann equation . . . . . . . . . . . . . . . . . 199
Summary 205
List of publications 207
Acknowledgements 208
CV 210
6
Chapter 1
Introduction
As the title of this thesis makes abundantly clear, this work is about the physicsof solar cells. Our choice for this title deserves some extra clarification, since thephysics of solar cells is a very broad and developed field and one would probablyexpect to find such a title on a student handbook instead of a PhD thesis.There already exist sophisticated software packages that have implementeddetailed physical and mathematical models and that are capable of predictingthe efficiencies of complex cell designs, so the physics of solar cells might appearto be a closed chapter for the most part; a finished work. Then why do wedevote a PhD thesis to it? Our short answer to that question is, bluntly, thatwe still need to understand solar cells better than we currently do. Naturally,when we talk about understanding solar cells, we talk about improving them1
since photovoltaics (PV) is not a purely academic subject that we study justfor the science of it. The question then rises what the role of physics is (orshould be) in the design of solar cells. The ideal we normally have of scienceand physics is that we study a subject to learn about it and then use thisknowledge improve what whatever it was that needed improvement. However,this ideal is not as straightforward to realise as we would often like and thestep from knowledge to improvement is not always trivial (as is often assumed,unfortunately). We can ask a computer to calculate the efficiency a certaincell design and we would get a very accurate answer, but what we would muchrather do is ask the computer to calculate a cell design that achieves, e.g., a26 % efficiency given certain practical constraints. The physics of solar cellsmay provide us with very accurate models, but in the end it seems that forsolar cell design we still need something else; something nebulous we usuallycall “ingenuity”, “art” or “deeper understanding” or something like that.
1The term “improvement” can mean many different things in this context. Indeed, thereis a very fruitful discussion to be had about what we mean by “improvement of solar cells”.For the purposes of this work, we will mostly be talking about cell efficiency since that givesus a clear physical and thermodynamical measure of performance. For the argument in thisparagraph, though, any other metric of performance can be substituted if necessary.
7
So let us try to analyse this limitation of current solar cell physics a bitfurther. The first thing to note is that physics in general is, in its roots, ascience based on an alternating loop of observation and prediction. A physicistobserves a system and based on his observations he makes predictions. Next,he tests his predictions by further observations. However, if we want to improvea solar cell, we are not primarily interested in continually making predictionsand then observing if the cell does indeed follow the mathematical model wemade of it. Instead, what we are effectively trying to achieve is to “force”a particular observation we are interested in: the cell that performs best (seeFigure 1.1). So while physics is very good at making good models of solar cells,that does not immediately mean that these models are immediately useful formaking good cells. One could say that the problem of solar cell design is aninverse problem (i.e, one is trying to improve the observation rather than themodel that makes the predictions) compared to ordinary empirical science.2
At the start of this research project in November 2011, we set out to gaina better understanding of the crystalline silicon (cSi) heterojunction solar cell(abbreviated as SHJ cell) in order to come up with other potentially interestingand costefficient ways to create a cell out of a wafer. At the time there wasstill some debate about the success of the heterojunction between hydrogenatedamorphous silicon (aSi:H) and cSi (see Figure 1.2), which was –and at thetime of writing still is– achieving unusually high open circuit voltages (VOC)for a silicon solar cell. Early 2012, De Wolf et al. of EPFL published a reviewof this type of solar cell [1] and from this paper it becomes clear that thesuccess of the aSi:H/cSi heterojunction was only partially understood. Thelow defect density of the aSi:H/cSi interface was mentioned as an importantcontributor to the high VOC, but it was clear that this alone cannot be thewhole story. De Wolf et al. write:
“Key to the success of SHJ devices is the separation of highly recombinationactive (ohmic) contacts from the crystalline surface by insertion of a passivating, semiconducting film with a wider bandgap [2]. For SHJ devices, ideally,charge trickles through this buffer layer sufficiently slowly to build up a highvoltage, but fast enough to avoid carriers recombining before being collected.The buffer layer may thus be considered as a semipermeable membrane forcarrier extraction [3].”
It is very significant to note that the authors here make no use of termslike “space charge region” (SCR), “drift current”, and “diffusion current” that
2Without getting to far ahead of ourselves, it is worth mentioning here that there is onebranch of physics that specialises in these kinds of optimisation (i.e., engineering) problems.We are talking, of course, about thermodynamics. There is perhaps a certain irony in the factthat the physical theory that deals with optimisation of energy conversion is also the one thatdoes not really care about microscopic details. Our first instinct as scientist to understandsomething is to take it apart, but are more details always the best way to get to a betterdevice?
8
Figure 1.1: The contrast between learning about solar cells and improving them. Bothdisciplines are rooted in experiment and observation, but for science the ultimate goal is toimprove the mathematical models of solar cells while engineering is concerned with improving the cell itself. Of course, the two are not mutually exclusive: engineering can lead tointeresting new questions science can investigate (top red arrow) while the scientific modelscan help to find new solutions to engineering problems (bottom red arrow).
9
Figure 1.2: Schematic layout of the aSi:H/cSi heterojunction cell as described by, e.g.,De Wolf et al. [1]. It is fabricated by depositing films of intrinsic aSi:H on both sidesof a texturised silicon wafer (usually ntype), followed by films of doped aSi:H of oppositepolarities on either side. Typically, the aSi:H films are have a combined thickness of around10 nm. These films form the electron and hole selective membranes that allow the differentcharge carriers to be extracted at opposite sides of the wafer. On top of the aSi:H films onethen deposits TCO (short for transparent conductive oxide) films that provide lowresistancecurrent pathways to the metal contacts. Commonly used TCOs include tindoped indiumoxide (ITO) and aluminiumdoped zinc oxide (ZnO:Al). SHJ cells of this simple planardesign have proven to be relatively easy to fabricate in only a few lowtemperature (< 200 C)processing steps while still achieving very respectable efficiencies; some of them rivalling theworld record such as Panasonic’s 750 mV SHJ cell from 2011 [4]. In fact, a modified version(also by Panasonic) of the SHJ cell holds the current world record for single junction cSicells [5]. What makes this record cell different, is that it has both the ntype and ptypedoped aSi:H films on the rear side of the cell in a configuration often called “interdigitatedback contacts” or IBC. The IBC SHJ solar cell design is a solution to the main drawback ofthe planar SHJ cell, namely its parasitic absorption. As it turns out (and as we will discussin greater depth later), the photons absorbed in the aSi:H films in the SHJ cell contributerelatively little to usable current. Thus, by putting the aSi:H films at the back of the cell inthe IBC design, the amount of absorption in the amorphous films in minimised so that it canprovide more current. The main disadvantage of the IBC SHJ cell is that it is significantlymore complex to design and fabricate.
10
are traditionally used to explain how homojunction solar cells work. Instead,they rely on the relatively new idea of semipermeable membranes, first coinedby Peter Wurfel. Reading his book Physics of Solar Cells made it clear thatWurfel has a very different view of solar cells than the one presented in mosttext books on semiconductor physics, even though Wurfel never really disputesthe validity of the equations those text books use. Wurfel demonstrates thatthere is more to the physics of solar cells than just the equations that describethem: there is also a bigger picture –an overall philosophy if you will– consistingof easily identifiable elements and a clear understanding of how they interact.
So while the equations of solar cell physics are mostly clear and cut, thebig picture view of solar cells is still developing. But what does that mean,exactly? How can such a framework improve? Needless to say, a general idealike Wurfel’s selective membrane model should not clash with the fundamentalsolar cell equations; otherwise it would be no more than a superstition ormisconception. This means that its predictive power (the usual metric by whichwe judge a physical theory) should not be different than that of the basic solarcell equations. It also means that we cannot choose between two competingpictures purely based on their predictive power: both should be physicallycorrect to begin with. Instead, if we have to choose between two such pictures,we should look at how much they simplify the process of improving solar cells.In other words, we are looking for a language that allows us to have meaningful,clear discussions about solar cells and that makes it easy to find design flawsin cells we want to improve. Thus, a good overall picture of solar cells is veryimportant to solve the inverse problem of solar cell design mentioned earlier.
In the summer of 2012 the author of this thesis was lucky enough to meetWurfel in person and have some discussions with him. It became apparentthat, at the time, he was not very optimistic about the general acceptance ofhis ideas. Three years later, we think that his reservations are, fortunately,unwarranted: during the many discussions with different researchers in (aswell as outside of) the field, we noticed that the semipermeable membranemodel has a universal appeal due to its intuitive simplicity and most peoplewe introduced it to were quick to adopt it. In fact, we have heard peopleadmit more than once that they never felt like they really understood muchabout solar cells before we introduced them to Wurfel’s ideas. In our ownexperience, it is a very powerful way of thinking about solar cells that makesthe discussions about solar cell design much more transparent and less naivecompared to what we had before (see Figure 1.3). Still, even though theselective membrane model is steadily gaining ground, the old solar cell picture(left in Figure 1.3) is still commonly found in literature, especially in articlesfrom authors that originate from other fields (such as graphene processing, seee.g., [6, 7]) that pay a short visit to the world of PV. Even in the field of siliconPV there are still authors who, e.g., attribute the success of the SHJ cell to–in our opinion quite erroneously– the inversion layer in the cSi [8]. In fact,
11
the reader will see in Chapter 5 (which is a paper we wrote in 2013) that wehad some trouble in the past as well to completely shed our old conceptions ofsolar cells and adopt the selective membrane model.
Wurfel’s ideas raise new and interesting questions that need to be answered.What exactly is a semipermeable membrane in the context of solar cells andhow do you make one? What makes it effective? Apparently the bandgap ofsuch a membrane is important (see the quote of De Wolf et al.); why? And isthat the only thing that matters? What makes the semipermeable membranemodel a useful way to look at solar cells and how does it follow from the basicunderlying physics? Questions like these we have tried to address over thelast four years and in this thesis we hope to answer them to the reader. Asalways turns out to be the case, simple ideas can become pretty complicatedwhen you examine them closely, so it is important to guard against pitfalls andoversimplification.
If rules of thumb and heuristic explanations are not investigated and theirlimitations explained, the risk exists that they become rigid laws in the mindsof researchers that steer them away from potentially interesting directions ofthinking. Take, for example, the often used rule that the VOC of a singlejunction cell cannot be larger than the bandgap of the semiconductor. Thisrule is often taken for granted, but what does it mean, exactly? For one, whatdo we exactly mean by “the bandgap”: the optical or the electrical bandgap?Looking at Figure 1.4 it seems that the electrical bandgap is rather immaterialto the question, even though that is the number most people have in mind.Indeed, it has already been pointed out by Yablonovitch [9] (among others)that a very effective cell should have a dense internal photon field, just in thesituation shown in the figure. The next (rather difficult) question is then whatthe exact limitations are when it comes to confining the internal photons byenergyselective mirrors; a question that would remain unasked if one wouldnot venture to take a close look at the rule that the VOC cannot be larger thanthe bandgap. Unfortunately, for cSi based cells the possibility of achieving aVOC larger than 1.124 V can be ruled out because Auger recombination willalways dominate over radiative recombination in silicon3 [10]. Still, Figure1.4 demonstrates why it is important to take a hard, critical look at broadideas about the way solar cells work; the selective membrane model is noexception and in Chapter 3 we will take a closer look at it. In that sectionwe demonstrate that the selective membrane model is indeed a useful way ofthinking about solar cells. The main reason for this is that the functions ofthe selective membranes and the photon absorber in the cell are so dissimilarthat they require very different material properties to be effective at theirjob. Because of this complementarity of functions, it makes sense to mentally
3This is also the reason that the photonic design principles of solar cells will not be treatedin great depth in this thesis, since the main focus is on cSi based cells. In Sections 2.4 and2.5 we will briefly deal with this issue in broad terms.
12
Figure 1.3: Two competing pictures of solar cell junctions. The left picture is a rathernaive visualisation of the operation of a solar cell for several reasons. First of all, it putsgreat emphasis on the buildin voltage Vbi and the space charge region (SCR) and the forcesthe electric field exert on the carriers. However, the electrostatic force is only part of thetotal (thermodynamic) force that the carriers experience. Drawing an electron that falls ofa electrostatic potential hill makes sense if that electron exists in a vacuum between twoplates of a capacitor, but not in a solar cell where the motion of a single electron is bothunpredictable and unimportant. Moreover, the left picture leaves the incorrect impressionthat the electric field drives the current, but an electric field cannot perform net work sinceit is a conservative force. The left picture also depicts the thermalisation of the energy of anelectronhole pair after excitation. This is also slightly naive, since the (total) energy of anelectronhole pair is, thermodynamically speaking, rather inconsequential: the total energy isnot necessarily the amount of energy one can convert into work. In fact, the diagram shownon the left is in equilibrium; in this situation none of the energy of the excited pair can beextracted as work in the same way one cannot extract thermal energy from a silicon waferand use that to power a machine. The right picture (Wurfels’) is a thermodynamically lessnaive presentation of a solar cell and it puts the emphasis on the quasi Fermi levels EFn,pthat represent the free energy of the ensembles of electrons and holes. This also means thatthe red and blue dots do not represent individual electrons and holes: they represent theaverage of a large number of particles. These averaged particles do not feel electrostaticforces (the gradients of EC,V) but electrochemical forces (the gradients of EFn,p). BecauseEFn and EFp come together in the metal, there will always be electrons flowing towards theholecollecting contact and the only way to do something about that is by making sure thatthe electrons encounter much more resistance (represented by rectangular resistor symbols)than the holes on their way from the bulk to the contact. This asymmetry between electronand hole resistance is what we call selectivity. Note that the SCR in this picture suddenlybecomes rather unimportant: as it turns out, the SCR contributes only a little to selectivityof the membrane (see Section 3.3). The free energy also allows us to provide a new, moreinsightful, view of thermalisation losses associated with photon absorption, because the freeenergy is the maximum energy one can hope to extract as useful work from the system.For example, by considering free energy thermalisation rather than energy thermalisation itsuddenly becomes obvious why photon absorption in selective membranes is less effective thanin the bulk of the cell: in the membranes the Fermi level splitting is less and the free energythermalisation losses are larger. In practise, these thermalisation losses manifest themselvesas parasitic absorption; a wellknown problem in aSi:Hbased SHJ cells [1].
13
divide the cell into these different parts and understand how they work andinteract. Furthermore, this complementarity also immediately makes it clearthat heterojunction cells provide the design flexibility we need to push the cellefficiency to its limit.
Halfway through 2012 we started playing around with ideas for making newheterojunction concepts based on Wurfel’s selective membrane model. Ourresearch group has had significant success in the past with the material Al2O3,which is a surprisingly good passivation layer for silicon [11]. Passivation (thelast word in the title of this thesis that has gone unmentioned so far) is thepractise of making the surface of a silicon wafer (where it is not contacted bymetal leads) less recombination active. This is important, because ordinarilysurfaces are very defective and poorly passivated surfaces will cause significantlosses in a cell. The reason that aluminium oxide is a good passivation layer isbecause of the low defect density of the Al2O3/cSi interface and because of thenegative fixed charge in this interface that generates a hole inversion layer at thecSi surface [12]. Under the motto “If you have a good hammer, why not lookfor some more nails to hit?”, we started to think if it would be possible to extendthe application of Al2O3 to selective membranes. In Chapter 5 the results of thisresearch are described. One of our conclusions at the time was that one on handwe need a thin (∼1 nm) film of Al2O3 to make it possible for the holes to tunnelthrough the oxide into the ZnO (which we used as a transparent conductor),but on the other hand that very thin oxide films also lead to large recombinationlosses and low carrier lifetimes. This result should have tipped us off that thecontact we were trying to make is actually not selective enough. Indeed, wewere trying to make a holeselective membrane by creating a hole inversionlayer in the cSi and we now know (see Section 3.3) that such an inversionlayer simply cannot provide enough selectivity to make a good cell; an insightthat we simply did not have at the time4. The Al2O3 itself, unfortunately, doesnot provide holeselectivity either5. At the time we were still a bit stuck inthe past in that regard and we focussed a lot on passivation (interface defectreduction) and on the hole inversion layer (i.e., the SCR). Of course, passivationis very important when it comes to making selective heterojunction membranes:precisely because the inversion layer cannot provide selectivity, the defects atthe cSi interface need to be reduced as much as possible or you lose yourcarriers before the selective membrane even gets to do something (see alsoSection 3.6). So in this thesis when we are talking about using heterojunctionsto make a selective contacts, we really mean passivating selective contacts.However, when it comes to making selective contacts, passivation is only thefirst step: between the passivated cSi interface and the metal there needs
4In fact, much of the work in Chapter 3 is motivated precisely by our initial inability toget a better understanding of the results from the Al2O3/ZnO experiments.
5If anything, quite the opposite: looking at the tunnelling barriers in Figure 5.2, the Al2O3
itself should be electron selective
14
Figure 1.4: Is it possible to make a cell with a higher voltage than its bandgap? (Counterclockwise from the topleft.) 1: If enough carriers are injected into the semiconductor,both the electrons and holes become degenerate. The optical bandgap EG,opt (the minimalphoton energy that can be absorbed by the semiconductor) widens and becomes equal to theFermi level splitting instead of the electrical bandgap EG,el. 2: Photons are then emittedby radiative recombination in the energy range between EG,el and EG,opt. 3: The emittedphotons will deexcite nearby electrons due to stimulated emission, generating even morephotons and causing rapid loss of electronhole pairs. 4: To avoid this avalanche reaction, itis necessary to confine the photons in the [EG,el, EG,opt] range by selective mirrors so thatinternal equilibrium between the photons and e−–h+ plasma can form, just like in a semiconductor laser. In this case we clearly have VOC < EG,opt, since the VOC is the maximumpossible Fermi level splitting. However, it seems likely that VOC > EG,el is possible if thephotons inside of the cell can be confined well enough by the mirrors. Interestingly, in thissituation the free energy thermalisation losses in the cell are significantly lower than if theelectronhole pairs were nondegenerate.
15
to be some sort of layer that provides a source of selectivity, otherwise toomany minority carriers will end up in the wrong metal contact, which is just asbad as interface recombination. Sometimes the term passivating contacts (orpassivated contacts) can also be heard in the solar cell world, but we think thatthis term gives the wrong impression that it is somehow possible to passivatea metal; to make it less recombination active. This is simply not the case: allyou can really do is make it as difficult as possible for one type of carrier toreach the metal in the first place.
We then tried to salvage the situation by inserting a little bit of aSi:Hbetween the cSi and Al2O3, even though this was the material we initially setout to avoid. The unfortunate thing about aSi:H is that it is a strong photonabsorber, which is something you do not want out of a selective membrane sinceit leads to parasitic absorption (see Figure 1.3, Section 3.5, and also De Wolf etal. [1]). As expected, the aSi:H improved the measured carrier lifetimes. Atthe time we attributed this effect mainly to a reduction of the defect densityat the cSi/aSi:H interface (compared to the original Al2O3/cSi interface),but the interface defects are probably only part of the story. Looking back atthe data in Chapter 5 with the insights we have gained since then, we nowthink it is very likely that the main reason for the improved carrier lifetimesshould be attributed to a significant increase in the resistance the electronsexperience on their way to the contact (for which we used ZnO). In a sense,the fixed charges in the Al2O3 act as a sort of induced ptype doping in theaSi:H. So while the induced SCR in the cSi only has a very low selectivity,the SCR induced in the aSi:H actually is resistive enough to make a goodselective contact. However, we also found that the holeselective contacts wefabricated with these materials (ZnO, aSi:H and Al2O3) were too resistivefor holes. Here, we think that the original conclusions from Chapter 5 stillstand and that the main problem is the choice of ZnO as a TCO (transparentconductive oxide), which simply does not have a large enough electron affinityto efficiently collect holes (as demonstrated by modeling the contact like anEsaki diode; see Figure 5.2 and Figure 5.3). Ultimately, the idea behind theTCO/aSi:H/Al2O3 stacks is still sound enough to warrant further investigationof this concept and those related to it (such as the successful MoOxbased holecontacts by Battaglia et al. [13, 14]). The attractive feature of these concepts isthat they use a thin, transparent metal oxide layer to replace the doped aSi:Hin traditional SHJ cells so that only the intrinsic aSi:H is needed. So while theproblem of parasitic absorption cannot be completely solved by fixedchargedielectrics such as Al2O3, at least they provide feasible alternatives to dopedaSi:H without having to discard the good qualities of intrinsic aSi:H.
Graphene is another material that caught our attention as potentially interesting for the fabrication of selective membranes. Of course, graphene isa very unique material with remarkable properties matched by a remarkablehype to go with it. It should not come as a surprise that many researchers
16
have already made solar cells by putting graphene on a silicon wafer –just tosee what happens– but so far this field has been explored mainly by expertsof graphene and not so much by solar cell experts. We therefore thought itwas a good idea to review this very active field from our own perspective tosee if graphene can indeed live up to the hype when it comes to PV. This isthe subject of Chapter 6, where we tried to give an overview of the physics ofgraphene that are relevant for a solar cell researcher to make the entry intothis field a little simpler. Furthermore, these physics are then used to see ifthe electrical properties of graphene are indeed remarkable enough to makea relevant contribution to the toolbox of the silicon solar cell designer. As itturns out, the answer to this question is a tentative “yes”. For one, the conductance of a single sheet of graphene can, in principle, be high enough to actas a transparent electrode for a cSi solar cell. However, this high conductanceis far from straightforward to achieve since the 2D material is rather sensitiveto its surroundings and its substrate. As a selective contact is shows morepotential since it seems to behave like a metal with a tunable work functionand an extremely low (for metal standards) effective Richardson constant. Infact, the Richardson constant of graphene could potentially be so low that thegraphene/silicon Schottky junction could be the exception to the old rule ofthumb that Schottky junctions cannot make good solar cells. Unfortunately,the literature data so far cannot prove for certain that this is actually possible and more focussed experiments are necessary to confirm this hypothesis.Additionally, graphene is known to be a material that is difficult to dope (andgood doping control is definitely necessary for PV applications) and difficult toprocess, so graphene is certainly not a material that will just solve any problemwithout creating new ones as the hype might sometimes lead you to believe.Still, it is not unlikely that at some point it will earn its place in the field ofPV.
Parallel to the selective membrane model we also developed a thermodynamical view of solar cells in this thesis. Indeed, Wurfel’s book is also ratherexplicit about the importance of thermodynamics when it comes to understanding solar cells and in a sense this is a natural thing to do since thermodynamicsis the natural language of energy conversion. The mere idea to view a solar cellas a thermodynamic energy converter that turns heat from the sun into workis already a valuable concept to broaden the discussion about what solar cellsare (and are not) capable of. It may seem like a trivial idea, but many fellowphysicists we have spoken to (especially those not directly involved with PV)were surprised at first when presented with the idea of applying thermodynamics to solar cells6. There seems to be a sort of implicit consensus that electricaldevices are not really in the realm of thermodynamics for some reason. Some
6Even though it is actually not a new idea at all; it can already be found the famousShockleyQueisser paper [15] and in earlier works cited by that paper
17
physicists also seem to have an aversion to the thought that sunlight is a formof heat because it does not come in the form of thermal vibrations7.
So if a thermodynamic treatment of solar cells is not new, what is our motivation for presenting one? The thing about thermodynamics is that there aredifferent ways to approach the subject depending on the a priori assumptionsyou make about your system. Our goal is to make thermodynamics accessibleto solar cell researchers and that means we want to stay relatively close to thesemiconductor physics they are (hopefully) already familiar with. We do this todemonstrate that the thermodynamics of solar cells is more than just academicdiscussions about the upper efficiency limit of hypothetical devices: the scienceof thermodynamics is, from its very roots, an engineering toolbox8. Yet in thesolar cell community it is not usually recognised as such and we think thatthis is because the languages of thermodynamics and semiconductor physicshave been rather distinct. That is not to say that it is all bad: the efforts ofWurfel and other authors have already helped to spread some thermodynamicideas in the PV community, such as the view that the quasi Fermi levels represent the free energy (i.e., the energy one can hope to extract as useful work)of electrons and holes. However, there are still open ends and many works(including Wurfel’s) rely on traditional equilibrium thermodynamics and thenmake a sudden leap to the nonequilibrium problem of describing a workingsolar cell without really motivating how such a leap can be made.
In our opinion, the missing link between thermodynamics and semiconductor physics is the book Nonequilibrium Thermodynamics by De Groot andMazur [16]. In its own field, it is a wellknown work that is known for beingthorough yet rather dense. When cast in the right form, the theory of DeGroot and Mazur can produce the thermodynamic equivalent of semiconductor physics without much trouble, as we will show in Chapter 2. In the end,this means that one does not have to learn many new things to discuss solarcells thermodynamically: semiconductor physics actually were a form of nonequilibrium thermodynamics all along. By recognising this equivalence, wesuddenly gain access to all kinds of thermodynamical tools that were hiddenbefore, such as the entropy generation rate that tells us where in the cell (and
7To be fair, there are some peculiarities about photons that cannot be glossed over. Whatmakes photons strange is that they cannot interact with each other: if you throw a bunchof light particles together, they will not equilibrate because they cannot interact. However,they can equilibrate with a dense collection of charged particles, such as the plasma of thesun’s surface. Thus, in the sun the photons can reach equilibrium with the photosphere andbecause of the zeroth law of thermodynamics this also means that they are in equilibriumwith each other, even though they do not feel each other. Then they are send off to earth andmaintain that equilibrium until they interact with the solar cell (ignoring the atmosphere).Thus, the interaction of sunlight with a solar cell can be viewed as a form of heat transferfrom the photosphere to that cell.
8After all, Carnot was an engineer who was very much interested in solving practicalproblems.
18
how much) potential output power is being wasted.Then in Chapter 4 we will use the derived expression of the entropy gener
ation rate to set up a mathematical model called VEGM (variational entropygeneration minimisation) that can predict efficient cell designs. VEGM is, inprinciple, the mathematical answer to the inverse problem that was posed atthe start of this chapter: how can you make a computer spit out the most efficient cell for a given set of practical constraints? The reader may notice thatChapter 4 does not actually contain a computer calculation that implementsthe VEGM model. This is not for lack of trying, but it turned out that thedifferential algebraic equations produced by VEGM are not straightforward toimplement into an existing solver (we tried COMSOL Multiphysics®, but raninto convergence issues) and at the moment we are of the opinion that thisimplementation requires dedicated effort from an expert on numerical computation.
To conclude this introduction, we would like to present a brief helicopterview of the content in the next chapters in Figure 1.5. The central theme ofthis dissertation is the optimisation problem of solar cells we introduced in thefirst two paragraphs of this chapter: how do you “invert” the known solar cellphysics so that you can predict which cell is the most efficient? This questionis approached from two different angles, namely that of the selective membranemodel and that of thermodynamics. The thermodynamics provide the physicalfoundation necessary to quantitatively understand the loss mechanisms in solarcells while the selective membrane model provides a qualitative language thathelps to get a better intuitive grasp of the overall design of a cell as well as thestrengths and weaknesses of its components.
We hope that between these two complementary angles the reader findsnew insights that will help him or her come up with fruitful new ideas abouthow to improve the cell he or she is working on. Of course, if you are left withany questions, you are kindly invited to contact the author. You are kindlyreferred to the contact details in the CV on page 210.
19
Figure 1.5: Overview of the themes in this thesis and the contents of the chapters.
20
References Chapter 1
[1] Stefaan De Wolf, Antoine Descoeudres, Zachary C. Holman, andChristophe Ballif. Highefficiency Silicon Heterojunction Solar Cells:A Review. green, 2(1):7–24, January 2012. ISSN 1869876X. doi:10.1515/green20110018.
[2] E. Yablonovitch, T. Gmitter, R. M. Swanson, and Y. H. Kwark. A720 mV open circuit voltage SiOx:cSi:SiOx double heterostructure solar cell. Applied Physics Letters, 47(11):1211, 1985. ISSN 00036951. doi:10.1063/1.96331.
[3] Peter Wurfel. Physics of Solar Cells. WileyVCH Verlag GmbH & Co,Weinheim, 2005. ISBN 3527404287.
[4] Martin A Green, Keith Emery, Yoshihiro Hishikawa, Wilhelm Warta, andEwan D Dunlop. Solar cell efficiency tables (version 43). Progress in Photovoltaics: Research and Applications, 22(1):1–9, jan 2014. ISSN 10627995.doi: 10.1002/pip.2452.
[5] Martin A. Green, Keith Emery, Yoshihiro Hishikawa, Wilhelm Warta,and Ewan D. Dunlop. Solar cell efficiency tables (version 46). Progress inPhotovoltaics: Research and Applications, 23(7):805–812, jul 2015. ISSN10627995. doi: 10.1002/pip.2637.
[6] Yu Ye and Lun Dai. Graphenebased Schottky junction solar cells. Journal of Materials Chemistry, 22(46):24224, 2012. ISSN 09599428. doi:10.1039/c2jm33809b.
[7] Xinming Li, Hongwei Zhu, Kunlin Wang, Anyuan Cao, Jinquan Wei,Chunyan Li, Yi Jia, Zhen Li, Xiao Li, and Dehai Wu. GrapheneonsiliconSchottky junction solar cells. Advanced materials (Deerfield Beach, Fla.),22(25):2743–8, July 2010. ISSN 15214095. doi: 10.1002/adma.200904383.
[8] J. Poortmans M. Ghannam, G. Shehadah, Y. Abdulraheem. Basic Understanding of the Role of the Interfacial Inversion Layer in the Operationof Silicon Solar Cells with aSi/cSi Heterojunction (HIT). In 28th EU
21
PVSEC Proceedings, page 822, 2013. doi: 10.4229/28thEUPVSEC20132BO.2.6.
[9] Eli Yablonovitch and Owen D. Miller. The OptoElectronics of Solar Cells.IEEE Photonics Society News, 27(1), 2013.
[10] Armin Richter, Martin Hermle, and Stefan W. Glunz. Reassessment ofthe Limiting Efficiency for Crystalline Silicon Solar Cells. IEEE J. Photovolt., 3(4):1184–1191, oct 2013. ISSN 21563381. doi: 10.1109/JPHOTOV.2013.2270351.
[11] G. Dingemans and W. M. M. Kessels. Status and prospects of Al2O3basedsurface passivation schemes for silicon solar cells. Journal of Vacuum Science & Technology A: Vacuum, Surfaces, and Films, 30(4):040802, 2012.ISSN 07342101. doi: 10.1116/1.4728205.
[12] Bram Hoex, S. B. S. Heil, E. Langereis, M. C. M. van de Sanden, andW. M. M. Kessels. Ultralow surface recombination of cSi substrates passivated by plasmaassisted atomic layer deposited Al2O3. Applied PhysicsLetters, 89(4):042112, 2006. ISSN 00036951. doi: 10.1063/1.2240736.
[13] Corsin Battaglia, Xingtian Yin, Maxwell Zheng, Ian D Sharp, TeresaChen, Stephen McDonnell, Angelica Azcatl, Carlo Carraro, Biwu Ma,Roya Maboudian, Robert M Wallace, and Ali Javey. Hole Selective MoOx
Contact for Silicon Solar Cells. Nano Letters, 14(2):967–971, feb 2014.ISSN 15306984. doi: 10.1021/nl404389u.
[14] Corsin Battaglia, Silvia Martın de Nicolas, Stefaan De Wolf, XingtianYin, Maxwell Zheng, Christophe Ballif, and Ali Javey. Silicon heterojunction solar cell with passivated hole selective MoOx contact. Applied Physics Letters, 104(11):113902, mar 2014. ISSN 00036951. doi:10.1063/1.4868880.
[15] William Shockley and Hans J. Queisser. Detailed Balance Limit of Efficiency of pn Junction Solar Cells. J. Appl. Phys., 32(3):510, 1961. ISSN00218979. doi: 10.1063/1.1736034.
[16] S.R. de Groot and Peter Mazur. Nonequilibrium Thermodynamics. DoverPublications, Mineola, New York, 1984. ISBN 0486647412.
22
Chapter 2
The physics of solar cells:semiconductor physicsenhanced by thermodynamics
23
Symbols used in Chapter 2 and Chapter 3
Sym. Definition
Ai General thermodynamicvariable when U is used asthe potential. E.g., S, V .i = 1, ..., l.
B Magnetic field (T).Bi General thermodynamic
variable when S is used asthe potential. i = 1, ..., l.
Dn,p Electron/hole diffusion coefficient (cm2 s−1).
e Elementary charge (C).EC Conduction band energy
level EC = −φ− χ (eV).EF Equilibrium Fermi level
(eV).E Electric field (V cm−1).EFn,p Quasi Fermi energies for
electrons/holes (eV).EG Semiconductor bandgap
(eV).EV Valence band energy level:
EV = −φ− χ− EG, (eV).fi Conjugate variable to Ai
when U is the potential:fi = ∂U/∂Ai, i = 1, ..., l.
Fi Thermodynamic force. i ∈U, S,Q, n, p.
F1/2 FermiDirac integral.
F←1/2 Inverse of the FermiDiracintegral.
FF Fill factor.gi Conjugate variable to Bi
when S is the potential:gi = ∂S/∂Bi, i = 1, ..., l.
Sym. Definition
G Generation rate of electronhole pairs (cm−3 s−1).
Gnet Net generation rate ofelectronhole pairs G − R(cm−3 s−1).
Ji Thermodynamic current (orflow) of quantity i. i ∈U, S,Q, n, p. The particle currents Jn,p are incm−2 s−1.
Jn,p 1D electron/hole particleflux (cm−2 s−1).
JSC Short circuit current density((A cm−2)).
kB Boltzmann constant(J K−1).
Lij Scalar transport coefficientthat relate force Fj to fluxJi.
Lij Second order tensor transport coefficient that relateforce Fj to flux Ji.
n Electrons density (cm−3).ni Intrinsic carrier
density: n2i =
NCNV exp(−EG/kBT )(cm−3).
neh Density of electronholepairs (cm−3).
NC,V Conduction/valence bandeffective density of states(cm−3).
24
Sym. Definition
Nn,p Total number of electrons/holes (dimensionless).
Ndop Semiconductor doping density (cm−3).
Neh Total number of electronhole pairs (dimensionless).
p Hole density (cm−3).P Pressure (N cm−2).qi Source term in continuity
equation for quantity i. i ∈U, S, n, p.
Q Heat (J).Qnp Total electronhole charge
divided by e (cm−3).R Recombination rate
of electronhole pairs(cm−3 s−1).
RRad Radiative recombinationrate of electronhole pairs(cm−3 s−1).
R Pseudo resistance(C Ω cm2).
R Intrinsic resistance(C Ω cm2).
s Volumetric entropy density(J K−1 cm−3).
S Entropy (J K−1).
S Pseudo conductance(S cm−2 C−1).
S Intrinsic conductance(S cm−2 C−1).
t Time (s).T Temperature (K).u Volumetric internal energy
density (J cm−3).
Sym. Definition
U Internal energy (J).V Volume (cm3).VOC Open circuit voltage (V).VT Thermal voltage = kBT/e
(V).x Position coordinate (cm);
can be 1, 2, or 3 dimensional.
β Inverse temperature 1/T(K−1).
γ Index that indicates that asymbol pertains to photons.
δ Variational differential.E.g., when f(x) is a function of position, δf(x)represents a small deviationof that function.
∆ηeh Fermi level splitting orelectrochemical potentialper electronhole pair(eV). ∆ηeh = ηn + ηp =EFn − EFp.
∆n Injection level; excess carrier density (cm−3).
ε Dielectric constant εrε0(F cm−1).
ηn,p Electron/hole electrochemical potential (eV). ηn =EFn, ηp = −EFp.
ηn,p βηn,p.∆ηeh β∆ηeh.ηPC Photovoltaic conversion ef
ficiency, PCE (dimensionless).
25
Sym. Definition
µn,p Electron/hole mobility(cm2 V−1 s−1).
µcn,p Electron/hole chemical po
tential (eV).νn,p Selectivity of an elec
tron/hole selective membrane (dimensionless).
ρnet electronhole charge densitydivided by e (cm−3).
σirr Total entropy generation rate per unit volume(J K−1 s−1 cm−3).
Σirr Total entropy generationrate (J K−1 s−1).
σn,p Electron/hole conductivity(S cm−1).
ΦQ Conjugate variable of Qnpwhen U is the potential:ΦQ = ∂U/∂Qnp (J).
ΦQ Conjugate variable of Qnpwhen S is the potential:ΦQ = ∂S/∂Qnp (J).
φ Electrostatic energy (eV).χ Electron affinity (eV).
26
2.1 The theory of nonequilibrium thermodynamics
The description of solar cells is usually framed in the language of semiconductorphysics (SCP) because many photovoltaic devices rely on the unique properties of semiconductors to work. The literature on SCP has accumulated a largewealth of detailed models (such as recombination and mobility models) thatcan be used to accurately predict the efficiencies of industrial device designs.Paradoxically, this level of detail can also be detrimental to the global understanding of the device because only a computer can work out the complex SCPmodels so that it quickly becomes unclear which details are the most importantand what parts of the device need to be addressed to yield the largest gainsin efficiency. Indeed, for a long time there have been misconceptions in thePV field about the general principles of photovoltaic energy conversion suchas the idea that the electric field in the space charge region of a junction isresponsible for driving the photocurrent [1, 2].
An alternative way to look at solar cells is by considering it as a thermodynamic system. The motivation for this viewpoint is that, unlike mostsemiconductor devices, a solar cell is first and foremost an energy convertorand the natural language of energy conversion are thermodynamics. Specifically, since a solar cell is always operating under nonequilibrium1 conditions,it should be described by nonequilibrium thermodynamics (NET) rather thanequilibrium thermodynamics (ET). The advantage of thermodynamics is thatit provides methods to characterise losses of free energy (i.e., useful outputpower). In literature many different thermodynamic descriptions of solar cellphysics can be found [4, 5, 6, 7, 8, 9, 1, 10, 11] and addition, several workshave presented thermodynamic frameworks for SCP in general [12, 13, 14, 15]without specific application to PV. Yet despite these efforts, the SCP view ofsolar cells is still by far more common than the thermodynamic view, especiallyin engineering domain of cSi based cells. About the reasons for this differenceone can hypothesise:
The PV community simply does not see the value of an alternative modelas long as SCP does a good job of predicting cell efficiencies.
Thermodynamics is thought of as a subject that is mainly useful foracademic discussions about the maximum possible efficiency of highlyhypothetical devices under idealised circumstances. Indeed, many existing works on solar cell thermodynamics focus on a very broad descriptionof the device rather than on the detailed engineering that is necessary toimprove the efficiency of practical designs.
NET is a relatively new field that is still developing and thus has not fully
1There seems to be no general consensus about the spellings “nonequilibrium” vs.“nonequilibrium”. In this work the spelling by De Groot and Mazur [3] will be followed.
27
crystallised yet. This is in stark contrast to the SCP description of solarcells, which has been solidified into a uniform shape. As was mentioned,different formulations of solar cell thermodynamics exist and potentiallythis gives the impression that there are no established methods yet onecan safely rely on.
The PV community is simply not aware enough of the progress in thearea of thermodynamics to appreciate the value of the many tools thathave become available throughout the last few decades.
A combination of some or all of these factors.
Under scrutiny, these objections do not hold up. Van Vliet [12], Lindefelt [14], and Parrot [15] already demonstrated that SCP can quite readily beincorporated into NET as a specialised area. Furthermore, the use of thermodynamics is very common in other engineering disciplines (chemistry beingthe prime example), so the question rises why this should be different for solarcells. The main goal of this chapter is to build up a comprehensive treatmentof NET applied to solar cell physics that will be referred to as NETPV. Theend product of this treatment is a theory that combines the strengths of SCP(i.e., detailed models for the engineering of practical solar cell designs) and ofNET (i.e., generality and a clear interpretation of free energy losses).
In NETPV, certain assumptions relevant to PV will be made from the startto allow for simplifications and to avoid unnecessary abstraction. The commongrounds between NETPV and SCP will be made as clear as possible by choosingnotation familiar from SCP, especially in Chapter 3. Where necessary, it willbe stated how NETPV interprets or describes physical phenomena differentlycompared to SCP. Special attention will be drawn to cases where NETPV
potentially extends SCP or even disagrees with it.
To give a firm foundation for NETPV, the book “Nonequilibrium Thermodynamics” by De Groot and Mazur (abbreviated as GM) [3] is used as thestarting point. This work, first published in 1962 and republished in 1984, iswidely considered to be a standard work in its field and is commonly referencedby more modern works [16, 17, 18]. Their theory for the description of nonequilibrium systems (abbreviated as NETGM) is very well equipped to describethe energy conversion processes in solar cells. One of the main goals of thischapter is to present an accessible and comprehensive application of NETGM
to solar cells, since the book by GM is known to be rather dense. It should benoted, though, that the thermodynamic description of solar cells requires someunique considerations related to the interaction between the device and thesunlight. These subtleties are not treated in the sources mentioned above anddeserve some extra attention. The main references for the thermodynamics oflight are the works by Wurfel [8, 1] and Landsberg [19].
28
It is assumed that the reader of this thesis is familiar with the basics ofthe SCP description of solar cells, but for clarity a brief summary is given inAppendix A.1.
2.1.1 Literature discussion
Perhaps surprisingly, it seems that most authors in the field of cSi PV (eventhose that have given thermodynamic descriptions of solar cells) are unawareof the work on nonequilibrium thermodynamics by GM, even though some(but certainly not all) of its methods have found their way into the field of PVindirectly. Unfortunately, the book by GM is not indexed in major publicationdatabases, making it difficult to determine precisely how influential it is invarious fields of research or in the field of PV in particular. All that can besaid for sure is that none of the work by GM can be found in the 2generationbackward citation maps of the works by Brendel [10], Greulich [11], Harder [9],P. Wurfel [8], and U. Wurfel [2].
The closest link between the PV literature and the work by GM seems tobe the work of J.E. Parrot, who refers to GM in his work “Thermodynamictheory of transport processes in semiconductors” [15]. However, in his earlierworks on solar cell thermodynamics [4, 6] it seems that influences from GM areabsent. An expression for the irreversible entropy generation rate in a solar cellis obtained in his article “Thermodynamics of solar cell efficiency” [6], but thisderivation relies on an earlier paper [13] that uses microscopic theory based onthe Boltzmann transport equation rather than the macroscopic theory of GM.
2.2 Overview of NETPV
Here in Section 2.2, a brief overview will be given of NETPV with its methodsand goals. This should provide the reader with a map that will hopefullyreinforce a sense of direction while also providing some motivation as to whyNETPV is worth learning.
These are the steps and ingredients that go into NETPV:
1. Because of the fact that microscopic physics cannot give a definitive foundation for thermodynamics, the first step towards a mathematical modelfor NETPV is perhaps the most crucial one: the choice of variables. InNET, the choice of variables is motivated by ET and to do so, it is necessary that the system under study (i.e., a solar cell in our case) has anequilibrium state that more or less resembles the nonequilibrium stateone wishes to describe. Therefore, the ET description of a solar cell willbe described in Section 2.3 and its meaning elaborated on. It is assumedthat the reader has a basic understanding of ET, but to make sure thatthe reader is on the right page, Section 2.3 will also give a brief overview
29
of the subject in general terms. This section does not aim to give a detailed account of all of the mathematical methods from ET, but focusesmore on the underlying assumptions and ideas that are useful for NETPV
as well.
It will also be explained how the equilibrium description can be extendedto nonequilibrium situations: this is done by dividing the cell into manysmall subsystems that are each approximately in equilibrium and thenassigning thermodynamics variables to every subsystem. In a sense, theNET description of the cell is very similar to the ET description, but thenumber of thermodynamic variables is significantly greater in the nonequilibrium situation. The potential pitfalls in the generalisation stepfrom equilibrium to nonequilibrium are also discussed in Section 2.3.
2. The description of operating solar cells mostly focuses on nonequilibrium steady state conditions, but any system that is insulatedfrom its environment will return to equilibrium. This means that theoperating state of a cell is inherently characterised by its environment.The interaction of a solar cell with its surroundings is not straightforwarddue to the nonlocal nature of light absorption and will be considered inSection 2.4.
3. After specifying the relevant thermodynamic variables (step 1) and theinteraction of the cell with its environment (step 2), the next step is toobtain the equations that describe the cell. This is done by generalisingthe first law of thermodynamics to a local form and then writing downcontinuity equations for the conserved quantities. Section 2.5 will discussthis step.
4. The continuity equations introduce new quantities, namely the fluxes(i.e., currents) of the conserved quantities. To describe these fluxes, thetheory of Onsager [20] is used, which provides a general framework forobtaining fluxforce relations. To find the thermodynamically correctfluxes and forces in Onsager’s theory, the local entropy production rateis of crucial importance. The fluxforce relations will be discussed inSection 2.6.
5. Finally, symmetry considerations (such as isotropy of the material andreversibility of microscopic physical laws) can be used to establish someimportant simplifications. The most important of these are the Onsagerreciprocal relations and they will be discussed in Section 2.7. There arealso material symmetries relevant to solar cells and these will be discussedby using what is known as the Curie principle.
Finally, Section 2.8 will wrap up the discussion about NETPV by giving anoverview of the main takehome messages.
30
2.3 The thermodynamic formulation of solar cellphysics step 1: Equilibrium and thermodynamicvariables
The goal of Section 2.3 is twofold. First of all, the aim is to get the reader toappreciate what a thermodynamic description of a solar cell actually encompasses. This is done by giving a broad introduction to ET in general terms,especially about its underlying assumptions rather than the mathematical formalism. Whereas the mathematical formalism of ET is well established, themotivation for arriving at that formalism can differ significantly from author toauthor. This section does not follow one source in particular, though most ofthe influences come from the texts by Callen [21], Chandler [22] and Zemansky[23]. These books (especially Callen) are recommended for the critical readerwho needs more background than the brief discussion below.
The second aim of this section is more practical, namely to explain howET can be applied to solar cells. This application is intermixed with the general discussion of ET to ground some of the more abstract ideas with practicalexamples relevant to the reader. However, a solar cell is not an ideal demonstration system for all thermodynamic notions, so other examples will be usedas well. The works by Peter Wurfel, e.g., his book “Physics of Solar Cells” [1],are important sources for the ET description of solar cells.
Thermodynamics is the study of macroscopic systems based on macroscopicvariables and this means that one cannot fully reproduce thermodynamicsfrom microscopic laws alone. This gives thermodynamics a unique position inphysics: it never attempts to reduce a system to its elementary parts or to givea first principles explanation of a system (based on, e.g., quantum mechanics).Instead, thermodynamics can be seen as a sort of recipe that prescribes how tobuild a model for a system. In this recipe there are certain requirements thatthe model should satisfy (such as energy conservation), but thermodynamicsalso leave degrees of freedom in the way that the problem can be describedrather than prescribing everything apriori. Because of this freedom a physicist is allowed to insert new ideas into the model if that is deemed necessary,giving thermodynamics a wide range of application.
It would be incorrect to say that thermodynamics is completely disconnected from microscopic phenomena and fundamental laws, since it is wellknown that statistical mechanics provide a valuable link between microscopicand macroscopic views. However, to establish this link, statistical mechanicsrely on its own set of assumptions that (in general) cannot be derived from firstprinciples, such as the assumption of ergodicity and the assumption that allmicroscopic states with equal energy are equally likely to occur. The thermodynamic and microscopic descriptions of a system therefore have an interestingmutual dependency: the microscopic description can illuminate the underlying
31
mechanisms behind macroscopic observations, while the macroscopic laws provide a benchmark for the microscopic models and assumptions. In this work,most of the emphasis will be on the macroscopic point of view, though someideas from and links with microscopic physics will be briefly indicated.
Thermodynamics rely only on a small set of assumptions that will be brieflyreviewed here. It is common to take as the first assumption the law of conservation of energy, which has been solidified in the celebrated First Law ofThermodynamics. There is a reason why energy is such a crucial quantityfor thermodynamics, even though there is a whole range of other conservedquantities (momentum, angular momentum, charge, etc.): energy is the onlyconserved quantity that has many different manifestations. Whereas quantitiessuch as momentum only manifest themselves macroscopically in one way (e.g.,the centre of mass motion of the system), energy has many forms: mass, kineticenergy, electromagnetic fields, chemical potential and more. Most physicistswill agree that the first law is among the most secure in the whole of physicsand is unlikely to be overturned any time soon, making the foundation of thermodynamics very firm. In a sense, thermodynamics can be seen as the branchof physics that tries to make the very most out of the law of conservation ofenergy.
Before continuing, it is interesting to note that it is not strictly necessaryto start with the law of conservation of energy. In Callen’s view (chapter21), symmetries of the fundamental laws of physics are the real foundationsof thermodynamics. Central to this view is Noether’s theorem, which is apurely mathematical result that states that “for every continuous symmetryof the dynamical behaviour of a system there exists a conservation law forthat system”. As an example, the (continuous) timetranslation symmetryof the laws of physics (i.e., the physics of today are the same as those oftoday + ∆t for any given ∆t) implies the existence of a conserved quantity,namely energy. By the same argument, spacetranslation symmetry impliesconservation of momentum and rotational symmetry implies conservation ofangular momentum.
The law of conservation of energy, at its bare minimum, does not predictmuch yet. All it says is that associated with any system there is a number calledinternal energy U and that this number U will not change unless you allowenergy to flow into the system or leave the system. The law of conservationof energy does not prescribe how to measure U or how it can be exchangedbetween systems. To be of any value, additional rules need to be imposed onhow U transforms. In thermodynamics, this is done by assuming that the stateof the system is determined by U as well as a number of additional extrinsicmacroscopic variables, which will be referred to as Ai in general, with theindex i running from 1 till l. The Ai are sometimes also called thermodynamiccoordinates. The Ai are measurable properties of the system itself (as opposedto space and time coordinates, that are independent of the system), such as
32
volume V and number of particles of species α, Nα. The variables Ai arerequired to be extensive, meaning that the magnitude of every Ai is linear inthe size of the system. In practice, this means that if two identical samples of acertain material (say, two samples of gas) are added together, then the Ai (e.g.,the volume) for the composite system is also twice as great2. Every systemalso has an extensive property S called entropy that, because of its ubiquity,will always be associated with i = 1 (i.e., A1 = S). For now it suffices just toknow that entropy exists; its meaning will be discussed in a separate subsectionbelow.
In general, the Ai can be identified with some special combination of themicroscopic coordinates of the system. These combinations are special in thatthey are essentially constant in time, even though most microscopic coordinatesfluctuate on a time scale of 10−15 s, making them macroscopically completelyinaccessible. To quote Callen:
“Only those few particular combinations of atomic coordinates that areessentially time independent are macroscopically observable.”
In addition, macroscopic coordinates also need to be well defined over alarge length scale to be measurable. To give an example of how microscopicfreedoms can give rise to macroscopic coordinates, consider the phonon modesof a solid in the long wavelength limit λ → ∞, i.e., macroscopic vibrations.Phonons with large λ are simply sound waves and their frequency ω is givenby ω = 2πvsound/λ (with vsound the speed of sound in the solid). As can beseen, ω vanishes in the limit λ→∞. To realise why this is significant, considerwhat would happen if this were not the case: if the phonons with macroscopiclength scales would have a nonzero frequency, they would be fluctuating andthe solid would exhibit random expansions and contractions. This would meanthat the volume of the solid would not be constant. It can be concludedthat the vanishing frequency of the longwavelength phonons gives rise to amacroscopically welldefined quantity, namely volume. It is not an accidentthat the longwavelength phonons have zero frequency: this is a consequenceof a quantum mechanical result known as Goldstone’s theorem (see Callenchapter 21). It is beyond the scope of this section to go into details aboutGoldstone’s theorem, but here it suffices to state that, like Noether’s theorem,it is again a theorem about (broken) symmetry. This emphasises the centralrole of symmetries in thermodynamics.
The values of the variables Ai together characterise the thermodynamicstate of a system Ai = S,A2, ..., Al. It is assumed that the internal energy
2Note that this means that extra care has to be taken when the interface of a substancecontains energy. For example, when two identical samples of a liquid with a strong surfacetension are added together, the volume of the composite system will be twice large, but not thesurface. In this case, it is necessary to treat the surface as a (2 dimensional) thermodynamicsystem of its own.
33
is a unique function of the thermodynamic state, so that it is possible to write3:
U = U(S,A2, ..., Al). (2.1)
The exact functional form of U(S,A2, ..., Al) is known only in the simplest cases(e.g., the ideal gas), but all that really matters is that it exists in principle.This statement is stronger than it might initially sound: by assuming U =U(S,A2, ..., Al), it is immediately asserted that the history of the system is notimportant: all that matters is the values of the variables Ai right now. Themere fact that U has the functional form postulated here is the basis for manyuseful thermodynamic results, such as the Maxwell relations. In this light it isalso common to refer to U as the fundamental thermodynamic potential.
It is commonly assumed that U is also differentiable with respect to theextensive variables Ai. This makes it possible to relate changes in U to changesin Ai. This is important, because changes in quantities are generally muchmore experimentally accessible than absolute values of those quantities. Thepartial differentials ∂U/∂Ai are measurable thermodynamic quantities and aredenoted by fi:
fi(S, ..., Al) =∂U(S, ..., Al)
∂Ai. (2.2)
Because both U and the Ai are extensive, the fi are independent of the sizeof the system (i.e., the differential divides out the scale of the system). Thismakes the fi intensive quantities. The reader may recall from ET that itis possible to use a Legendre transformation to trade a coordinate Ai withits conjugate fi as independent variable. This procedure gives rise to differentthermodynamic potentials, such as the Helmholtz free energy F = U−TS thatdepends on temperature T rather than S. However, for NETPV the Legendretransformation is not of great interest so it will not be discussed in detail here.
To give a concrete example of how thermodynamic coordinates are picked,a solar cell under equilibrium is now considered. A solar cell is commonlymodelled to a good degree of accuracy as a container with a mixture of twogases: an electron gas and a hole gas. The thermodynamic coordinates thatdescribe such a gas mixture are entropy S, volume V , the number of freeelectrons Nn, and the number of free holes4 Np. This choice of variables is notunique: depending on the situation, different and/or more variables can be usedas well. For example, it is also possible to replace Nn and Np by two differentcoordinates that are sometimes more convenient: the number of electronhole
3By immediately postulating that U = U(S,A2, ..., Al), several of the finer points ofthermodynamics (that are outside of the current scope) are glossed over. The critical readeris referred to the textbooks mentioned at the start of this section.
4Free electrons and free holes will be indicated in the rest of the text simply by electronsand holes for brevity unless confusion can arise.
34
pairs Neh and the total electronhole charge Qnp. It should also be clarified thatS is not only the entropy of the electronhole gas but also of the backgroundlattice of the semiconductor. In principle, it is possible to split up S in theentropy of the electrons S−e , the entropy of the holes S+
h , and the entropy of thelattice Slat. However, it will be assumed throughout (both for equilibrium andnonequilibrium conditions) that all three of these subsystems are in thermalequilibrium so that they have the same temperature. For this reason it is onlynecessary to consider the sum S = S−e + S+
h + Slat. Furthermore, at this stageit is important to note that the energy in the field of photons in the solar cellis explicitly not included in the thermodynamic description, even though thephotons obviously play a crucial role in the operation of the device. In Section2.4 it will be explained that (and why) the photons will be considered as a partof the environment rather than the solar cell, though this is a matter of choiceand convenience rather than necessity.
The partial differentials corresponding to S, V , Nn, and Np are temperature T , (negative) pressure −P , and the electrochemical potentials ηn,p. Theelectrochemical potentials deserve some extra explanation. Like their namessuggest, ηn,p are the sum of electrostatic energy (+φ for holes, −φ for electrons) and chemical energy µc
n,p5. Electrostatic energy, in turn, is related to
charge while chemical energy is related to an amount of particles. In a solarcell, however, charge and particle number are both quantised in one and thesame entity, namely the electron (and consequently also the hole). Becauseof this fundamental coupling between charge and particle number it is impossible to remove charge from the system without removing particles and thedistinction between electrostatic and chemical energy cannot be made in practise. Thus, only the electrochemical energies are thermodynamically relevant.Electrochemical energies (or potentials, when divided by e) are not mysteriousnew quantities either: it was shown by Wurfel [1] that a regular Volt meteractually measures electrochemical potential rather than electrostatic potential,as is often believed.
The electrochemical potentials are basically the same quantities as the quasiFermi levels commonly used in semiconductor physics [1]. The only differenceis one minus sign for the holes: EFn = ηn, EFp = −ηp. In a thermodynamiccontext the minus sign can make equations confusing to read, so the choice wasmade to use ηn,p in this chapter. The intensive variables relevant for a solar
5Furthermore, there is also a contribution to ηn,p from the material in which the electronsand holes a located. These contributions are expressed using the electron affinity χ andbandgap EG, see Eqs. (A.3) in Appendix A.1
35
cell are defined by:
T =∂U(S, V,Nn, Np)
∂S=
(∂U
∂S
)V,Nn,Np
, (2.3a)
−P =∂U(S, V,Nn, Np)
∂V=
(∂U
∂V
)S,Nn,Np
, (2.3b)
ηn =∂U(S, V,Nn, Np)
∂Nn=
(∂U
∂Nn
)S,V,Np
, (2.3c)
ηp =∂U(S, V,Nn, Np)
∂Np=
(∂U
∂Np
)S,V,Nn
. (2.3d)
As will be discussed in the next section, T is always the intensive variablecorresponding to S. The somewhat peculiar notation on the rightmost sidesof Eqs. (2.3) is used in thermodynamics to remind the reader what remaining variables are considered to be the independent freedoms of the system.This also means that for this choice of variables the intensive quantities arefunctions of S, V , Nn, and Np as well (e.g., T = T (S, V,Nn, Np)). This is especially important when Legendre transformations are used to trade extensivecoordinates for intensive ones.
The idea that U is a differentiable function of several coordinates is commonly stated briefly using the Gibbs form of the first law. The general formis:
dU =l∑
i=1
fi dAi. (2.4)
The differential d is used here to denote what is called an exact differential.This simply means that U can be considered to be a function of the Ai, asis required. If the differentials were inexact (denoted by d), it would not bepossible to consider U as a function of the Ai. When Eq. (2.4) is applied tosolar cells, it becomes:
dU = T dS − P dV + ηn dNn + ηp dNp. (2.5)
In a sense, Eq. (2.5) can be considered as a condensed version of Eqs. (2.3).Eq. (2.5) can also be given in terms of Neh and Qnp by using the followingtransformations:
dNeh =1
2( dNn + dNp) , (2.6a)
dQnp = dNp − dNn. (2.6b)
36
Note that Qnp is defined here in units of cm−3. With these definitions, thefirst law can be written as:
dU = T dS − P dV + (ηn + ηp) dNeh +1
2(ηp − ηn) dQnp,
dU = T dS − P dV + ∆ηeh dNeh + ΦQ dQnp. (2.7)
Here ∆ηeh = (ηp + ηn) is the free energy per electronhole pair and ΦQ =(ηp − ηn)/2 is the conjugate variable for the charge. The latter should notbe confused with the electrostatic energy φ since it is not possible to extractcharge from the cell without extracting electrons or holes. In other words,ΦQ accounts for both the changes in electrostatic energy as chemical energywhen charge is removed/added to the system. If the carrier statistics (eitherMaxwellBoltzmann or FermiDirac) expressions for the electrons and holesare used (Eqs. (A.3) in Appendix A.1), then the thermodynamic energy percharge ΦQ is
ΦQ = φ+ χ+EG
2+kBT
2
[F←1/2
(p
NV
)− F←1/2
(n
NC
)](2.8)
and it can be seen that it includes φ, the electron affinity χ, the bandgap EG,as well as terms that take into account that charge has to be changed by adding(or removing) electrons/holes in such a way that the e−–h+ plasma stays inequilibrium.
The discussion above should make it clear that the first step in makinga thermodynamic description of a system is to identify the variables Ai forthe system under study and that this first step is crucial to the success of thethermodynamic approach. If not all relevant variables are found, there is agreat chance that thermodynamics cannot be applied unless special conditionsare met. If one tries to describe the system as U(S, ..., Al−1) (i.e., withouttaking Al into account), the thermodynamics will only work as long as Alstays constant during the experiment (and is therefore essentially still underexperimental control) or if U is insensitive to Al (meaning that Al is simplynot relevant to the physics at hand).
Suppose, for example, one would like to describe a pure gas (such as N2) ina sealedoff container and one would identify S and V as the relevant coordinates. In this example, the number of molecules N has been deliberately leftout, perhaps as a simplification. The proper thermodynamic function for theinternal energy is denoted by Ugas(S, V,N). Because the container is sealedoff,N = N0 is constant and for the sake of the experiment at hand, the descriptionin terms of just S, V will work just as well as that in terms of S, V,N. Theinternal energy for this experiment is denoted by Ugas(S, V ) = Ugas(S, V,N0)and Ugas(S, V ) will be referred to as a reduced potential. However, the momentN is no longer constant (think of, e.g, a safety valve that releases gas when
37
the pressure reaches a critical value), the reduced potential Ugas(S, V ) will nolonger contain enough information to give a thermodynamic description of thesystem. Conversely, by using the original description S, V,N one has alreadymade a lot of implicit assumptions about the physics relevant for the gas. Forexample, all possible chemical reactions that N2 can have with itself have beenneglected because they are so rare in practice.
Note how the volume of the cell can be omitted in the solar cell description U(S, V,Nn, Np) proposed earlier in this section. Of course U is not trulyindependent of V , but this (reduced) representation of U is still useful becausethe volume of a cell is constant to a very good approximation under most experimental conditions. For this reason, V will be omitted in most discussionsof solar cell thermodynamics in this work to simplify the mathematics. However, care should be taken because certain thermodynamic results cannot beused when working with reduced potentials. For example, the Euler equation6
states that if:
U(λS, λA2, ..., λAl) = λU(S,A2, ..., Al), (2.9)
for every scaling factor λ, then:
U =
l∑i=1
fiAi. (2.10)
The Euler equation applies to every system where all the extensive Ai correspond to effects of the same dimensionality (e.g., all Ai are bulkrelatedvariables or they are all surfacerelated variables). For a solar cell, S, Nn, andNp are all bulk coordinates, however if one wishes to use the Euler equation,it is necessary to include V as a variable as well. The correct expression for Uis:
U = TS + ηnNn + ηpNp − PV. (2.11)
Here, P = −(∂U/∂V )S,Nn,Np is the pressure of the (ideal) free electronholegas. The pressure is the sum of the partial pressures of the electrons and holes:
P = P−e + P+h =
kBT
V(Nn +Np). (2.12)
Note that a naive application of the Euler equation on the reduced potentialU(S,Nn, Np) would give the incorrect result U = TS + ηnNn + ηpNp, whichmisses the −PV term.
6It is somewhat confusing that so many equations and mathematical results carry Euler’sname due to his incredible productivity. The Euler equation referred to here is also knownas the Euler homogeneous function theorem.
38
The situation of describing a system while using insufficient thermodynamicvariables is somewhat analogous to the phenomenon of degeneracy in quantummechanics (QM): in QM, degeneracy occurs whenever a certain quantum number no longer uniquely specifies the state of the system and more quantumnumbers need to be added to make the specification unique again. In the sameway, the energy of the system Ugas(S, V ) is degenerate in the numbers S andV because extra information about the particle number N is needed to specifythe energy uniquely. The similarity with QM is not just a superficial one: justlike in QM, degeneracy of variables in thermodynamics can happen becauseof symmetries that suddenly become important. A famous example given byCallen is the case of ortho and parahydrogen molecules: in an orthohydrogenmolecule the proton spins of two atoms are in a triplet state, while in parahydrogen they are in a singlet state. At high temperatures, these two differenttypes of hydrogen gas can be described by a single particle number NH becausethey behave essentially the same. At very low temperatures, however, the fundamentally different symmetries of ortho and parahydrogen necessitate theuse of two particle numbers Northo and Npara.
The case of ortho and parahydrogen should illustrate that it can be a bitof an art to find coordinates Ai such that the system can be described by afunction U(S, ..., Al). In other words: thermodynamics provides a prescriptionfor how to build a macroscopic model of a system, but ultimately that modelwill have to be verified by experiment just like any other physical model. Itwas demonstrated that too few variables will lead to inconsistencies in the description, so how about the other extreme of the spectrum? Obviously, onecan always resort to a fully microscopic description and use all internal quantum mechanical degrees of freedom, which will be denoted by νi. So in thiscase Ai = νi. No doubt this will result in a mathematically correct model: nomatter what system is under scrutiny or even how close or far away it is fromequilibrium, the quantum mechanical equation of motion guarantees that theenergy is a unique function of the νi. From a practical point of view, though,it is desirable to not invoke more variables than strictly necessary and certainly not as many as the full microscopic description demands. Moreover, aswas indicated previously in this section, only very few specific combinations ofthe νi are accessible on macroscopic temporal and spatial scales. Invoking theremaining inaccessible degrees of freedom will only lead to a theory that is completely disconnected from experiment. Still, for the sake of the argument it willsometimes be pretended that the choice Ai = νi is a pseudothermodynamic(denoted as: “thermodynamic”) description. As a result, there is now a wholespectrum of thermodynamic descriptions ranging over the number of coordinates used: at one extreme there are the formalisms that use too few variablesand at the other end there are those that use too many. A formalism withtoo few variables is mathematically inconsistent while one with too many is nolonger empirical and therefore has no physical content.
39
The previous discussion shows where the limitation of thermodynamics lies:the moment one loses track of the variables that describe where energy is hidingduring the experiment is the moment the thermodynamic description breaksdown. In principle, every system, whether it is in thermodynamic equilibriumor not, can be described by adding enough coordinates to the description. Afterall, the conservation of energy should apply to any system and the energy is,microscopically, only a function of the current state and never of its history orfuture. Ultimately, one can keep adding variables until every internal freedomhas been accounted for, though doing so quickly makes it impossible to exertcontrol over all of these variables.
2.3.1 Entropy
So far the entropy S has only been mentioned in passing as one of the thermodynamic coordinates Ai. The role of S in thermodynamics has a coupleof different facets and properties. These will be outlined below, though thefollowing list should be treated as not more than a list of known results: nohard proofs will be presented here.
1. Entropy is an important state variable for the calculation of efficiencies ofworkproducing apparatus. As an example, consider a heat engine thatoperates between a hot reservoir at temperature Th and a cold reservoir attemperature Tc. Then the efficiency is always bounded by η = W/QH ≤1−Tc/Th, with Qh the amount of heat extracted during one cycle and Wthe work produced during that cycle. If during the cycle also S amountof entropy is produced, then the work W done by the engine is given by:
W =
(1− Tc
Th
)QH − TcS = ηmaxQH − TcS. (2.13)
As can be seen, the production of entropy is in direct relation with theloss of useful work that can be extracted from the engine. A solar cell isno different in that regard: any production of entropy inside of the devicediminishes the output power and leads to extra production of lowqualityheat.
2. The internal energy U(S, ..., Al) is a monotonically increasing function ofS and the slope of U vs S is defined to be the temperature T . In short:(
∂U
∂S
)A2,...,Al
= T > 0. (2.14)
Especially the property ∂U/∂S > 0 is very significant: it means that Ucan be inverted with respect to S so that the entropy can be consideredto be a function of U and the remaining Ai:
S = S(U,A2, ..., Al). (2.15)
40
By using this inversion it becomes possible to do thermodynamics with Sinstead of U as the fundamental potential. In fact, it will turn out that fornonequilibrium systems, S is actually a more convenient potential thanU because U is a conserved quantity and is therefore more suitable tobe used as an independent variable than S. To avoid notational clutter,whenever S is used as a potential, the variables it depends on will becalled Bi, with B1 = U and Bi = Ai for i ≥ 2. The partial differentialsof S are called gi = (∂S/∂Bi)Bj ,j 6=i so that the change in entropy of asystem can be written as:
dS =l∑
i=1
gi dBi. (2.16)
For a solar cell, the differential form of S can be found by inverting Eq.(2.5):
dS =1
TdU − ηn
TdNn −
ηpT
dNp
= β dU − ηn dNn − ηp dNp (2.17)
The conjugates coordinates β and ηn,p have been introduced for convenience: the tilde indicates that the quantity has been divided by T . Interms of Neh and Qnp, dS is given by:
dS = β dU − ∆ηehT
dNeh −ΦQ
TdQ
= β dU −∆ηeh dNeh − ΦQ dQnp. (2.18)
3. The Second Law of Thermodynamics states that the entropy of a closedsystem (meaning: a system that has no exchange of energy of any kindwith the outside world) cannot decrease. Closely related to the secondlaw is the maximum entropy principle (explained in detail below), whichis a crucial tool for the analysis of the thermodynamic equilibrium of asystem. It states that the entropy of a closed equilibrium system takes thehighest possible value consistent with the internal constraints imposed onthat system.
4. From a microscopic point of view, the entropy S(U,B2, ..., Bl) is relatedto the number of possible microstates of a closed system with macroscopic parameters Bi. This number of microstates will be denoted byΩ(U,B2, ..., Bl) and the famous Boltzmann result then states that:
S(U,B2, ..., Bl) = kB ln Ω(U,B2, ..., Bl). (2.19)
41
Note the dependence of Ω on the variables Bi: not only does Ω dependon the values of the Bi, but also on the choice of the set of variables. Themost extreme example of this second dependency is the “thermodynamic”description based on the full set of microscopic coordinates νi: in thatcase, every “thermodynamic” state is a microstate so that Ω(ν1, ..., νl) =1 and:
S(ν1, ..., νl) = kB ln 1 = 0. (2.20)
This means that the value of the entropy depends on what is assumed tobe known and what not. If this sounds surprising, it is helpful to thinkof the analogous problem of the interpretation of probabilities. Considerthe question “What is the probability that a coin is head side up?”.Obviously, this question cannot be answered in a meaningful way withoutfurther details about the coin. Was it flipped just now or did someone putit on its side on the table? Who needs to answer the question and did thisperson see the coin? Is the coin fair? Questions about probability canonly have meaningful answers in a framework of all of the prior knowledgethat is involved and assumed. Entropy is no different in that regard (seealso, e.g., Ottinger [17]).
The maximum entropy principle deserves some clarification, since it willbe used in Section 2.6. A simple example of this principle can be given byconsidering the equilibrium state of a solar cell. For example, if the cell isinsulated from its environment, the system is free to find its own values forNn and Np because electrons and holes can be generated and annihilated inpairs. Imagine that the system spontaneously generates a small amount ofδNeh electronhole pairs. Because the cell is insulated, the total energy andcharge of the cell cannot change spontaneously, so δU = δQnp = 0. Then fromEq. (2.18) the total first order entropy change can be calculated:
δS = −∆ηehδNeh = −∆ηehT
δNeh. (2.21)
The maximum entropy principle now states that under equilibrium any suchvariation δNeh will decrease the entropy so that ∀δNeh : δS ≤ 0. Since δNeh canbe both positive and negative, this yields the familiar result that ∆ηeh = EFn−EFp = 0, i.e., there is no Fermi level splitting in equilibrium and electronholepairs are in electrochemical equilibrium and have no free energy. In principlethis means that under equilibrium Neh is a thermodynamic variable that canbe neglected, but the essential feature of a solar cell is that ∆ηeh > 0 so forthe generalisation to nonequilibrium Neh is retained.
The imaginary change in Neh is an example of applying an internal constraint. By considering what kind of internal freedoms a closed system has,equilibrium conditions can be obtained. In the example above, only the first
42
order variation in S was considered, which usually yields a necessary condition for equilibrium, but not a sufficient condition. This is because the firstorder variations of S usually yields δS = 0, so if the second order variationδ2S would be positive, the equilibrium would still be unstable. Therefore, toobtain sufficient conditions (often referred to as stability criteria), higher orderterms in the variation of S need to be considered as well. The second ordervariation in entropy for electronhole variations δNeh is given by:
δ2S =1
2
∂2S
∂N2eh
δN2eh = −1
2
(∂∆ηeh
∂Neh
)U,Qnp
δN2eh ≤ 0, so:(
∂∆ηeh
∂Neh
)U,Qnp
≥ 0. (2.22)
This result means that the creation of an electronhole pair will increase theFermi level splitting, which is a crucial property that makes it possible togenerate useful work from a solar cell.
2.3.2 Generalisation to nonequilibrium
So far only the equilibrium state for a solar cell has been considered, whichcan be described by the three coordinates S, Nn and Np. The question thatwill be addressed now, is how this equilibrium description can be expandedupon to give a description of a solar cell under nonequilibrium conditions.The main idea that will be used here is that a thermodynamic descriptionof a nonequilibrium system is not fundamentally different, except that thechoice of variables can be significantly more difficult. In such systems theenergy can be distributed over many different phenomena depending on theexact nature of the nonequilibrium situation. For example, in a laminar fluidflow the energy can be traced quite easily and in such a situation NET canbe used to obtain transport equations (i.e., the NavierStokes equations) forthe fluid [3]. However, when the flow transitions from laminar to turbulent itsuddenly becomes very difficult to find out how much energy is in the turbulentvortices. Clearly, the energy associated with a vortex is some sort of kineticenergy, but unless the exact flow pattern of the vortex is known, this energygenerally cannot be accounted for. It is just as undesirable to calculate theexact flow of a vortex as it is to track heat by considering the kinetic energy ofindividual particles. Furthermore, in nonequilibrium thermodynamics it canbecome very difficult to assure that the extensive variables truly scale with thesize of the system. If one scales a block of ice to ten times its original size,nothing special happens. However, if a system with a fluid flow is scaled insize, the flow might change completely (going from laminar to turbulent, forexample), so in NET it is not always possible to scale extensive variables likein Eq. (2.9).
43
It suffices to say that there is no single method that can reliably provide afunctional set of thermodynamic coordinates that describe any nonequilibriumsystem, but fortunately there is a method that works well for reasonably wellbehaved systems (like solar cells) that do not suffer from complications such asturbulence. This is the method of De Groot and Mazur which basically usesthe ET description of a system as a starting point. In NETGM the assumption of local thermodynamic equilibrium (LTE) is used. This means that thesystem is divided into many small (but still macroscopic) subsystems, each ofwhich is approximately in equilibrium so that they can be described by thesame thermodynamic coordinates that were used in the ET description. Eachsubsystem is labeled with a space coordinate xj with j ∈ 1, ...,M and Mthe number of subsystems. The entropy S is used as thermodynamic potentialand the variables for the system are then denoted by Bi,xj . In general, thecoordinates are also allowed to depend on time, though this possibility is notconsidered here since the main goal is to describe the steadystate operationof a solar cell. The functional dependence of S is now given as:
S = S (Ux1 , ..., UxM , B2,x1 , ..., B2,xM , ..., Bl,x1 , ..., Bl,xM ) , (2.23)
i.e., there are l×M independent variables. For a solar cell this means that theGibbs form of the first law in NETPV generalises Eq. (2.17) and becomes:
dS =
M∑j=1
[βxj dUxj − ηn,xj dNn,xj − ηp,xj dNp,xj
]. (2.24)
As can be seen, NETPV uses 3M coordinates. Obviously, M has to be largeenough that there is enough spatial resolution to, e.g., assign a proper temperature Txj to each subsystem. Yet at the same time 3M still has to be muchsmaller than the number of microscopic coordinates, otherwise NETPV wouldbe overdetermined and would not qualify as a practical macroscopic description. Besides these two requirements, there is no clear criterion for how largeM should be. This means that the resulting theory should be independent ofM over a wide range of values.
The generalisation of Eq. (2.17) to Eq. (2.24) is mathematically simple,but its physical implications are substantial. It is important to realise that inEq. (2.17) the three variables U , Nn and Np (or their conjugates β and ηn,p)are in principle experimentally accessible. However, it cannot be expected thatthe experimentalist has simultaneous control over all 3M variables occurringin Eq. (2.24), so it can be said that a nonequilibrium system is more difficult to control because its description involves more variables. This loss ofexperimental control can be considered to be the reason that nonequilibriumsystems generate entropy.
Because the description of the cell should not depend on the choice of M(as long as M is large enough), it is more convenient to write Eq. (2.24) as
44
a integral over the cell. The integration domain will be referred to as Ω andthe integration densities will be denoted by lower case letters. For example,dUxj = du(x) dx3 = du dx3. The dependence of u on x will be suppressedto save space unless extra attention needs to be called to it. Eq. (2.24) thenbecomes:
dS =y
x∈Ω
dx3 (β du− ηn dn− ηp dp) (2.25)
=y
x∈Ω
dx3 ds. (2.26)
Here, s has been introduced as the local entropy density. It is worth notingthat in the book by GM slightly different definitions are used for the densitiess, u, n, and p since there the densities are normalised to the mass density. Ina solar cell with electrons and holes, however, the concept of mass is not veryuseful and it is more convenient to work with volumetric densities instead.
The notation in Eq. (2.25) is mathematically sloppy since du refers to achange in a thermodynamic variable while dx3 is simply a volume element forthe integration. Nevertheless, for convenience this is the form that will be usedand the expression x ∈ Ω is placed under the integral to remind the reader thatthe integration is over x. However, despite its appearance, Eq. (2.25) shouldstill be treated formally as a finite sum: the use of an integral is nothing morethan mathematical and notational convenience.
If the maximum entropy principle is applied to Eq. (2.25), it can bedemonstrated that under equilibrium all of the intensive variables are constant throughout the system. As before, the e−–h+ density neh(x) and chargedensity ρ(x) are the most convenient coordinates to work with. The first ordervariation of S is given by:
δS =y
x∈Ω
dx3(βδu−∆ηehδneh − ΦQδρ
)= 0. (2.27)
The δu(x), δneh(x), and δρ(x) can be considered to be unknown functions thatrepresent how the system can potentially rearrange its internal configurationand the equality should hold for every conceivable combination of such functions. Since the variation δneh is unconstrained, it can be concluded again (likein the equilibrium case) that its prefactor has to be zero: ∆ηeh = 0. Note thatthis is why δS = 0 has been imposed, rather than δS ≤ 0. Since the system isclosed, the total variations in U and Qnp have to be zero:
δU =y
x∈Ω
dx3δu = 0, (2.28)
δQnp =y
x∈Ω
dx3δρ = 0. (2.29)
45
These constraints can be imposed by using Lagrange multipliers, but here adifferent method is introduced based on displacement vectors δDu,ρ(x). Thesedisplacement vectors describe how the internal energy and charge can be redistributed through the solar cell. In the continuum limit, the total change inenergy or charge in a subvolume at position x is then:
δu = −∇ · δDu, (2.30)
δρ = −∇ · δDρ. (2.31)
The internal constraint that the system is insulated completely can then beimposed by demanding that δDu,ρ ·n = 0 on the boundary ∂Ω (with n the unitnormal vector). This means that no displacements will take energy or chargein or out of the system. Eq. (2.27) then becomes (recall that ∆ηeh = 0):
δS =y
x∈Ω
dx3(−β∇ · δDu + ΦQ∇ · δDρ
)=
x∈∂Ω
dx2 n ·(−βδDu + ΦQδDρ
)+
y
x∈Ω
dx3(δDu · ∇β − δDρ · ∇ΦQ
)= 0. (2.32)
The surface integral (x ∈ ∂Ω) is zero because δDu,ρ · n = 0. From the volumeintegral it can be concluded that ∇β = ∇ΦQ = 0, since that is the only waythe integral can be zero for all vector fields δDu,ρ. Thus, β, ∆ηeh = 0, andΦQ are all constant as claimed. This justifies why in ET, e.g., only a singletemperature is needed to describe the cell: it is possible to use more thanone nonlocal temperature, but the maximum entropy principle can be usedto immediately prove that all temperatures are equal anyway. Note how theproblem of the number of variables has also sorted itself out in this situation:by pretending that dS can be written in the integral form of Eq. (2.25),one formally assumes an infinite number of coordinates, which is certainly toomany from a practical point of view. However, for the equilibrium situationthis infinitude of variables can be quickly reduced to three, so this gives avote of confidence that (as long as the mathematics are applied correctly) theintegral form of dS does not lead to big inconsistencies or overdeterminationof the problem.
Finally, note that the idea of rearranging internal variables in a closedsystem only makes sense when extensive coordinates are used as the primaryindependent variables for the system. Constraints such as Eqs. (2.28) and(2.29) cannot be applied to quantities like (local) temperature and neither isit possible to talk about displacements or flows of temperature. This is oneof the reasons why in NETGM extensive coordinates are often preferred overintensive ones.
46
2.4 The thermodynamic formulation of solar cellphysics step 2: Interaction with the environment
So far the discussion of the solar cell thermodynamics has been almost exclusively about closed systems. In fact, the maximum entropy principle was usedto demonstrate that in a closed system it does not matter if one divides thecell into subsystems with different temperatures etc.: in the end, the cell willonly have just one welldefined temperature. To prove this, the assumptionthat the cell is a closed system was crucial, otherwise it would not be possibleto conclude that the boundary term in Eq. (2.32) is zero.
Interaction with the environment is essential for understanding nonequilibrium situations, especially those that show steadystate behaviour, likea solar cell does. Of course, it would be impossible for a solar cell to generateuseful work if it were completely closed off from the rest of the universe and itwould be equally impossible to extract that work. However, for a solar cell theinteraction with the environment is more complex than for most systems. Tosee why, it is instructive to first understand how nonequilibrium steadystatesituations can occur for simple systems.
In most systems (the solar cell being an important exception, as will beexplained) the only interaction with the environment happens at a clearlydefined interface that separates the inside world from the outside. For mostsystems it is possible to draw an imaginary box around the system and toaccount for the influence of the environment by specifying boundary conditionsat the surface of that box. For example, when a metal rod is placed such thatone end is in contact with a cold reservoir (T = Tc) and the other end isin contact with a hot reservoir (T = Th > Tc), then it can be said that theenvironment forces two different temperatures at either end of the rod. As wasshown in Section 2.3, thermodynamics tries to achieve∇T = 0 inside of the rod,but because of the BCs imposed by the environment this is simply not possible(unless discontinuities in T are allowed, but those would not make physicalsense). After a while, a steadystate nonequilibrium situation is achievedwhere the temperature in the rod assumes a nonuniform distribution overits length that gradually goes from hot to cold and stays constant in time.Of course, in the long run the combined system of “rod+environment” willreach an equilibrium nonetheless: the rod will conduct heat from hot to coldand eventually the temperature difference will be equalised. However, the keyaspect here is that this global equilibration time is much slower than the timeit takes the rod to arrive at an internal steadystate nonequilibrium situation.Note, however, that it is not always the case that a system reaches a steadystate just because the BCs provided by the environment change much slowerthan the internal dynamics of the system. As an example, a steady stream of
47
fluid that is guided through a partially obstructed canal can develop turbulenceand the flow will not reach a steady state even though the BCs have no timedependence. In this case, the erratic behaviour is intrinsic to the system itself.
In nonequilibrium situations there is always generation of entropy and sincethis entropy cannot accumulate inside of the system (because of the steadystate assumption), entropy has to be ejected from the system continuously. Forexample, consider the metal rod again over a short period of time dt. Duringthis time, the hot reservoir injects a certain amount of heat dQh > 0 into therod. It is assumed that the hot reservoir and the local temperature of the rodare equal, so dQh is reversible heat and therefore the hot reservoir also injectsan amount of entropy dSh = dQh/Th into the rod. Because of the steadystatecondition, the same amount of heat dQc = −dQh is ejected from the rod atthe cold reservoir, along with an amount of entropy dSc = dQc/Tc. Note thatdSh + dSc < 0, yet the steadystate assumption asserts that the entropy of therod cannot have changed, so clearly extra entropy dSirr has been created insideof the rod such that dSh + dSc + dSirr = 0. This is the entropy generationassociated with the irreversible process of heat conduction inside of the rod.The main conclusion to draw from this thought experiment is that irreversibleentropy production is related to gradients in intensive variables (∇T 6= 0) andflows of extensive variables (in this example the flow of energy that heats up thecold reservoir). In Section 2.5 this relation will be discussed more thoroughly.
In the case of a solar cell, the interaction with the environment is more complex than for the heat conducting metal rod. This is because the environmentis providing energy to the cell in the form of a constant stream of photons thatdo not interact with the cell at a welldefined interface. In fact, some of the lowenergy photons can travel all the way through the cell and reflect on internalinterfaces several times before either being absorbed or exiting the cell. Thismeans that if one chooses to do the energy bookkeeping by putting an imaginary box around the cell and then imposing BCs on the edges of that box, it isimportant to keep track not only of the cell itself but also of the photons insidein order to make the sure the balance adds up. As a consequence, it is thenrequired to include thermodynamic coordinates for the energy in the photonfield and to model transport of energy due to radiative recombination (RR)and reabsorption of photons, which is a formidable task. A model whereby thephotons are considered as part of the thermodynamic system will be referredto as a bilateral model. This terminology refers to the fact that the photonscan affect the electrons and vice versa. The complexity of such a descriptioninvites the use of additional simplifications. Such a simplification can be toconsider the photons as part of the environment, meaning that the photonsaffect the electrons in the cell, but not the other way around. This is calleda unilateral description and in this case there are no thermodynamic variablesthat describe the photons inside the cell. To see how the thermodynamic description of a solar cell (which is bilateral in principle) can be simplified to
48
a unilateral one, it is instructive to first consider how the problem is usuallyhandled in semiconductor physics.
In solar cell simulations (especially for cSi devices), it is common practise toseparate the optical and electrical description of the device. First, an opticalsimulation is done using, e.g., a LambertBeer model or ray tracing. Theoptical simulation calculates how the light propagates through the cell andhow much light is absorbed in the semiconductor at every position and thenthe result of the optical model is used as an input for the electrical modelof the device that calculates the electron and hole densities from transportmodels. In this procedure, the absorption profile is calculated from knownmaterial properties (i.e., the complex dielectric function or refractive index) anddoes not depend on the nonequilibrium situation of the cell (e.g., the electronand hole densities, which are not even known yet at this first stage). Thereason this unilateral coupling of optical and electrical models generally workswell, is that there is a great asymmetry in the way photons interact with theelectrons/holes in the cell. Whereas the main source of photons is the externalinflux from the sun, the main source of electrons and holes is the generationdue to photons. The exceptions to this rule are highefficiency devices basedon directbandgap semiconductors: in those, the radiative recombination (andpossibly even stimulated emission) provides a significant contribution to thephoton field [24], making it absolutely necessary to couple the optical andelectrical models bilaterally rather than unilaterally. Thus, if one wishes topush the efficiency of solar cells to the absolute limit, it becomes essentialto explicitly include the thermodynamic coordinates of the photons into themodel.
The question of whether to use a unilateral or bilateral coupling of photonsand electrons can be rather subtle. It is discussed briefly in the paper byLindefelt [14], where he remarks that for the accuracy of a calculation it is bestto either use a full bilateral coupling between electrical and optical model or touse a fully unilateral model. The inbetween option, whereby RR is includedas a loss mechanism for the electronhole pairs but not as a source term for thephoton field, is less accurate according to Lindefelt and he bases that claim ona paper [25] that numerically compares these three methods for a GaAs device.The idea is that in RR the photons that are generated are often recycled sincethe strengths of emission and absorption are proportional to each other. Thus,if in a unilateral model the RR is included, reabsorption is not considered andthe recombination losses are overestimated. In the modelling of cSi solar cells,however, it is not uncommon to use a unilateral model together with RR. Thesituation for cSi (which has an indirect bandgap) is different than for GaAs (adirect bandgap semiconductor), since in cSi the RR is generally much smallerthan the Auger recombination and because the reabsorption of photons is veryunlikely due to the very low absorption coefficient for photons with energiesclose to the cSi bandgap.
49
Figure 2.1: Schematic representation of the extension of equilibrium to nonequilibriumthermodynamics for a solar cell: the equilibrium variables become localised and the systemis no longer insulated from its environment.
The preceding discussion shows that it is not always entirely clear how tosimplify a bilateral description to a unilateral one, but the main idea is clear:first the absorption profile of the photons is calculated from predeterminedmaterial parameters and then this generation profile is used as a source termfor the thermodynamic processes in the solar cell. These source terms willbe addressed in Section 2.5. So to conclude, the environment couples to asolar cell in two distinct ways: at the cell boundaries there is the thermaland electrical contact with the environment which is described by boundaryconditions. Inside of the cell there is the interaction between the light fieldand the electronhole gas which is (approximately) taken into account throughsource terms.
2.5 The thermodynamic formulation of solar cellphysics step 3: Continuity equations
Figure 2.1 illustrates the main ideas that were discussed so far in Sections 2.3and 2.4. At this point it is time to develop the mathematics that describethe solar cell. It was explained how the equilibrium solar cell description wasgeneralised to nonequilibrium by dividing the cell in M small subsystems withcoordinates xj and assigning thermodynamic coordinates to each subsystem.This made it possible to write dS as a sum of the local entropy dsxj over the
50
subsystems, with ds given by:
ds = β du− ηn dn− ηp dp. (2.33)
Eq. (2.33) can be considered to be the local form of the first law. Recall that,for mathematical convenience, the sum over xi was treated as a volume integraland that the densities u, n, and p were used as the independent thermodynamiccoordinates for the solar cell.
The description of a working solar cell does not only deal with densitiesbut also with flows. Flows (denoted by J) are introduced into the model bypostulating continuity equations for the densities of extensive variables, justlike in SCP. However, a significant difference between NETGM and SCP is thatin the former the entropy continuity equation is of central interest while in SCPthe main focus tends to be on the conservation laws for electrons and holes.The continuity equations for s, u, n, and p are given by:
∂s
∂t+∇ · Js = qs, (2.34a)
∂u
∂t+∇ · Ju = qu, (2.34b)
∂n
∂t+∇ · Jn = qn, (2.34c)
∂p
∂t+∇ · Jp = qp. (2.34d)
The symbol q is used to represent source terms in the continuity equations andthe ∂/∂t terms have been included for completeness because they will be necessary for deriving the expression for qs in the next subsection. For the remainderof this chapter, however, the time derivatives will be set to zero because onlysteadystate solutions are of interest here. Eqs. (2.34) put constraints on whatflows can be considered, but they do not give a unique definition since J onlyappears inside of a divergence in each equation. The unique definitions of theflows will be given in Section 2.6, but first the continuity equations, and theentropy source term qs in particular, will be considered on their own merits.
The source terms qu,n,p in Eqs. (2.34) are, in principle, known quantitiesand will be discussed first because they are important for deriving qs. Theyare:
qu = εγ(x)G(x)− εγ,RadRRad, (2.35a)
qn = G(x)−R(n, p, ...), (2.35b)
qp = G(x)−R(n, p, ...). (2.35c)
Here, G is the generation rate of electronhole pairs obtained from an opticalmodel, εγ the average absorbed photon energy, εγ,Rad the average energy of
51
photons emitted by radiative recombination7, and R (RRad) the (radiative)electronhole recombination rate. At this point it is important to make aclear distinction between two different type of sources: those that are due tointeraction with the environment and those that are due to internal irreversibleprocesses in the system. This will be especially important when considering theentropy source term, since there is a fundamental difference between entropythat is generated due to irreversible dynamics and entropy that is transferredbetween the system and its surroundings.
Section 2.4 discussed that in a solar cell the photons interact with thecell all the way throughout the bulk. If the photons were represented by aset of thermodynamic coordinates, then such an interaction would not changethe energy density and qu = 0. However, the choice for a unilateral couplingbetween photons and electrons necessitates the use of a nonzero source termqu > 0 which represents the interaction between the environment and the cell.Note that the source term for u depends on whether or not the backgroundsemiconductor lattice of the cell is considered as part of the thermodynamicsystem or not8: if only the electronhole gas would considered (assuming it isnondegenerate), then qu would instead be given by:
qu,electronhole gas = (EG + 3kBT )G− εγ,RadRRad +H, (2.36)
with EG the bandgap of the semiconductor. The 3kBT term is the averagekinetic energy of an electronhole pair and H is the energy transferred between the lattice and the e−–h+ gas9. To put it succinctly: qu in Eq. (2.35a)represents all the energy transferred to and from the cell by the photons andincludes the heating of the semiconductor lattice, whereas qu,electronhole gas inEq. (2.36) only represents the energy transferred to and from the electronholepairs.
Looking at the source terms qn,p, it can be seen that these have two different contributions: the generation G that represents an interaction with theenvironment and the recombination R that is mostly due to the internal dynamics of the cell. The exception to the latter is radiative recombination RRad,which also represents a coupling to the environment. For now, RRad = 0 willbe assumed for the reasons given by Lindefelt (see Section 2.4) and this choicealso makes the distinction between internal dynamics (R) and interaction with
7Which is equal to the semiconductor bandgap if broadening effects are ignored8recall from Section 2.3 that the choice was made to include the lattice in the thermody
namic description presented here.9Usually in the from of heat, hence the symbol H. Note that the energy thermalisation
loss upon the excitation (the average difference between the absorbed photon energy andthe energy of an electron hole pair) of an e−–h+ pair is not included in H because onlythermalised electrons and holes are considered to be part of the system. This means that thethermalisation energy transfer is directly from the photons to the lattice, both of which arepart of the environment here.
52
the environment (G) more clear. In situations where RR is of interest, it willbe accounted for explicitly by writing R+RRad.
2.5.1 The entropy source term qs
Now that the role of the other source terms is clear, it is time to obtain anexpressions for qs and for Js and to interpret their meaning. Deriving them isdone by combining the local form of the first law Eq. (2.33) with the continuityequations (2.34). The former is used to obtain ∂s/∂t:
∂s
∂t=∂s
∂u
∂u
∂t+∂s
∂n
∂n
∂t+∂s
∂p
∂p
∂t(2.37)
= β∂u
∂t− ηn
∂n
∂t− ηp
∂p
∂t. (2.38)
Next, the continuity equations are used to eliminate all ∂/∂t:
qs −∇ · Js = β (qu −∇ · Ju)− ηn (qn −∇ · Jn)− ηp (qp −∇ · Jp) (2.39)
The next step is to push β and ηn,p inside of the divergences by using theproduct rule f∇ ·w = ∇ · (fw)−w · ∇f . This gives:
qs −∇ · Js = βqu − ηnqn − ηpqp + Ju · ∇β − Jn · ∇ηn − Jp · ∇ηp−∇ · (βJu − ηnJn − ηpJp) . (2.40)
At this point there are two methods that are commonly used in literatureto obtain expressions for qs and Js. Lindefelt [14], for example, proceeds bypostulating that:
TJs = JQ = Ju − ηnJn − ηpJp, (2.41)
with JQ the heat flow. This definition of Js appears to be motivated by Eq.(2.33) and seems reasonable, but there is no clear argument why Eq. (2.41)necessarily follows from Eq. (2.33) since flows are not a type of differential.The advantage of postulating (2.41) is that qs then follows immediately fromEq. (2.40):
qs = βqu − ηnqn − ηpqp + Ju · ∇β − Jn · ∇ηn − Jp · ∇ηp. (2.42)
Another convenient form for the entropy source term is obtained by replacingJu with JQ using Eq. (2.41):
Tqs = qu − ηnqn − ηpqp − JQ ·∇TT− Jn · ∇ηn − Jp · ∇ηp. (2.43)
The second method to obtain Eqs. (2.41) and (2.42) is found in, e.g., the bookby De Groot and Mazur [3]. Here it is asserted that in Eq. (2.40) the parts
53
inside of the divergence have to be equal (yielding Eq. (2.41)) as well as theparts outside of the divergence (yielding Eq. (2.42)). The authors assert thatthis split of Eq. (2.40) is uniquely determined by two additional requirements,namely that of Galilei invariance and the requirement that qs becomes zerowhen global thermodynamic equilibrium is reached. This assertion is madewithout proof, however, so it remains unclear which method is the best tojustify Eqs. (2.41) and (2.42). Fortunately, this does not mean that the accuracy of these equations is in serious doubt, since there are also works thatderive very similar results from microscopic principles (see, e.g., Parrot [13]and Greulich [11]).
2.5.2 Loss processes in the bulk of a solar cell and the entropygeneration rate
Having derived qs in Eq. (2.42), it is time to discuss its physical meaning. Aswas stated earlier, the entropy source term can be split up into two differentcontributions: entropy that is transferred from the environment (i.e., the sunlight) to the cell qs,env→cell and entropy that is generated due to irreversibleprocesses qs,irr. The irreversible contribution can again be split up into entropy generation due to (nonradiative) recombination and due to transportphenomena. According to the second law of thermodynamics, irreversible processes always generate net entropy, even locally. Thus, the entropy source termfor the solar cell qs can be written as:
qs = qs,env→cell + qs,irr, (2.44a)
qs,env→cell = βqu − (ηn + ηp)G, (2.44b)
qs,irr = qs,rec + qs,trans ≥ 0, (2.44c)
qs,rec = (ηn + ηp)R ≥ 0, (2.44d)
qs,trans = Ju · ∇β − Jn · ∇ηn − Jp · ∇ηp ≥ 0. (2.44e)
It was discussed in Section 2.3 that the creation of entropy goes at the costof useful work that can be extracted from the cell, making the entropy sourceterm a useful tool for understanding loss processes. However, it is importantto keep in mind that neither of the terms qs and qs,irr are equal to the totalentropy production rate in the complete photovoltaic process, since there is alsoan entropy source term associated with the photon field, which will be referredto as qs,γ (with γ referring to photons). Due to the unilateral treatment ofthe interaction of photons with the cell, this term remained outside of thescope of the discussion, but of course it does matter in the greater scheme.The exact form of qs,γ can be deduced from the entropy formula for radiationpresented by Landsberg (Eq. (5.6) in his article [19]) and depends on thespectral shape of the radiation field (which varies throughout the cell) and onthe angular distribution of the photon propagation directions. So, for example,
54
a collimated laser beam has a very low entropy because it has a very lowspread in both energy and angular distribution. Sunlight is also wellcollimatedbut has a large spread in its photon energy distribution and therefore also alarger entropy. There is generally no entropy generation associated with the(reversible) propagation of light through a refractive medium, so if all lightpropagation in the cell is reversible then all contributions to qs,γ are due toabsorption and emission of photons. Irreversible (i.e., nonrefractive) scatteringof light, such as Rayleigh scattering and scattering with free electrons, can alsoincrease the entropy of the photons by increasing the angular spread of theradiation [1]. These scattering contributions can be included in qs,γ as well, ifnecessary.
Usually qs,γ is negative because the light field is transferring energy to thesolar cell, though it can be positive if there is locally more radiative recombination than absorption or if the light is being irreversibly scattered. Furthermore,the loss of entropy from the radiation field due to loss of energy qs,γ does notnecessarily cancel against the gain in entropy in the cell due to absorption (oremission) of energy βqu. Only if the transfer of energy between the cell andthe radiation field is reversible (which is usually not the case) are these termsequal and opposite. In this work, the symbol σirr will be used to indicate thetotal entropy production rate in the combined system “solar cell + photons”.The second law states that the total entropy production rate is always largerthan zero:
σirr = qs + qs,γ +RRad(ηn + ηp)
= qs,γ + βqu + β∆ηeh(R+RRad −G)
+ JQ · ∇β − βJn · ∇ηn − βJp · ∇ηp ≥ 0. (2.45)
Recall the convention to mention RRad explicitly when necessary. The terms inEq. (2.45) capture all local loss processes that can occur in the bulk of a solarcell. No exact form for qs,γ will be given or used here, but some general considerations about the role of qs,γ in solar cell design are in order and these arepresented below. In particular, it will be motivated why qs,γ is ultimately notof great importance for the optimisation of many types of solar cells, especiallythose based on cSi. To see why this is the case, it is important to understandthe physical meaning of the entropy generation processes and what possiblepractical methods are available to reduce the corresponding losses. To put itin different words: for the purpose of solar cell optimisation it is unnecessaryto consider entropy generation terms that belong to loss processes one is notwilling to (or incapable to) address anyway.
The bulk losses can be categorised and interpreted as follows:
Generation related losses. These are losses associated with the absorptionof photons and the production of e−–h+ pairs. The most important loss
55
in a cSi cell is of course the thermalisation of an e−–h+ pair directly afterthe absorption of a photon with energy ≥ EG. The entropy generationassociated with thermalisation loss is β(qu − ∆ηehG). In practice, themost feasible method to reduce thermalisation losses is to increase theproduct ∆ηehG as much as possible. This can be achieved by lettinggeneration take place in parts of the cell with a large Fermi level splittingand by building multijunction cells with different bandgaps for eachjunction. Note that the benefit of increasing EG is that this also increases∆ηeh. Often, great emphasis is put on the value of EG, but ultimately itis the free energy per e−–h+pair ∆ηeh that determines how much usefulenergy can be extracted per absorbed photon. For illustration, recall thatfor an electronhole gas satisfying MaxwellBoltzmann statistics ∆ηeh isgiven by:
∆ηeh = EG + kBT ln
(np
NCNV
), (2.46)
which not only shows that ∆ηeh increases with EG, but also that otherquantities matter just as well. Indeed, it is even possible to increase ∆ηehby using materials with low NC and NV as was also noted by Osterloh[26]. Since NC,V ∼ (m∗n,p)
3/2, this means that it is beneficial to usematerials with a low effective mass.
The term qs,γ contains generation related contributions that depend onthe angular distribution of the photon propagation directions and thespectral distribution of the photon energies. Those contributions basically characterise how well the photon field can be trapped inside of thecell to absorb as much of the incident light as possible. In the design ofa solar cell this problem is usually optimised beforehand and separatelyfrom the electrical design. Thus, considering qs,γ becomes importantonce the solar cell has been improved so extensively that disjointed optimisation of optical and electrical design can no longer yield any gains.Some of the optimisations that are possible by considering qs,γ are highlyacademical, though. For example, it is possible to redirect photons emitted from the cell (through thermal radiation or radiative recombination)back towards the sun as much as possible. This way, the lifetime of thesun is extended and more solar energy can be extracted in the long run(see also Wurfel [1] section 2.5). Of course such an optimisation schemeis not very interesting in practice. This should help to illustrate that forsolar cell engineering it is not necessary to consider every entropy generation contribution imaginable and that one should always consider thephysical content of the loss terms one is trying to reduce. An interestingdiscussion of optical design principles is presented by Polman [27].
Recombination related losses. Nonradiative recombination is accounted
56
for by the product ∆ηehR and since it is undesirable to reduce ∆ηeh thisjust means that the total recombination over the whole cell
Rtot =y
x∈Ω
R dx3, (2.47)
needs to be kept as low as possible to reduce the total entropy generation associated with recombination. This is achieved by reducing thenumber of recombinationactive defects (i.e, making the integrand of Rtot
smaller) and by keeping the cell as thin as possible (i.e., making the integration domain Ω smaller). The entropy generation due to RR requiressome extra consideration since this process makes positive contributionsto the terms qs,γ and β∆ηehRRad while giving a negative contribution toβqu (since energy is ejected from the cell). Because of this, the entropygeneration due to RR is usually lower than due to other recombinationprocesses. The physical reason for this is that the photons emitted dueto RR have a welldefined energy which makes it possible to use specialoptical tricks (energyselective mirrors etc.) to keep them inside of thecell. However, it is still a spontaneous process, so the total contributionto all three terms together has to be ≥ 0. This example further illustrates how the practical limitations can influence the interpretation ofloss processes: if one is not considering to use special optical techniquesto capture photons from RR, then for the optimisation of the cell it isunnecessary to consider the entropy generation terms corresponding toRR.
The remaining loss terms JQ · ∇β, −βJn · ∇ηn, and −βJp · ∇ηp are thetransport losses and they will be the subject of Section 2.6 below.
2.6 The thermodynamic formulation of solar cellphysics step 4: Onsager theory
So far no specific mathematical form has been given for the currents Js, Ju,Jn, and Jp. As was briefly alluded to in Section 2.4, the NETGM view of flowsis that they always arise from gradients in local intensive variables: temperature gradients drive heat flows; pressure gradients drive mass flows; gradientsin chemical potential cause diffusion etc.10 Interestingly, in SCP a commonviewpoint is that diffusive flows are driven by gradients in density (which is,from a thermodynamic point of view, a local extensive variable) rather than
10In fact, the idea that gradients in thermodynamic quantities drive flows is a useful startingpoint to separate the interesting transport phenomena from trivial ones such as uniformmotion of the whole system.
57
chemical potential. The diffusive flow Jdiffn of electrons (with density n) is
given in Fick’s law:
Jdiffn = −Dn∇n, (2.48)
with Dn the diffusion constant. If the current is considered to be driven by thechemical potential µc
n, however, the expression should be written instead as:
Jdiffn = −σn
e2∇µc
n. (2.49)
If the electrons are considered to be an ideal gas, then µcn = kBT ln(n/NC) (see
also Eqs. (A.3) in Appendix A.1) and:
Jdiffn = −µnn
e∇[kBT ln
(n
NC
)]= −kBT
eµn∇n. (2.50)
The motivation for writing the proportionality constant as a conductivityσn = eµnn is that ∇µc
n is a force (unit: N) just like ∇φ and it is commonpractice to write currents driven by forces as “mobility × density × force”.Note that the two rightmost expressions in Eq. (2.49) are only valid whenthe electrons can be described by Boltzmann statistics and when T and NC
are constant. Indeed, these are crucial assumptions for the validity of Fick’slaw as well. By comparing Eqs. (2.48) and (2.49) the wellknown Einsteinrelation Dn = µnkBT/e is obtained, demonstrating that µn in Eq. (2.49) isthe familiar carrier mobility from SCP. Usually the Einstein relation is derivedby comparing diffusion to another flowdriving force such as gravity, but thisis not strictly necessary: all that is needed is to identify the chemical potentialas the driving force of diffusion.
In NETGM the gradients of intensive variables that drive flows are called“thermodynamic forces” or “generalised forces”. In some works (such as LeBellac [28]) those two terms are already reserved for other quantities and thennew jargon is introduced by the author (“affinities”, for example), but in thiswork the terminology based on forces is used throughout because this expressesthe central idea most intuitively. When the context is clear the thermodynamicforces will simply be referred to as forces for brevity.
The identification of the right thermodynamic forces and the flows is nottrivial if one has to do this based on first principles, but fortunately NETGM hasa standard procedure for obtaining the correct fluxforce pairs (and the transport relations between them) from the entropy generation rate. The methodis based on the work by Lars Onsager [20] and on Einstein fluctuation theory[29] but the details of those works will not be discussed here. The main resultcan be summarised as follows as follows:
1. First an expression for the irreversible entropy generation rate in thesemiconductor (qs,irr) is written out. As was shown in Section 2.5 there
58
are various possible forms for qs,irr that can be obtained by substitutions,such as:
qs,irr = (ηn + ηp)R+ Ju · ∇β − Jn · ∇ηn − Jp · ∇ηp, (2.51)
or:
qs,irr = β∆ηehR− JQ ·∇TT 2− Jn · β∇ηn − Jp · β∇ηp. (2.52)
Both of these expressions can be used, resulting in different fluxforcepairs. Of course, the different choices for qs,irr lead to equivalent thermodynamic descriptions of the fluxes in the solar cell, though there often isa practical preference for a particular expression for qs,irr. In this case itwill turn out that Eq. (2.52) is more convenient to work with than Eq.(2.51).
2. From each term in qs,irr a fluxforce pair of the form Ji · Fi is identified,so the terms in Eq. (2.51) yield the pairs:
Ju ↔ Fu = −∇TT 2
= ∇β, (2.53a)
Jn ↔ Fn = −∇(βηn), (2.53b)
Jp ↔ Fp = −∇(βηp). (2.53c)
Alternatively, one can identify from Eq. (2.52) the pairs:
JQ ↔ FQ = −∇TT 2
= ∇β, (2.54a)
Jn ↔ Fn = −β∇ηn, (2.54b)
Jp ↔ Fp = −β∇ηp. (2.54c)
As can be seen, care should be taken with the symbols Fn,p: dependingon the form of qs,irr that is used the forces take different forms. For therest of Section 2.6 the forces FQ,n,p from Eqs. (2.54) will be used becausethey have the advantage that the inverse temperature β does not appearunder the gradient in Fn,p.
The perceptive reader may have observed that the term β∆ηehR has notbeen discussed here. Indeed, associated with this term are the scalar fluxR and the scalar force β∆ηeh, but these can be ignored for now and willbe discussed in Section 2.7.
3. Finally, Onsager’s theory asserts that the fluxes (measured in the reference frame of the cell) can be written as a general linear combination of
59
the forces. The coefficients in this linear combination are denoted by thesymbols Lij with i and j labelling the fluxes and forces:
JQ = LQQFQ + LQnFn + LQpFp, (2.55a)
Jn = LnQFQ + LnnFn + LnpFp, (2.55b)
Jp = LpQFQ + LpnFn + LppFp. (2.55c)
These equations can be stated more compactly as:
Ji =∑j
LijFj (2.56)
It should be noted that these equations are valid for transport in anisotropic system. In Section 2.7 the consequences and limitations of thisassumption will be analysed, but for now the assumption of isotropy willbe used to simplify the discussion.
In Eqs. (2.55), the diagonal terms LQQFQ, LnnFn, and LppFp accountfor well known transport phenomena such as heat diffusion due to atemperature gradient (i.e., Fourier’s law) and charge transport due togradients in the electrochemical potentials. The offdiagonal elementslike LQnFn account for effects such as the Peltier effect whereby heatis transported along with the flow of electrons. The crossterms LnpFpand LpnFn represent momentum exchange between electrons and holesdue to microscopic collisions [14] arising from shortrange interactionsbetween electrons and holes that are quantum mechanical in nature. Forexample, at close proximity an electronhole pair can temporary forman exciton, which is a quantum mechanical state similar to that of thehydrogen atom (i.e., a bound state between two oppositely charged particles). During this binding the two particles can exchange momentumand in this manner the electrons can exert a shortrange force on theholes and vice versa. Macroscopically this force then gives rise to theoffdiagonal transport terms LnpFp and LpnFn. It is expected that thiseffect becomes stronger in materials with a strong exciton binding energy, which are usually materials with a low dielectric constant (see, e.g.,Ibach and Luth [30]) such as polymers. The effect of these shortrangeinteractions should be distinguished from the long range Coulombic interactions between electrons and holes in a solar cell that are accountedfor by the electrostatic potential φ (which modifies ηn,p and Fn,p) andthe Poisson equation (see Eq. (A.1) in Appendix A.1).
Due to the linear form of Eqs. (2.55) it is sometimes said that NETGM
is a linear theory, but care should be taken when interpreting this statementbecause NETGM only asserts that the fluxes are always linear in the forces,(meaning that the Lij cannot depend on the FQ,n,p). However, the coefficients
60
Lij are not necessarily constant: they can depend on other thermodynamicquantities such as T , ηn,p, n, p and on x explicitly. For example, the electronelectrical conductivity and Lnn can be related as Lnn = Tσn/e
2 = Tµnn/e,so Lnn is not constant. When Eqs. (2.55) are inserted into the continuityequations Eqs. (2.34), the resulting transport equations are therefore generallynonlinear11.
The fluxforce equations (2.55) can be used to rewrite the transport dissipation term qs,trans from Eqs. (2.44):
qs,trans = JQ · FQ + Jn · Fn + Jp · Fp (by definition of the forces)
=∑j
(LQjFj · FQ + LnjFj · Fn + LpjFj · Fp
)=∑i,j
LijFi · Fj ≥ 0. (2.57)
The inequality qs,trans ≥ 0 immediately imposes a constraint on the coefficientsLij : since the Lij are independent of the forces Fj , the inequality qs,trans ≥ 0has to hold for every possible combination of forces FQ, Fn, and Fp. This isonly possible if the elements Lij form a positivedefinite matrix, meaning thatall of its eigenvalues are positive. Consequently, the diagonal elements LQQ,Lnn and Lpp are all positive as well. The offdiagonal elements can be negative,but their absolute values are bounded. For example, a simple bound for theelements Lnp and Lpn is given by:
4LnnLpp ≥ (Lnp + Lpn)2 . (2.58)
In Section 2.7, the Onsager relations are discussed and these require that Lnp =Lpn, so that LnnLpp ≥ L2
np. The offdiagonal coefficients have a significantinfluence on the transport losses that occur in the cell. To illustrate this,consider for the moment only the dissipation due to the electron and holeforces in a 1D solar cell. For simplicity it is assumed that FQ = 0. Thereis a total charge current Jcharge = e(Jp − Jn) running through the cell andthen the problem is to find the ideal values of Fn,p for a given set of transportcoefficients. This optimum is found by solving a constrained minimisationproblem for qs,trans. Using the method of Lagrange multipliers, the followingquantity Λ is minimised with respect to Fn, Fp, and the multiplier λ:
Λ = qs,trans + λ
[Jcharge
e− (Jp − Jn)
]= LnnF
2n + LppF
2p + 2LnpFnFp
+ λ
[Jcharge
e− (LppFp + LnpFn − LnnFn − LnpFp)
]. (2.59)
11see also the remarks from the authors in preface to the Dover edition of their work [3].
61
By setting ∂Λ/∂Fn = ∂Λ/∂Fp = ∂Λ/∂λ = 0 and solving, the following solutionis obtained:
Fp = −Fn =Jcharge/e
Lnn + Lpp − 2Lnp, (2.60)
qs,trans =(Jcharge/e)
2
Lnn + Lpp − 2Lnp. (2.61)
This shows that the ideal way to drive a current Jcharge is by making surethat the electron and hole forces are equal and opposite. Recall that Lnn ≥ 0and Lp ≥ 0, so due to the constraint LnnLpp ≥ L2
np the entropy production isalways positive. As can be seen, qs,trans is smaller for materials with greaterLnn and Lpp because those materials that are more conductive. Furthermore,the entropy production is lower for materials where Lnp < 0 than for those withLnp ≥ 0. The physical reason is that whenever Lnp < 0, the electron force Fnpushes the holes in the opposite direction and vice versa, thereby facilitatingcharge separation. To put it differently: the electron force is helping the holesand the other way around. Since the entropy generation terms are Jn ·Fn andJp · Fp, it is beneficial to drive the electron current Jn towards its collectingcontact by forces other than Fn (and vice versa). Conversely, when Lnp > 0the electrons and holes tend to be transported together in the same direction,making the photovoltaic conversion less efficient. Indeed, it is known that thiscodirectional transport of electrons and holes is one of the limiting factors inorganic solar cells. For a material in which Lnn = Lpp and that achieves thethermodynamically allowed limit Lnp = −
√LnnLpp, the reduction of charge
transport losses can be up to 50 % compared to Lnp = 0. This demonstratesthat both the diagonal and the offdiagonal transport coefficients can have asignificant influence on the rate of entropy production.
Traditionally, the SCP description of solar cells does not consider the offdiagonal transport coefficients Lnp and Lpn. Presumably, the error that occursfrom this (implicit) assumption is not severe given the success with whichSCP can model photovoltaic devices. However, this does not necessarily meanthat Lnp = Lpn = 0, since it is always possible to transform Eqs. (2.55) toa diagonal form (i.e., through diagonalisation of the matrix Lij). By doingso, the effects of Lnp and Lpn are incorporated into Lnn and Lpp (i.e., theelectron and hole conductivities). However, the diagonalisation of Lij alsomuddles the distinction between electrons and holes and this has repercussionsfor other empirical models such as the expression for the recombination rateand the mobility. It is therefore worth exploring whether greater accuracy andmathematical and/or physical simplicity can be achieved for these empiricalmodels when the offdiagonal transport coefficients Lnp and Lpn are explicitlyincorporated in the transport equations.
Conversely, offdiagonal transport coefficients can also arise when a changein variables is made to a transport problem that was originally diagonal. Such
62
a transformation of fluxes and forces can sometimes provide advantages thatweigh up against the added complexity of having a more complicated matrix oftransport coefficients. As an example, it is possible to transform the electronand hole currents Jn,p to the current of electronhole pair Jeh = 1/2(Jn + Jp)and the charge current Jc = Jp−Jn. This is exactly analogous to the situationin Section 2.3 (Eqs. (2.5) and (2.7)) where one can choose between using thenumbers of electrons and hole (Nn and Np) as thermodynamic variables or,instead, the number of electronhole pairs (Neh) and the electronhole charge(Qnp). The advantage of this transformation is, of course, that the chargecurrent has no source term (i.e., ∇ · Jc = 0) since charge is always conserved.The accompanying forces for Jeh and Jc are:
Jeh ↔ Feh = −β∇∆ηeh = −β∇(ηn + ηp), (2.62a)
Jc ↔ Fc = −β∇ΦQ =β
2∇(ηn − ηp). (2.62b)
It can be verified that these are indeed correct fluxforce pairs since:
Jeh · Feh + Jc · Fc = Jn · Fn + Jp · Fp, (2.63)
which demonstrates that the change in variable from Jn and Jp to Jeh andJc (along with the correct change in forces) leaves the irreversible entropygeneration rate (Eq. (2.52)) invariant. Now suppose that the original transportmatrix for Jn and Jp is diagonal so that Jn = LnnFn and Jp = LppFp. It canthen be readily verified that the transport matrix for Jeh and Jc is not, sincesome algebra demonstrates that the Onsager relations for the new fluxes are:
Jeh =Lnn + Lpp
4Feh +
Lpp − Lnn2
Fc, (2.64a)
Jc =Lpp − Lnn
2Feh + (Lnn + Lpp)Fc. (2.64b)
Thus, the convenience of having a flux with zero divergence should be contrasted against the inconvenience of have more complicated fluxforce relations.
Finally, it should be noted that in various literature sources a theorem calledthe principle of minimum entropy generation is frequently mentioned. It willnot be discussed in detail here, but it is worth mentioning that this theoremdoes not apply to solar cells. This is because a critical condition for the validityof the minimum entropy generation principle is that the transport coefficientsLij are true constants (i.e., independent of thermodynamic variables like n andp as well as x) [3]. This condition is not fulfilled in the case of solar cells sothe theorem can be disregarded.
63
2.7 The thermodynamic formulation of solar cellphysics step 5: Symmetry, the Onsager reciprocal relations and the Curie principle
The transport coefficients Lij are purely empirical from a macroscopic point ofview, so to specify them further one either has to measure them; calculate themfrom microscopic theory; or make adhoc assumptions about them. Typicaltheoretical tools that can be used to link the Lij to microscopic phenomenalike collisions include the Boltzmann transport equation, Kubo formalism, andfluctuation theory. The books by De Groot [3] and Le Bellac [28] are among thesources that can be referred to for more details on the microscopic descriptionof the transport coefficients.
However, even without microscopic models for the Lij it is possible to obtainsome important universal results for the transport coefficients. For example,in Section 2.6 it was already mentioned that the Lij have to form a positivedefinite matrix because entropy cannot decrease. Recall from Section 2.3 thatthermodynamics is a theory about symmetries of the underlying microscopicphysics of a system and here in Section 2.7 two important symmetries alongwith their consequences for the transport coefficients will be discussed, namelytimereversal symmetry and material isotropy.
2.7.1 The Onsager reciprocal relations
Time reversal symmetry is a fundamental property of all microscopic laws thatultimately govern the behaviour of everyday macroscopic objects. Newton’slaws of motion, Maxwell’s laws of electromagnetic fields and quantum mechanics are all symmetric under the reversal of the flow of time. In some casesone has to transform certain quantities when time is reversed (e.g., magneticfields get a minus sign when time is reversed) but ultimately it is not possible to distinguish the forward and reverse directions of time flow based onmicroscopic physics: only on the macroscopic scale is there a clear breaking ofsymmetry that manifests itself as the second law of thermodynamics12. Themicroscopic time reversal symmetry has interesting macroscopic consequencesthat are known as the Onsager reciprocal relations. Applied to a solar cell,these relations state that the matrix of the transport coefficients is symmetric,
12Even though much work has been devoted to explaining how microscopically reversiblelaws can give rise to macroscopically irreversible phenomena, this question is still an activetopic of debate and will not be discussed here since it is far beyond the scope of the currenttext.
64
i.e.:
LQn = LnQ, (2.65a)
LQp = LpQ, (2.65b)
Lnp = Lpn, (2.65c)
or simply Lij = Lji. This result may seem surprising at first. The scepticalreader is advised to verify that, e.g., the coefficients LQn and LnQ have thesame units before accepting that they are, in fact, equal. The Onsager relationspresent an important link between phenomena that superficially appear unrelated such as the Peltier effect and the Seebeck effect. The derivation of thereciprocal relations will not be given here; it can be found in various literaturesources [20, 3]. However, it is possible to gain some heuristic understandingof the reciprocal relations by considering that time reversal also reverses causeand effect. If one would assert that a flow of electrons Jn causes a flow of heatJQ along with the electrons (Peltier effect), then the principle of timereversalsymmetry states that it is equally valid to assert that a flow of heat JQ causesa flow of electrons Jn (Seebeck effect). In other words, the reciprocal relationsexpress the idea that, macroscopically, it is impossible to distinguish whichof the two phenomena is the cause and which is the effect. It should be emphasised that the principle of time reversal symmetry does not imply that theflows JQ, Jn, and Jp are reversible: macroscopic flows generate entropy andare therefore always irreversible.
2.7.2 The Curie principle
The Curie principle (named after Pierre Curie) is the general idea that asymmetric system cannot give rise to phenomena that break the symmetries ofthe original system. For example, a gas in a container is completely isotropicin every direction and therefore it will conduct heat in the same way regardlessof the direction of the heat current. In other words, if the heat conduction isdescribed by Fourier’s law JQ = −(LQQ/T
2)∇T from Eqs. (2.55), then LQQhas to be a scalar constant for the gas rather than a tensor. The Curie principleis a useful concept, but it has limitations. A good example of a violation ofthe Curie principle is (ironically) the cooling of a ferromagnet from aboveits Curie temperature Tc to below. At T > Tc, the magnet is completelyisotropic (or at least has a highly symmetrical crystal structure). Yet once itis cooled to T < Tc, the symmetry of the system spontaneously breaks and thematerial develops a net magnetisation M . In more general it can be said thatphase transitions can give rise to broken symmetries in otherwise completelysymmetric systems, so care should be taken when applying the Curie principlewhen phase transitions can occur. Fortunately, this is not a very importantlimitation in solar cell physics.
65
Most parts of a solar cell (such as the bulk of a cSi wafer) are to goodapproximation isotropic and it is therefore instructive to review what consequences this isotropy has on the macroscopic physics of the device. This way,one can also appreciate what kind of special phenomena can be expected inparts of the device where the isotropic symmetry is broken. While formulatingthe fluxforce equations Eqs. (2.55) it was already assumed that the system isisotropic to simplify the discussion, because for a nonisotropic system significantly more terms are needed in Eqs. (2.55). To understand why, recall thatthe fluxforce pair in Eqs. (2.54) were obtained from the terms that occur inthe irreversible entropy generation rate qs,irr. In Section 2.6, qs,irr was suggestively written out in vector form, but is of course also possible to expand theinner products in Cartesian components as follows:
qs,irr = β∆ηehR− JQ · ∇β − Jn · β∇ηn − Jp · β∇ηp
= β∆ηehR− JQ,x∂β
∂x− JQ,y
∂β
∂y− JQ,z
∂β
∂z
− Jn,xβ∂ηn∂x− Jn,yβ
∂ηn∂y− Jn,zβ
∂ηn∂z
− Jp,xβ∂ηp∂x− Jp,yβ
∂ηp∂y− Jp,zβ
∂ηp∂z
. (2.66)
This form of qs,irr suggests that there actually are nine fluxforce pairs relatedto heat and charge transport instead of three. Consequently, there are alsonine fluxforce relations with nine terms in each equation instead of the threeterms shown in Eqs. (2.55). This means that strictly speaking, each of thecoefficients Lij in Eqs. (2.55) is actually a second order tensor rather than ascalar. For clarity, tensors will be denoted in roman symbols as:
Lij =
Lxxij Lxyij LxzijLyxij Lyyij LyzijLzxij Lzyij Lzzij
. (2.67)
The Onsager reciprocal relations for these tensors are:
Lij = LTji, i, j ∈ Q,n, p, (2.68)
where T denotes the transpose operation. Note that Eq. (2.68) also impliesthat LQQ, Lnn and Lpp are always symmetric.
The reason it is possible to reduce the tensors Lij to scalars Lij is the Curieprinciple: if the system does not exhibit broken symmetry between the threeCartesian directions, then neither should the transport equations. In fact, itis not even completely necessary for the system to be completely isotropic:even in a system that only has cubic symmetry (which is a common symmetrytype for many crystals, such a cSi) the tensorial transport coefficients still
66
reduce to scalars and for the purposes of this text cubic symmetry can beconsidered equivalent to complete isotropy. In the works of GM and Kuiken,general mathematical methods are given that can reduce the complexity of thetransport coefficients for any given type of symmetry of the system [3, 16].
However, the Curie principle does more than just assert that the fluxforcerelations are isotropic. At this point the reader is asked to recall from Section2.6 that qs,irr in Eq. (2.52) also has the term β∆ηehR that yields the scalarfluxforce pair R ↔ β∆ηeh. Since β∆ηeh is a thermodynamic force, it shouldalso be able to drive the currents JQ,n,p. In other words, in Eqs. (2.55) thefollowing terms are also expected:
JQ = ...+LQR β∆ηeh, (2.69a)
Jn = ...+LnR β∆ηeh, (2.69b)
Jp = ...+LpR β∆ηeh. (2.69c)
As can be seen, the transport coefficients LQR, LnR, and LpR are necessarilyvectors since they relate the scalar force β∆ηeh to the vectorial fluxes JQ,n,p.Conversely, there should also be a fluxforce relation for the scalar flux R:
R = LRQ · FQ +LRn · Fn +LRp · Fp + LRRβ∆ηeh. (2.70)
Again, the coefficients LRQ, LRn, and LRp have to be vectors, since the innerproduct is the only way to make a general linear transformation from thevectorial forces FQ,n,p to the scalar flux R. Of course, there are also Onsagerrelations for the vectorial transport coefficients LiR and LRi that have beenintroduced just now:
LQR = LRQ, (2.71a)
LnR = LRn, (2.71b)
LpR = LRp. (2.71c)
The cross effects between recombination and transport in Eqs. (2.69) and(2.70) were not mentioned in Section 2.6 because these cross phenomena donot occur in an isotropic medium. This is again a consequence of the Curieprinciple: in an isotropic system no preferential direction can exist, so thevectors like LQR and LRQ have to be zero since they are material properties.In other words it can also be said that in an isotropic medium the scalar forceβ∆ηeh cannot drive a vectorial current since there is no direction the currentcan be forced towards.
In conclusion, for a fully nonisotropic system, it is necessary to generalise
67
Eqs. (2.55) to:
JQ = LQQFQ + LQnFn + LQpFp +LQR β∆ηeh, (2.72a)
Jn = LnQFQ + LnnFn + LnpFp +LnR β∆ηeh, (2.72b)
Jp = LpQFQ + LpnFn + LppFp +LpR β∆ηeh, (2.72c)
R = LRQ · FQ +LRn · Fn +LRp · Fp + LRRβ∆ηeh. (2.72d)
Here it is understood that terms such as LQQFQ represent matrix multiplications. Having compared the isotropic fluxforce relations with the fully nonisotropic form in Eqs. (2.72), it is time to consider what kind of departures fromisotropy can be expected in a solar cell. The first possibility is that the bulkmaterial of the cell itself has an inherent anisotropy due to its crystal structure.However, many materials relevant for solar cells are either amorphous (aSi:H,polymers) or have cubic crystal symmetry and both of these types of materialscan be considered isotropic to a good degree of accuracy. Material isotropywill therefore not be considered in detail. Secondly, and more importantly, theisotropy of the system can be reduced by the presence of electric or magneticfields (see also Kuiken [16] for a detailed mathematical treatment of symmetrybreaking due to electromagnetic fields). It is well known that electric fields arecommonly encountered in solar cells and in, e.g., cSibased cells they can beas strong as 106 V m−1, which is enough to alter the electrical properties of thecrystal. To discuss the macroscopic consequences of such an electric field, it isassumed that the field E is in the z direction (so that E = Ez) in an otherwiseisotropic medium. The tensorial transport coefficients in the general fluxforcerelations in Eqs. (2.72) can then be shown to reduce to the form:
Lij =
L⊥ij 0 0
0 L⊥ij 0
0 0 L‖ij
, i, j ∈ Q,n, p. (2.73)
As can be seen, transport in the plane perpendicular to E is still isotropic,but a different coefficient appears for the transport along E. Furthermore, thevectorial transport coefficients all become scalar multiples of E:
LQR = LRQ = LQRE, (2.74a)
LnR = LRn = LnRE, (2.74b)
LpR = LRp = LpRE. (2.74c)
Heuristically, it can be said that broken symmetry makes it possible to couplescalar and vector processes. Because the electric field is the source of thisbroken symmetry, the transport coefficients LQR, LnR, and LpR that couplethe scalar and vectorial processes have to be codirectional to E. In the firstorder, the prefactors LQR, LnR, and LpR are independent of the strength of E,
68
but for strong electric fields they can become dependent on the field strengthE ·E.
Thus, the broken symmetry due to the electric field can influence the currents of the electrons and holes by the terms:
Jn = ...+ LnREβ∆ηeh, (2.75a)
Jp = ...+ LpREβ∆ηeh. (2.75b)
It should be emphasised again that this contribution is not directly due to theelectrostatic force of the electric field on the charge carriers, since this forceis already accounted for in Fn and Fp in the fluxforce equations. In fact,the electric field does not act like a thermodynamic force at all in this casebut only a factor in a transport coefficient: β∆ηeh is the thermodynamic forcethat drives the current. From a microscopic point of view, the electric fieldcreates an asymmetry between recombination of electrons/holes with different momenta by distorting the recombination potential, as shown an Figure2.2. Thus, if electrons (holes) with a certain momentum are more likely torecombine than those with the opposite momentum, this will macroscopicallyinfluence the current Jn (Jp). The idea that electric fields affect carrier recombination is not new and has been described by microscopic physics (see, e.g.,Schenk [31]). On the other hand, the conclusion that the recombination therefore also acts as a force for Jn,p is not immediately obvious from microscopicphysics (and has not been pointed out before, to the author’s knowledge) whilethis consequence follows in a straightforward manner from a thermodynamicdescription. This illustrates how macroscopic physics can help to illuminatethe consequences of microscopic processes and correlate seemingly unrelatedphenomena. From a pure modeling point of view it is probably more naturalto write the recombination contributions to Jn,p as:
LnRβ∆ηehE = CnRRE, (2.76)
LpRβ∆ηehE = CpRRE, (2.77)
where the coefficients CnR and CnR measure the asymmetry in recombinationprobability between electrons/holes moving with or against the electric fieldE.
Having demonstrated that in the spacecharge region of a solar cell it is possible for crossphenomena to occur between recombination and charge transport, the question arises how this affects the generation of entropy. As wasillustrated in Section 2.6 for the offdiagonal transport coefficients Lnp = Lpn,the understanding of crossphenomena can help to make the device more efficient. When considering the coupling coefficients LnR and LpR, it can be seenthat it would be beneficial to look for materials where LnR ≤ 0 and LpR ≥ 0since in that case the scalar force β∆ηeh will provide extra driving terms forJn,p that guide the electrons and holes to their respective contacts.
69
Figure 2.2: Comparison of the Coulomb potentials of electrons near a hole. In the presenceof an external electric field E the symmetry between electrons moving left and those movingright is broken and one of the two can become more likely to recombine. In the recombinationmechanism described by Schenk [31] (Figure 1 in his article), the electron moving from leftto right in the second image would be the one more likely to recombine.
It is worth mentioning that there is a significant difference between thedescription of (nonradiative) recombination between SCP and NET. In SCP,bulk recombination rates are usually parameterised as:
R = α(np− n2i ), (2.78)
with ni the intrinsic carrier density and α a parameter (not necessarily a constant) that is commonly a polynomial in powers of n and p. The factor (np−n2
i )(which is essentially the exponent of ∆ηeh) occurs naturally to make sure thatR = 0 under equilibrium conditions. With Eq. (2.78) it is possible to conveniently model collisions between two, three or more carriers as terms withvarying powers of n and p. On the other hand, NET prescribes the bulk recombination as a scalar fluxforce relation:
R = LRRβ∆ηeh = LRRkB ln
(np
n2i
), (2.79)
since the remaining terms from Eq. (2.72d) do not occur in the bulk. Thereis no true disagreement between Eqs. (2.78) and (2.79), since the parameterLRR is not necessarily constant and because Eq. (2.79) also yields R = 0under equilibrium. However, the strong nonlinearity of LRR makes Eq. (2.79)less practical for the modeling of recombination than Eq. (2.78). In theirown work, GM already remark that the scalar fluxforce relations for chemicalreactions are often not very useful because of the strong nonlinearity of thecoefficients (LRR in this case) that occur in real systems. This suggests thatstrong deviations from chemical equilibrium often happen in practice. Indeed,the strong nonequilibrium of electrons and holes is precisely what characterisesa solar cell and what allows it to generate power.
70
2.8 Wrap up: what does thermodynamics tell us?
The mathematical formalism of NETGM has strong parallels with that of SCP.Both rely on the continuity equations and use empirical laws for the fluxes.The main difference is that SCP also introduces the Poisson equation for theelectrostatic potential φ and the Boltzmann (or FermiDirac) expressions forthe carrier densities:
n = NC exp
(EFn + φ+ χ
kBT
), (2.80a)
p = NV exp
(−EFp + φ+ χ+ EG
kBT
). (2.80b)
Furthermore, SCP has many detailed models for various transport and recombination phenomena.
There are, however, no limitations to incorporate these elements into NET.The Poisson equation and carrier statistics can be included as auxiliary equations while the transport and recombination models simply prescribe the values of the empirical transport coefficients Lij . This means that any discussionabout solar cells framed in terms of SCP can be translated to NET and viceversa, so that both disciplines can benefit from the strengths of the other. ForSCP, the main enrichments coming from NET are the addition of entropy asa tool for discussing losses of useful output power and the systematic analysisof symmetries (and their consequences) in the system. It would not be anexaggeration to say that SCP actually is a form of nonequilibrium thermodynamics that is often just not recognised as such. By making this link explicit,an invaluable extra level of depth becomes available for the interpretation ofresults and calculations from SCP. Due to its generality, NET can also help toground the mathematical formalism of SCP on fundamental principles and toclarify assumptions that are used in SCP.
Moreover, NET can help to point out phenomena predicted by the empirical transport relations (Eq. (2.55) and (2.72)) that are possibly relevant toinvestigate. Examples are the crosseffects between electron and hole transport (characterised by the coefficient Lnp, see Section 2.6) or those betweencharge transport and recombination (characterised by the coefficients LnR andLpR, see Section 2.7). An important lesson that is learnt from NET, is thatthe discovery of new phenomena (e.g., a new recombination process) also hasconsequences for other physical processes in the cell as predicted by the Onsager reciprocal relations. Finally, NET also demonstrates that the ultimatesolar cell design with the highest possible efficiency can only be achieved if theentropy generation rates in both the cell and the photon field are considered simultaneously since both are an essential in the photovoltaic conversion process(see Section 2.4 and the discussion following Eq. (2.45)). This means that,at some point, the unilateral treatment of the light (which is still prevalent
71
for most solar cell modeling tools) will reach its limits and no further designimprovement can be achieved without switching to a bilateral description ofthe coupling between cell and light.
It can be concluded that there are no arguments left against the use ofthermodynamics in solar cell research: The apparent objections raised at thestart of Section 2.1 can be countered by modern NET and in a sense SCPcan be viewed as a particular application of the work by GM. Nonequilibriumthermodynamics offer tools that are not only useful for academic research aboutthe ultimate efficiency potential, but they can also be combined with SCP toassist the downtoearth engineering of current cell designs.
72
References Chapter 2
[1] Peter Wurfel. Physics of Solar Cells. WileyVCH Verlag GmbH & Co,Weinheim, 2005. ISBN 3527404287.
[2] Uli Wurfel, Andres Cuevas, and Peter Wurfel. Charge Carrier Separationin Solar Cells. IEEE Journal of Photovoltaics, 5(1):461–469, 2015. ISSN21563381. doi: 10.1109/JPHOTOV.2014.2363550.
[3] S.R. de Groot and Peter Mazur. Nonequilibrium Thermodynamics. DoverPublications, Mineola, New York, 1984. ISBN 0486647412.
[4] J.E. Parrott. Theoretical upper limit to the conversion efficiency of solar energy. Solar Energy, 21(3):227–229, 1978. ISSN 0038092X. doi:10.1016/0038092X(78)900257.
[5] A. De Vos and H. Pauwels. On the thermodynamic limit of photovoltaicenergy conversion. Appl. Phys., 25(2):119–125, June 1981. ISSN 03403793. doi: 10.1007/BF00901283.
[6] J.E. Parrott. Thermodynamics of solar cell efficiency. Solar EnergyMaterials and Solar Cells, 25(12):73–85, 1992. ISSN 09270248. doi:10.1016/09270248(92)90017J.
[7] C. H. Henry. Limiting efficiencies of ideal single and multiple energy gapterrestrial solar cells. J. Appl. Phys., 51(8):4494, 1980. ISSN 00218979.doi: 10.1063/1.328272.
[8] Peter Wurfel. Thermodynamic limitations to solar energy conversion.In Physica E: LowDimensional Systems and Nanostructures, volume 14,pages 18–26, 2002. ISBN 13869477.
[9] NilsPeter Harder and Peter Wurfel. Theoretical limits of thermophotovoltaic solar energy conversion. Semiconductor Science and Technology, 18(5):S151–S157, 2003. ISSN 02681242. doi: 10.1088/02681242/18/5/303.
[10] R. Brendel, S. Dreissigacker, N.P. Harder, and P. P. Altermatt. Theoryof analyzing free energy losses in solar cells. Applied Physics Letters, 93(17):173503, 2008. ISSN 00036951. doi: 10.1063/1.3006053.
73
[11] Johannes Greulich, Hannes Hoffler, Uli Wurfel, and Stefan Rein. Numerical power balance and free energy loss analysis for solar cells including optical, thermodynamic, and electrical aspects. Journal of Applied Physics,114(20):204504, 2013. ISSN 00218979. doi: 10.1063/1.4832777.
[12] K.M. Van Vliet. Entropy production and choice of heat flux for degeneratesemiconductors and metals. physica status solidi (b), 78:667, 1976. ISSN03701972. doi: 10.1002/pssb.2220780227.
[13] J.E. Parrott. Transport theory of semiconductor energy conversion. Journal of Applied Physics, 53(12):9105–9111, 1982. ISSN 00218979. doi:10.1063/1.330422.
[14] U. Lindefelt. Heat generation in semiconductor devices. Journal of AppliedPhysics, 75:942–957, 1994. ISSN 00218979. doi: 10.1063/1.356450.
[15] J.E. Parrott. Thermodynamic theory of transport processes in semiconductors. IEEE Transactions on Electron Devices, 43, 1996. ISSN 00189383. doi: 10.1109/16.491259.
[16] Gerard D.C. Kuiken. Thermodynamics of irreversible processes. JohnWiley & Sons, Ltd., Chichester, England, 1994. ISBN 0471948446.
[17] Hans Christian Ottinger. Beyond Equilibrium Thermodynamics. JohnWiley & Sons, Inc., Hoboken, New Jersey, 2005.
[18] Signe Kjelstrup and Dick Bedeaux. NonEquilibrium Thermodynamics ofHeterogeneous Systems. World Scientific Publishing Co. Pte. Ltd., Singapore, 2008.
[19] P. T. Landsberg and G. Tonge. Thermodynamic energy conversion efficiencies. Journal of Applied Physics, 51(7):R1, July 1980. ISSN 00218979.doi: 10.1063/1.328187.
[20] Lars Onsager. Reciprocal Relations in Irreversible Processes. I. Physical Review, 37(4):405–426, February 1931. ISSN 0031899X. doi:10.1103/PhysRev.37.405.
[21] Herbert B. Callen. Thermodynamics and an Introduction to Thermostatistics. John Wiley & Sons, Inc., New York, 2 edition, 1985.
[22] David Chandler. Introduction to Modern Statistical Mechanics. OxfordUniversity Press, New York, 1987. ISBN 019504276X.
[23] Mark Waldo Zemansky and Richard Dittman. Heat and Thermodynamics: An Intermediate Textbook. McGrawHill International Book Company,London, 7 edition, 1997.
74
[24] Eli Yablonovitch and Owen D. Miller. The OptoElectronics of Solar Cells.IEEE Photonics Society News, 27(1), 2013.
[25] E. Velmre. Numerical modelling of semiconductor structures includingelectronhole scattering and recombination radiation recycling effect. Period. Polytech. Elec. Eng., 33(3):141–150, 1989.
[26] Frank E Osterloh. Maximum Theoretical Efficiency Limit of PhotovoltaicDevices: Effect of Band Structure on Excited State Entropy. The Journalof Physical Chemistry Letters, 5(19):3354–3359, October 2014. ISSN 19487185. doi: 10.1021/jz501740n.
[27] Albert Polman and Harry A Atwater. Photonic design principles forultrahighefficiency photovoltaics. Nature Materials, 11(3):174–7, January2012. ISSN 14761122. doi: 10.1038/nmat3263.
[28] Michel Le Bellac, Fabrice Mortessagne, and G. George Batrouni. Equilibrium and NonEquilibrium Statistical Thermodynamics. Cambridge University Press, Cambridge, 2004. ISBN 0 521 82143 6.
[29] A. Einstein. Zur allgemeinen molekularen Theorie der Warme [AdP 14,354 (1904)]. Annalen der Physik, 14(S1):154–163, February 2005. ISSN00033804. doi: 10.1002/andp.200590003.
[30] Harald Ibach and Hans Luth. SolidState Physics. SpringerVerlag BerlinHeidelberg New York, Berlin, Heidelberg, 3 edition, 2003. doi: PhysRevB.83.165113.
[31] A. Schenk. An improved approach to the ShockleyReadHall recombination in inhomogeneous fields of spacecharge regions. Journal of AppliedPhysics, 71(7):3339, 1992. ISSN 00218979. doi: 10.1063/1.350929.
75
76
Chapter 3
The physics of solar cells:semiconductor physicsenhanced by thermodynamics
3.1 The thermodynamics of the selective membranemodel
Chapter 2 and Appendix A.1 review the most important physical equationsthat are needed to describe a solar cell and to predict its efficiency. Theequations, however, are only part of the complete understanding of how asolar cell works and, more importantly, how it can be improved. The set ofequations that describes the charge transport in a cell is highly nonlinear andeven solving numerically on a computer is not entirely straightforward. In asense, the transport equations only replace the problem of understanding thesolar cell with another (not necessarily easier) problem: that of understandingthe mathematics underlying the equations. It is no surprise then, that differentconcepts and simplifications have been developed to understand solar cells ona more heuristic level, such as the selectivemembrane concept by P. Wurfel[1] and U. Wurfel [2]. Indeed, such simplifications are of crucial importanceto the field of PV (and science in general) because they make the exchange ofideas between people more efficient.
The goal of this section is therefore to present and justify a heuristic description of solar cells that uses NETPV from Chapter 2 as the main physicallanguage. First, the selectivemembrane concept as developed by P. Wurfelwill be presented briefly and will then be used as the main motivation for thethermodynamic discussion that follows.
77
3.2 The selective membrane model
A typical singlejunction solar cell consists of three parts that are essential forthe operation of the device: a photon absorber (or just absorber for short)which forms the centre of the cell and two selective membranes (one for electrons and one for holes) that are located between the absorber and the metalcontacts. The function of the absorber is to convert the incoming light intouseful work in the form electrochemical free energy, meaning that the photonabsorber has to be good at converting light into free charge carriers and alsoat sustaining the resulting electronhole plasma. The function of the selectivemembranes is to ensure that the electrochemical energy generated in the absorber is transported out of the cell as efficiently as possible in the form ofelectrical current. The selective membranes are highly conductive to one typeof carrier and highly resistive to the other type. A membrane that allows electrons (holes) to pass while blocking holes (electrons) is called an electron (hole)membrane or an n–membrane (p–membrane). The combination of a selectivemembrane plus metal contact is referred to as a selective contact. Due to thelarge asymmetry in the electron and hole conductivities between the two different selective membranes, electrons and holes are much more likely to exit thecell through their respective contacts (see Figure 3.1). It is important to notethat the selective contacts are ideally completely transparent to light so thatthere is no charge carrier generation inside of them. Heuristically, the reasonfor this is that holes generated in the middle of the n–membrane in Figure 3.1encounter approximately the same resistance in the path towards the electroncollecting contact as in the path towards the bulk of the cell (and ultimatelythe p–contact). Thus, holes generated in the selective contact are likely to becollected by the wrong electrode, leading to current loss. This phenomenon isknown as parasitic absorption and it will be discussed in more detail in Section3.6.
As can be seen, the concepts of conductivity and resistivity are key to theunderstanding of selective membranes and one of the goals of this chapter isto give these heuristic concepts a quantitative basis that is straightforward tointerpret. To do so, it is useful to first consider the most common type of solarcell, namely the doped homojunction where the absorber and the selectivemembranes consist of the same material. To create the selective membranes,a high doping concentration is used to drastically increase the conductivity ofone type of charge carrier. In Figure 3.2 the band diagram of a p–contact andpart of the photon absorber of the cell is shown. For simplicity, the cell underdiscussion is assumed to be 1D. The band diagram (as well as all the otherdiagrams in this chapter) is shown for operating conditions, since under theseconditions it is the most sensible to analyse the influence of the cell design onthe entropy generation in the cell.
In the bulk of the cell the quasi Fermi levels EFn,p are almost completely
78
Figure 3.1: Schematic overview of a working solar cell. The green part of the cell isthe photon (γ) absorber and the red and blue parts are the electron and hole selectivemembranes. The asymmetry between electron conductivity (σn) and hole conductivity (σp)drives a current through the load. In practice it is not possible to differentiate betweenelectron and hole current inside of a metal, but the underlying idea is that the selectivecontacts ensure that the easiest (i.e., least resistive) recombination pathway for the carriersis through the metal contacts and the external load.
79
Figure 3.2: Sketch of the band diagram of a p–contact under operating conditions. Thecontact consists of a highly pdoped region between the absorber and the metal. The quasiFermi levels are assumed to be continuous, but in practice it is possible to have a discontinuityin EFn across semiconductormetal interface. As will be demonstrated in the discussion ofthe Schottky contact in Section 3.3, this discontinuity does not complicate the discussion ofthe selective contacts significantly.
80
flat1. Of course, there have to small gradients in EFn and EFp to drive thecarriers to their collecting contacts, but for a material with a high enoughmobility (such as cSi) these gradients are typically so small that EFn and EFpcan be considered constant throughout the bulk of the cell. As a rule of thumbit should be remembered that the quasi Fermi levels EFn and EFp are almostcompletely straight in those parts of the cell where there are many electronsor holes respectively2. If this were not the case, the gradient in EFn (EFp)would drive a large amount of electrons (holes) in such a way that the gradientis nullified.
Bulk transport losses are generally small in the 1D cell for materials witha high mobility like cSi and they will therefore not be discussed in detail.However, it is interesting quickly compare the charge transport in the bulkwith the ideal transport requirement from Section 2.6. This requirement statedthat, for given transport coefficients Lnn, Lpp, the optimal way to drive a giventotal charge current Jcharge is by making the electron and hole thermodynamicforces equal and opposite (see Eq. (2.60)). This means that it is desirable tohave E′Fn = E′Fp in the bulk of the cell. Fortunately, it is not necessary toworry about this requirement, since the bulk of the cell is chargeneutral aslong as the background doping is uniform and from chargeneutrality it can bederived that:
0 =d
dx[p− n+Ndop]
=d
dx
[NV exp
(−EFp − EV
kBT
)−NC exp
(−EC − EFn
kBT
)+Ndop
]=
1
kBT
[NV(E′V − E′Fp) exp
(−EFp − EV
kBT
)−
NC(E′Fn − E′C) exp
(−EC − EFn
kBT
)]= 0. (3.1)
Since E′C = E′V, it follows that E′Fn = E′C = E′Fp and that charge neutrality
ensures that the charge transport is optimal3.Having determined that the transport losses in the bulk are not of great
concern, it remains to analyse the scalar entropy generation processes in thephoton absorber: the absorption of photons and generation/recombination ofelectronhole pairs. The entropy source term for the scalar processes in the bulkis denoted by qs,bulk. Assuming a constant Fermi level splitting EFn − EFp =
1From this point onward it is more convenient to work with the quasi Fermi levels EFn,prather than of ηn,p, since EFn,p are easier to draw in a band diagram. Recall that ηn = EFnand ηp = −EFp.
2Or, to be more precise: in those parts of the cell where the electron or hole conductivityis large
3Actually, Eq. (3.1) can be zero while E′Fn 6= E′Fp, but this typically only happens aroundvery strong local sinks or sources of electronhole pairs.
81
∆ηeh, the total entropy generation (per unit area of the cell) in the bulk isapproximately (see also Sections 2.5 and 2.6):
y
bulk
Tqs,bulk dx =y
bulk
(qu + ∆ηeh[R(∆ηeh)−G]) dx
= Iu −∆ηehIgen + ∆ηehdbulkR(∆ηeh). (3.2)
Here, Iu is the total absorbed energy flux (per unit area); Igen is the totalgeneration rate of electron hole pairs in the bulk; and dbulk is the thickness ofthe bulk. Recall that R is generally an increasing function of ∆ηeh. It is important to direct attention to the fact that the thermodynamic thermalisationlosses associated with photon absorption are given by Iu −∆ηehIgen and not,as commonly pictured, by Iu−EGIgen (see Figure 3.3). In other words, from athermodynamic perspective it is important to consider the free energy ∆ηeh ofthe generated pairs and not the total energy. This is because part of the totalenergy of the electronhole plasma simply cannot be extracted as useful workin the same way that it is not possible to cool the cell down and extract thethermal energy as work.
In Eq. (3.2, the fluxes Iu and Igen are more or less fixed by the propertiesof the incident light and the bandgap of the semiconductor, leaving ∆ηeh anddbulk as the main optimisation parameters to reduce the entropy generation inthe bulk. In practice, this means that dbulk should be as low as possible withoutimpairing the ability of the cell to absorb all of the incident photons. Indeed, itis wellknown that thin cells tend to have a higher performance (mainly due toa higher VOC) than thick cells (see, e.g., De Wolf [3]). The Fermi level splitting∆ηeh is controlled by maintaining a potential across the cell and the optimalpotential is commonly known as the maxpower voltage Vmpp. Thus, if the cellis completely limited by its bulk, the optimal potential is found making thebest tradeoff between the terms −∆ηehIgen (i.e, the total production of freeenergy) and ∆ηehdR(∆ηeh) (i.e., the loss of free energy).
It can be seen that the Fermi level splitting in the bulk of the cell is crucialto the operation of the device, so it is useful to consider for a moment whatmakes Fermi level splitting possible in the first place. As was demonstrated inSection 2.3.1, Fermi level splitting is only possible in a nonequilibrium state ofthe cell since ∆ηeh = 0 in equilibrium. Put differently, the Fermi level splittingrepresents the failing of electrons and holes to reach electrochemical equilibriumfast enough to counteract the external influences (the incoming light and thevoltage that is maintained over the cell) that are continuously disturbing theequilibrium. In the semiconductor, an electron is forced to make one big changein energy to recombine with a hole due to the bandgap of the material whichdoes not allow the electron to occupy a state with an intermediate energy.Since such a big change in energy is relatively improbable, the recombinationrate is much lower than if the electron has states available with intermediate
82
Figure 3.3: Two different visualisation of thermalisation losses after photon absorption.Figure (a) show the thermalisation losses of the energy of an e−–h+pair, while (b) shows thethermalisation losses of the free energy of the same pair. Of course there are no energy statesin the band gap, so (b) should not be interpreted as if the electron and hole are actuallyoccupying forbidden states.
83
energies that would allow the electron to lose its energy gradually stepbystep (such as when the semiconductor material is impure and has defect statesin the forbidden gap). This is why Fermi level splitting can be achieved insemiconductors but not in metals, since in a metal there are (by the definingproperty of a metal) many intermediate states that make it very easy for theelectrons to reach chemical equilibrium.
Next the selective contacts will be considered. To simplify the discussion,a p–contact will be taken as a specific example, but what follows applies toelectron contacts with equal validity. Thus, holes are the majority carriersand the electrons are the minority carriers for now4. Consider a short intervalx ∈ [0, L] close to the a holecollecting contact, with x = 0 a point in thebulk and x = L the position of the metal. The first thing to note about theband diagram of the p–contact in Figure 3.2 is that EFp is almost completelystraight because of the very high hole density. Due to the small gradient, thetransport of holes across the p–membrane is almost lossless, as can be seenwhen writing out the transport losses qs,trans (see Eq. (2.57)) for the problemat hand. There are three equivalent forms for qs,trans that can be obtained bysubstitution of the fluxforce relations (specifically: Eqs. (A.4) in AppendixA.1):
Tqs,trans = −E′FnJn + E′FpJp (3.3a)
=σne2
(E′Fn)2 +σpe2
(E′Fp)2 (3.3b)
=e2J2
n
σn+e2J2
p
σp. (3.3c)
Recall that here the chosen unit of EFn,p is eV and that of Jn,p is cm−2 s−1. Eq.(3.3c) shows that for a given current Jp (i.e., the photocurrent), qs,trans is smallsince σp is very large. Furthermore, Eq. (3.3a) demonstrates that if for somereason (e.g., Fermi level pinning at the interface) the hole quasi Fermi levelbends upward, a lot of entropy will be generated in the p–contact. A straightEFp is therefore an absolutely necessary condition for a good p–contact.
It can also be seen in Figure 3.2 that EFn and EFp meet at the metalcontact. As mentioned, the reason for this is that inside of the metal therecan be no Fermi level splitting since metals do not have a bandgap. Note inparticular that EFn bends towards EFp rather than the other way around. Thisis because the electron concentration is much lower in the doped region thanin the rest of the cell and this low concentration makes it possible to have large
4When selective contacts are discussed in this chapter, the terms “minority carriers” and“majority carriers” will always refer to the carriers that are least/most abundant in theselective membrane. This is different from the common terminology where minority/majoritycarriers are designated with respect to the doping of the bulk of the cell. Thus, in a p–membrane, the majority carriers are holes; in an n–membrane the majority carriers areelectrons.
84
gradients in EFn. The bending of EFn is also the reason it is undesirable to havegeneration inside of the doped region, since the ∆ηehG product is necessarilylower in the p–contact than in the bulk, meaning that the generation of e−–h+
pairs in the doped region produces less free energy than in the bulk, leading toparasitic absorption. It should be emphasised that the high selectivity of thep–membrane and the decreasing Fermi level splitting inside of it, are strictlyrelated to one another. Simply put, it is not possible to have a selective contactthat is efficient at absorbing photons. The reason it makes sense to discuss asolar cells in terms of absorbers and selective membranes can be traced backto this elementary duality between functions.
The gradient of EFn across the selective contact drives an electron recombination current Jn towards the surface. This gradient and the recombination current cannot be avoided since a large Fermi level splitting in the bulk∆ηeh = EFn(0) − EFp(0) > 0 is necessary to generate useful work. In otherwords: ∆ηeh is simultaneously the voltage over the cell (this is because thequasi Fermi levels are nearly constant in the bulk) as well as the driving potential difference of the electrons towards the metal. Thus, there will alwaysbe contact recombination whenever the cell is producing power. Because thegradient in EFn is unavoidable, Eq. (3.3b) is the most convenient form ofqs,trans to assess the losses due to the minority carrier transport, which showsthat the only way to reduce the entropy generation from the minority carriersis to make the σn as low as possible.
To gain insight into the relation between Jn, ∆ηeh and the design parameters of the solar cell, an approximate solution to the driftdiffusion equationwill given here in a fashion similar to Del Alamo [4]. This approximate solution will then be generalised and applied to other types of selective contactsto assess their potential for application in highefficiency solar cells. The mostimportant assumption that will be used, is that on the short length scales ofthe selective contacts, the source terms G and R have negligible influence onthe shape of EFn and EFp. In a cSi solar cell, this assumption holds to a gooddegree of accuracy for the junction on the rear side of the cell (known as theback surface field or BSF), so for the moment a BSF will be discussed. At thefront junction of a cSi cell, though, it is usually not possible to neglect G sincethe generation will affect the minority carrier quasi Fermi level significantly.This issue will be discussed briefly in Section 3.6 and as it will turn out, theissue of generation in the front membrane can be considered separately fromthe selectivity of that membrane, except for the case when the generation alsosignificantly affects the majority carrier quasi Fermi level (which is uncommon).
In the BSF, the conductivity can be taken as an explicit function of x, so
85
that the electron transport equation is:
−σn(x)
e2E′Fn(x) = Jn = constant, (3.4)
EFn(0)− EFn(L) = ∆ηeh. (3.5)
This equation is straightforward to integrate, giving:
Jn =∆ηeh∫ L
0e2
σn(x) dx. (3.6)
The integral of 1/σn can be interpreted as a resistance (normalised to area), soEq. (3.6) expresses (as expected) that the resistance of the region 0 ≤ x ≤ Ldetermines the recombination current for a given potential difference ∆ηeh overthe region. Eq. (3.6) is therefore simply Ohm’s law, but unfortunately it isonly useful qualitatively since σn = enµn is a function of EFn and therefore theresistance of the region 0 ≤ x ≤ L cannot be calculated directly. This makesthe ordinary resistance (or conductance) relatively poor tools for understandingthe working of a solar cell, so the next paragraphs will be used to develop twoalternative concepts of resistance that are easier to compute. To obtain thesealternative measures of resistance, first the electron driftdiffusion equation iswritten in full by expanding σn using the Boltzmann exponent for n:
σn(x) = eµn(x)NC exp
(−EC − EFn
kBT
). (3.7)
Thus, the electron transport equations is then:
−µn(x)NC
eexp
(−EC(x)− EFn(x)
kBT
)E′Fn(x) = Jn. (3.8)
To solve this equation, it is assumed that EC(x) is already known. Of course, itis not possible to find the exact shape of the conduction band without solvingall three driftdiffusion equations simultaneously, but in most cases it is possibleto obtain a good approximation to EC(x) without much difficulty using, e.g.,the Poisson Boltzmann equation under the assumption that EFn is straight(see Appendix A.2 and the red dashed line in Figure 3.2).
With EC(x) known, Eq. (3.7) can be solved for EFn by noting that:
exp
(EFnkBT
)E′Fn =
d
dx
[kBT exp
(EFnkBT
)](3.9)
The solution is therefore:
EFn(0)− EFn(L) = ∆ηeh
= −kBT ln
1− eJnkBT
∫ L
0
1
µn(x)NC(x) exp(−EC(x)−EFn(0)
kBT
) dx
.
(3.10)
86
Rewriting for Jn gives:
Jn = VT Sn
[1− exp
(−∆ηehkBT
)], with: (3.11)
Sn =
∫ L
0
1
µn(x)NC(x) exp(−EC(x)−EFn(0)
kBT
) dx
−1
=
[∫ L
0
1
µn(x)n(x)dx
]−1
. (3.12)
Here the symbol Sn is used to denote a quantity that will be called the electronpseudo conductance of the doped region. It is the conductance that is calculated by assuming that the quasi Fermi level for the electrons is straight (i.e.,EFn(x) = EFn(0) for 0 ≤ x ≤ L indicated by the red dashed line in Figure 3.2).The associated electron density n(x) will be referred to as the pseudo electrondensity and Rn = S−1
n is the electron pseudo resistance5. In Eq. (3.11), thelast factor is approximately 1 since ∆ηeh kBT under operating conditions.Thus, in a sense, Eqs. (3.6) and (3.11) can be interpreted as if one can eitheruse ∆ηeh or kBT as the driving force for Jn. When ∆ηeh is used as the drivingforce, then the real conductance should be used to calculate the recombinationcurrent; when kBT is used as the driving force, then the pseudo conductanceshould be used instead.
The pseudo conductance Sn depends exponentially on ∆ηeh due to theinjection of electrons from the bulk into the doped region, so it is preferable tosplit off this trivial exponential dependence in the hope that whatever remainsis approximately independent of ∆ηeh. Thus, Jn is written as:
Jn = VT Sn
[exp
(∆ηehkBT
)− 1
], (3.13)
= J0,n
[exp
(∆ηehkBT
)− 1
], (3.14)
The resulting parameter Sn = Sn exp (−∆ηeh/kBT ) will be called the intrinsicelectron conductance of the selective membrane because it usually does notdepend on the injection level in the bulk of the cell. It is related to the wellknown recombination parameter J0,n by J0,n = VT Sn. Some manipulation
5Because the default unit of current is cm−2 s−1 in this work, eS yields the conventionalmeasure of areanormalised conductance. Thus [eS] = S cm−2 and [R/e] = Ω cm2
87
yields:
Sn =
∫ L
0
1
µn(x)NC exp(−EC(x)−EFp(0)
kBT
) dx
−1
(3.15)
=
[∫ L
0
1
µn(x)n(x)dx
]−1
. (3.16)
In words: Sn is the electron conductance calculated by assuming that EFn(x)= EFp(0). The electron density calculated from this assumption is denoted byn and Rn = S−1
n is the associated resistance. Note that Sn is almost equal tothe electron conductance calculated under equilibrium conditions where EFn =EFp = EF and n = neq. The reason it is not identically equal to the equilibriumconductance is because in the bulk of the cell EFp 6= EF due to injection ofholes and because EC(x) depends on the operating conditions as well. However,the integral in Eq. (3.15) takes only a small contribution from the bulk, so thiseffect only has a small influence on Sn. In the p–membrane, which contributesthe most to Sn, the doping is typically high enough to pin EFp and EC totheir equilibrium positions regardless of injection level. Thus, even thoughequilibrium band diagrams cannot provide a complete picture of the operationof solar cells, they can still be useful for making estimates of the intrinsicminority carrier conductivities of selective membranes.
To conclude, there are now three different measures of electron conductance:real, pseudo and intrinsic:
The real conductance is calculated from the actual electron density n andthe corresponding current driving force is the gradient of EFn.
The pseudo conductance Sn is obtained by pretending that EFn is straightand then calculating the pseudo electron density n from that assumption.The current driving potential corresponding to the pseudo conductanceis VT (1 − exp(−∆ηeh/kBT )) ≈ VT . Thus, the pseudo conductance substantiates the intuition that the minority carrier recombination currentis thermally driven towards the metal contact.
The intrinsic conductance Sn is obtained by pretending that EFp is alsothe electron quasi Fermi level and calculating the density n from thatassumption and its current driving potential is VT (exp(∆ηeh/kBT )− 1).The main advantage of Sn is that it does not depend strongly on theoperating conditions, because the exponential dependence of the currenton ∆ηeh has been absorbed into the driving force. This makes Sn approximately a device parameter, though care should be taken to not mistakeit for a true constant: depending on the exact nature of the device Sn canstill depend on ∆ηeh and if it does, it should be evaluated at maxpowerconditions to be of use as a device parameter.
88
3.2.1 What is selectivity?
At this point it is a good moment to reflect on the meaning of the word “selectivity” that has been used a couple of times so far. Indeed, this word ismentioned more and more frequently in the field of PV, yet no quantitativemeasure of selectivity has been proposed (to the author’s knowledge), thoughthe recombination parameter J0 is commonly mentioned as an important quantity connected to selectivity. However, J0 is not a true measure of selectivity,since it does not measure the asymmetry between electron and hole conductance: a contact could have a low J0 by simply being poorly conductive to bothelectrons and holes without actually preferring one over the other. To addressthis caveat, a selective contact can then be defined by having not only a lowJ0 but also a low majority carrier resistivity (as has been assumed throughoutthis chapter).
Clearly, these two requirements are a good characterisation of a selectivecontact, yet they fail to precisely define what selectivity is by itself and amathematical definition of selectivity is still absent. Given the discussion in theprevious paragraphs, the first idea that comes to mind for defining selectivity,is to introduce a dimensionless number that is obtained by taking the quotientof some measure of minority carrier resistance and some measure of majoritycarrier resistance. Since it is desirable to have a figure of merit that is moreor less independent of the voltage over the device, the intrinsic resistance Rnis the most suitable candidate for the electron resistance of the p–membrane.For the holes it can be said that the real, pseudo and intrinsic resistances areall equivalent and will simply be denoted by Rp. Thus, the selectivity of ap–membrane would then be Rn/Rp. In terms of the usual definitions of J0 (inA cm−2) and contact resistance ρc = Rp/e (in Ω cm2) the selectivity can beexpressed as νp = VT /(J0ρc), confirming that high selectivity requires both alow J0 and a low ρc.
However, this measure of selectivity is somewhat unsatisfactory. To seewhy, it is necessary to answer the question why exactly selectivity is importantfor a solar cell. Intuition would probably say that a high selectivity is necessary to ensure that the losses due to minority carrier recombination in thecontacts are kept minimal, but this idea is actually not necessarily true andcertainly not the complete story. As an example, consider a simplified modelof a solar cell that is only limited by contact recombination (and perhaps otherrecombination mechanisms that can be described by an ideal diode equation).This means that EFn and EFp are approximately constant in the bulk6. In addition, it is assumed that the intrinsic conductivities of the n–contact and thep–contact are both constant, so that the losses in the cell can be described bya single recombination parameter J0 = kBT (Sn + Sp). Since transport losses
6It is possible to incorporate bulk resistance in the following argument, but it makes theformulae more complex yet it does not affect the result in Eq. (3.20) significantly.
89
are neglected, the total charge current through the cell Jcharge = Jp − Jn isgiven by an ideal illuminated diode equation:
Jcharge = Jgen − J0
(exp
(∆ηehkBT
)− 1
), (3.17)
with Jgen the photo generation current density. To extract as much free energy from the cell as possible, it is necessary to maintain an optimal potential∆ηeh = ∆ηmpp (i.e., the maxpower potential) across the cell that maximisesthe product ∆ηehJcharge. This maximisation of an ideal solar cell is a wellknown exercise and leads to the following transcendental equation for ηmpp:
Jcharge(∆ηmpp)− ∆ηmpp
kBTJ0 exp
(∆ηmpp
kBT
)= 0. (3.18)
The solution to this equation is not of real interest here: what should be notedis that the second term in Eq. (3.18) is almost equal to the power loss due tocontact recombination of minority carriers Ploss. After all, the recombinationcurrent is given by Eq. (3.14) (in which the −1 term can be safely omitted)and the dissipation is obtained by integrating −E′FnJn over the p–membraneand E′FpJp over the n–membrane. Since Jn,p are constant, these integrationsresults in the loss terms ∆ηmppJn and ∆ηmppJp. Thus the total power lossdue to recombination at the max power point is then:
Ploss = ∆ηmppJ0
(exp
(∆ηmpp
kBT
)− 1
)≈ ∆ηmppJ0 exp
(∆ηmpp
kBT
). (3.19)
According to Eq. (3.18) the power loss due to recombination is:
Ploss = kBTJcharge(∆ηmpp). (3.20)
What makes this result noteworthy and perhaps seemingly paradoxical, is thatPloss is nearly independent of J0, since it is wellknown that for an ideal solarcell (i.e., a cell described by a diode equation) the maxpower current is closeto Jgen, regardless of the recombination parameter. So if the power loss isapproximately constant, what is the use of improving J0? The answer is thata lower J0 leads to a higher ∆ηmpp, meaning that the majority carriers obtainmore free energy (or, conversely, that there is less entropy generation associatedwith photon absorption (see Eq. (3.2) and Figure 3.3). Thus, even though all ofthe recombination occurs in the contacts, the most important thermodynamiclosses occur in the bulk of the cell. The optimisation of J0 (and thereforethe selectivity of the contacts) is therefore less about minimising losses in thecontacts and more about maximising gains in the bulk! This example alsoserves to illustrate that the optimisation of solar cells is a strongly nonlocalproblem, meaning that a design flaw in one part of the cell might lead to powerlosses in a completely different part.
90
Thus, the problem with defining selectivity as Rn/Rp is that these tworesistances affect the cell in completely different ways: Rp (linearly) affects theohmic losses in the p–contact, while Rn (logarithmically) affects the generationlosses in the bulk. A better way to define selectivity is obtained by consideringthe electrochemical potential. It is the job of a selective contact to enable alarge ∆ηeh in the bulk of the cell while also losing as little free energy as possiblewhen the majority carriers are conducted out of the cell. From Eq. (3.3a) it wasderived that the gradient in EFp is a good measure of the extraction efficiencyof holes, since Jp is fixed and equal to the photo current. Integrating E′Fp overthe selective contact yields (analogously to Eq. (3.6)):
∆EFp = EFp(L)− EFp(0) = eJpRp = eJgenRp. (3.21)
This potential drop should be compared to the maxpower potential ∆ηmpp
that the contact can sustain in the bulk of the cell. However, since ∆ηmpp isslightly difficult to compute, it is more convenient to look at the open circuitpotential ∆ηOC that the contact can sustain (i.e., the potential at which Jn =Jgen). It is given by:
∆ηOC = kBT ln
(Jgen
J0+ 1
). (3.22)
Thus, a selective contact is expected to have a high ∆ηOC and a small ∆EFp.The selectivity of a p–membrane νp will now be defined as:
νp =∆ηOC
EFp(L)− EFp(0)=VT ln
(Jgen
J0+ 1)
JgenRp. (3.23)
The physical interpretation of νp becomes clear once its inverse is considered:ν−1p is the fractional voltage loss due to ohmic dissipation in the p–contact if
the cell would be completely limited by just that contact.Having defined the selectivity, it should be noted that selectivity by itself is
not enough to evaluate the performance of a selective contact. For example, thecontact could be selective because its majority carrier resistance is extremelylow rather than having a low J0. Such a contact would not be very usefulfor a solar cell. Indeed, no single parameter is capable of characterising aselective contact completely by itself since any assessment necessarily requiresconsideration of both electrons and holes and at the very least two figures ofmerit are necessary for this task. In a sense, J0 and ρc already provide thiscomplete characterisation, so the added value of discussing selectivity is notthat it provides a new figure of merit that yields more information. Instead,the added value provided by the terminology of selectivity is the fact that theword selectivity draws attention to concepts of resistance for the understandingof the operation of solar cells.
91
After this general discussion of selective contacts, the equations for thepseudo and intrinsic conductances/resistances will be used in the next threesubsections to assess the selectivity of three important kinds of selective contact: the homojunction, the heterojunction, and the Schottkyjunction. Tokeep the formulae simple, most of the attention will be directed towards Snand Rn (rather than νp), since these two parameters are the most crucial limiting factors for the contact performance in the examples that will be given.
3.3 The selectivity of Schottkytype junctions
In a Schottkytype junction illustrated in Figure 3.4a, the most importantfeature is a space charge region (SCR) in the semiconductor directly adjacentto the metal contact. In the ideal case, the source of this SCR is the missmatch between the metal workfunction ΦM and the intrinsic Fermi level of thesemiconductor (see, e.g., Sze [5] or Ibach & Luth [6]). For the moment thisideal model of Schottky junctions will be considered; nonideal factors will bediscussed afterwards.
In the Schottky SCR, one type of carrier (in this example the electrons) isalmost completely depleted, making the SCR more resistive to that carrier type.Schottkytype junctions are still occasionally proposed as selective contactsthat are potentially relevant for solar cells, so it is a useful exercise to analysetheir potential. For example, several authors have proposed devices based ongraphene/cSi junctions [7, 8, 9]. To determine the selectivity potential ofa Schottky junction, the intrinsic electron conductance Sn of the SCR will beestimated. Let the position x = 0 be the edge of the SCR in the semiconductorand x = L the position of the metal contact, noting that the width of the SCRdepends on the Fermi level splitting ∆ηeh in the bulk and on the total bendbanding across the SCR ∆φ. Next, the expression for Sn can be transformedby noting that np is approximately the equilibrium np = n2
i product since nis the electron density computed from EFp (recall that EFp 6= EF , though).Furthermore, the mobility will also be assumed constant over the SCR. Usingthese approximations, the intrinsic electron resistance Rn becomes:
Rn ≈1
µnn2i
∫ L
0p dx ≈ 1
µnn2i
(QSCR − LNdop) . (3.24)
Here, QSCR is the total amount of space charge (in units of cm−2) and Ndop isthe background charge of the doping in the semiconductor (in units of cm−3).The reason the integral of p can be rewritten like this, is because the contribution of the electron density to the total space charge is negligible.
Eq. (3.24) is useful to make an estimation of how much space charge isneeded to obtain a contact that is selective enough for a high efficiency cell.For example, if the aim is to make a cSi solar cell with a VOC of 750 mV,
92
(a) (b)
Figure 3.4: Sketch of the band diagram of a holeselective Schottky contact under workingconditions. In (a) the interface is assumed to be nonresistive, resulting in a continuouselectron quasi Fermi level. In (b) the interface is modelled as a transition region that linksthe bulk descriptions of the two materials. The exact nature of this transition region isnot known, but the current that crosses it can, for example, be modelled by a thermionicemission model. The resistance of the region creates a discontinuity E−Fn − E
+Fn > 0 across
the interface.
then the recombination current should not exceed the short circuit currentJSC ≈ 43 mA cm−2 in Eq. (3.13) (with ∆ηeh = 750 meV). This meansthat the intrinsic resistance Rn/e should be more than 2.6 · 1012 Ω cm2 andJ0,n < 10 fA cm−2. To achieve this, a total space charge QSCR > 4 · 1016 cm−2
is necessary in the Schottky contact according to Eq. (3.24) (the doping densityhas no influence on this result for realistic values of Ndop). To put this number into context, values of QSCR between 1012 and 1013 cm−2 are commonlyencountered in cSi inversion/accumulation layers7.
The Poisson Boltzmann (PB) equation in Appendix A.2 can be used tofind QSCR as a function of the total band bending and a straightforward calculation shows that a value of QSCR = 4 · 1016 cm−2 would require more than80 eV of band bending in the cSi: an amount that is completely unfeasiblein practice. For a cSi Schottky junction, the bandgap of silicon (1.124 eV)is a reasonable upper limit to the amount of (equilibrium) band bending thatcan be achieved. This upper limit corresponds to an amount of space chargeof QSCR < 1 · 1014 cm−2 (regardless of the voltage over the cell). According to Eq. (3.24), the lower limit for the recombination parameter is thenJ0 > 4 · 103 fA cm−2, giving an upper limit of VOC < 600 mV for spacechargelimited Schottky cells.
7This range of charge is, not coincidentally, also the typical amount of fixed charge commonly encountered in heavily charged oxide passivation films on cSi such as Al2O3 [10].
93
From this estimation can be concluded that the SCR in a cSi Schottkyjunction can only achieve a limited amount of selectivity. In fact, in the fieldof device modeling, the SCR in cSi cells can frequently be neglected withoutintroducing significant error in the simulation (see, e.g., the COBO model byBrendel [11] and the Quokka model by Fell [12]) precisely because the SCRpossesses so little selectivity. Clearly, if a SCRbased cell is to achieve a highefficiency, then it is necessary to introduce some extra source of selectivity between the cSi and the metal. At this point it is worth considering the nature ofthe cSi/metal interface in more detail, since it has been significantly simplifiedin the discussions until now. The assumption that EFn is continuous acrossthe interface essentially assumes that this interface is truly twodimensionaland therefore does not present any resistance to the carriers that cross it. Inreality this is not true and it is more accurate to regard the interface as a transition region of small but finite thickness where the bulk descriptions of the twojoining materials fail because of their close proximity (see Figure 3.4b). Theexact nature of this transition region is generally unknown, making it difficultto formulate a closed transport equation for this region. The most convenientway to deal with this uncertainty is to use an empirical model that describesthe current through the transition region by imposing a modified boundarycondition on Jn. In a sense, this means that the transition region is integratedout of the transport equation and by doing so, new empirical parameters areintroduced that need to be correlated with experiment. The process of integrating out the transition region also causes a discontinuity in EFn; the valuesof EFn on either side of the region are denoted by E−Fn and E+
Fn as indicatedin Figure 3.4b.
A commonly used approximation for the transport of electrons betweenthe semiconductor and the metal is the thermionic emission (TE) model. Thismodel essentially asserts that the electrons on both sides of the interface behavelike Fermi gases that are separated by an energy barrier of height ΦB = ΦM−χ,with ΦM the metal work function and χ the electron affinity of the semiconductor. Only an exponentially small fraction of the electrons in the metal haveenough kinetic energy to cross the energy barrier ΦB, while electrons from thesemiconductor are free to move down the energy barrier into the bulk. Thus,the current JM,S from the metal into the semiconductor is:
eJM,S = A∗T 2 exp
(− ΦB
kBT
), (3.25)
with A∗ an empirical parameter called the effective Richardson constant, whichcharacterises the microscopic details of the interface. Typically, A∗ is on thesame order of magnitude as the universal Richardson constant A0. At T =300 K it is given by:
A0T2 =
4πmek2BT
2e
h3= 1.08 · 107 A cm−2. (3.26)
94
Often, A∗ is slightly smaller than A0 due to the quantum mechanical probability that electrons reflect from the energy barrier even if (classically) they haveenough energy to cross the interface. Furthermore, A0 only takes the from inEq. (3.26) if the bands in the metal and semiconductor are parabolic and ifthe charge carriers are not confined to less than 3 dimensions.
The current JS,M from the semiconductor into the metal depends on thesurface electron density n(L) and the conduction band density of states NC:
eJS,M = A∗T 2n(L)
NC. (3.27)
There is a special motivation for using this form of JS,M that becomes apparentwhen JTE = JS,M−JM,S is written out and manipulated into the following form:
JTE =A∗T 2
e
[n(L)
NC− exp
(− ΦB
kBT
)],
=A∗T 2
e
n(L)
NC
[1− exp
(−E−Fn − E
+Fn
kBT
)]. (3.28)
This form suggests that JTE is driven by the electrochemical potential difference E−Fn−E
+Fn across the transition region, just like Jn is driven by the ∆ηeh
in Eq. (3.11). Note especially that JTE becomes zero whenever E−Fn = E+Fn,
showing once more that the gradient in Fermi level across the interface is thedriving force behind the thermionic emission, with electrons flowing from highto low EFn just like in the rest of the cell. Indeed, it would be a violationof the second law of thermodynamics if electrons would flow from low to highEFn across the interface since they would be gaining (rather than losing) freeenergy from being transported.
This suggests that the TE interface can be seen as a (zerodimensional andnonlinear) electron resistance not fundamentally different from the rest of thecell. Indeed, if the same analysis that led to Eq. (3.11) is carried out for theSchottky contact with TE transport at the interface, the pseudo and intrinsicresistances are given by:
Rn =kBTNC
A∗T 2n(L)+
∫ L
0
1
µn(x)n(x)dx, (3.29a)
Rn =kBTNC
A∗T 2n(L)+
∫ L
0
1
µn(x)n(x)dx, (3.29b)
=kBT
A∗T 2exp
(ΦB
kBT
)+
∫ L
0
1
µn(x)n(x)dx. (3.29c)
Thus, the total resistance the electrons encounter is simply a sum of the resistance of the SCR (given by the integral) and the interface. Eqs. (3.29a) and(3.29b) show that interface resistance is found by calculating VT /JS,M from n or
95
n. Eq. (3.29c) (which is obtained by assuming that the majority carrier Fermilevel EFp is constant throughout the transition region) show that the intrinsicresistance of the transition region is a constant that only depends on the temperature, the barrier height, and the effective Richardson constant. Note that,perhaps surprisingly, the intrinsic resistance of the TE interface increases exponentially with ΦB, even though the electrons cross the semiconductor/metalbarrier in the energetically downward direction. This demonstrates once morethat, when discussing transport of charge carriers, the total energy of the carriers is relatively unimportant since only the free energy drives the current.Thus, the formula Rn ∼ exp(ΦB/kBT ) should not be interpreted as if the electrons have to cross an energy barrier, but rather that the barrier depletes theelectron density near the interface.
It is an interesting exercise to calculate how large the energy barrier shouldbe to salvage the VOC = 750 mV goal for cSi Schottky junctions that wasproposed earlier. If the Richardson constant is taken as A∗ = A0, thenΦB > 1.251 eV will yield a high enough interface resistance to achieve thisgoal without taking into account the SCR. This is a rather significant number and it is not straightforward to achieve such an energy barrier in practice.However, the value of A∗ can be significantly lower than A0 for some junctions.As an example, graphene/cSi junctions, which will be discussed in Chapter 6,have an effective Richardson constant8 of more than three orders of magnitudelower than A0 [13], which brings down the requirement on the energy barrier toΦB > 1.026 eV; a value that is physically feasible for a graphene/cSi junction.
As can be seen, if a cSi Schottky junction is to be successful as a selectivecontact, the metalsemiconductor interface is of great importance since that isthe part where most of its selectivity will need to be derived from. Primarily,this means that metalsemiconductor interface needs to be of high quality: ifthe interface is defective, then the electrons will recombine before reaching theTE interface and the resistance of the interface becomes irrelevant9. Unfortunately, interface defects are common in Schottkytype junctions since the closeproximity of the metal makes impurities in semiconductor very likely. Moreover, even if one succeeds in making an atomically sharp interface, there willbe states in the metal that decay into the semiconductor where they generate ahigh density of midgap states called MIGS (Metal Induced Gap States [6, 14]).These MIGS will often influence the barrier height ΦB significantly and mayeven cause EFp to bend due to Fermi level pinning. It is therefore very difficultto fabricate Schottky junctions that can serve as a good selective contact aslong as the interface consists of nothing more than a metal on a (lowly doped)
8as will be explained in Chapter 6, these junctions actually do not have Richardson constant of the form in Eq. (3.26), but this detail is unimportant for now.
9In fact, as Section 3.6 will demonstrate, the recombination that happens before thecarriers have crossed the interface can simply be regarded as a parallel resistance that shuntsthe interface resistance, thus limiting its selectivity.
96
semiconductor. An appealing solution is to insert a thin film of oxide betweenthe semiconductor and the metal that can prevent impurities from reachingthe semiconductor while simultaneously subduing the MIGS. For example, ingraphene/cSi based junctions, the inclusion of an SiO2 film has already beenshown to lead to a better VOC [9]. However, even with an oxide buffer film,the Schottky junction still needs to have a high intrinsic ΦB and a low A∗ toact as a selective contact.
3.4 The selectivity of homojunctions
The next selective membrane that will be considered is the homojunction shownin Figure 3.2, which is currently the most common type used in industry.To assess the selectivity potential of the doped p–membrane, a blockshapeddoping profile of width d and uniform doping Ndop is assumed. For such aprofile, Sn and Sn are straightforward to calculate since the resistance integrals(Eqs. (3.12) and (3.15)) are completely dominated by the interval L − d ≤x ≤ L and because the valence and conduction bands are flat in the selectivemembrane. Note that the SCR in the bulk induced by the homojunction isignored here: just like in the Schottky cell, the SCR in a homojunction canonly achieve a very limited amount of selectivity and its contribution to Sn isnegligible.
If ∆φ is used to denote the band bending across the junction (see Figure3.2), then the pseudo electron conductivity is approximately:
Sn ≈n(0)µn,BSF
dexp
(− ∆φ
kBT
). (3.30)
Here, µn,BSF is the electron mobility in the doped region (referred to as backsurface field for convenience). In Eq. (3.30) the semiconductormetal resistanceof the interface at x = L has been neglected (hence the continuous EFn inFigure 3.2), but it can be added in the same fashion as was done for Schottkyjunctions in Eq. (3.29a).
It is appealing to think of ∆φ as an energy barrier that blocks electronsfrom diffusing into the metal. This view is perhaps not even completely wrong,but it is important to remember that ∆φ is not constant but depends on thecarrier densities in the cell. This expression for Sn can therefore be deceptive.The intrinsic conductance does not have this problem and some manipulationyields Sn for a blockshaped doping profile:
Sn =µn,BSF n
2i,BSF
dNdop,BSF=µn,BSF neq
d, (3.31)
with n2i,BSF the equilibrium np product in the doped region, Ndop,BSF the p
type doping density in the BSF, and neq the equilibrium electron density in the
97
BSF. As was alluded to in Section 3.2, the high doping concentration in theBSF ensures that Sn is a true constant in the homojunction cell. Eq. (3.31)shows the three main parameters that influence the selectivity of a doped membrane: the minority carrier mobility, the equilibrium electron density and thedepth of the doping profile. In practice, however, µn,BSF and neq both dependon the doping density Ndop,BSF, since the mobility decreases with increasingNdop,BSF. This is because doping creates scattering centres that impede thetransport of electrons. The dependence of neq on the doping level is morecomplicated, since neq depends in the intrinsic carrier density ni,BSF, which inturn also depends on the doping density. There are two different phenomenathat influence ni,BSF, namely bandgap narrowing (BGN) and the transitionfrom Boltzmann to FermiDirac (FD) statistics for the holes. BGN tends toincrease the intrinsic carrier density because there is more thermal excitationof electron hole pairs when the bandgap shrinks. FD statistics, on the otherhand, tend to decrease ni,BSF. To see why, first consider the intrinsic carrierdensity in the bulk ni where Boltzmann statistics apply. Under equilibriumthere is a single Fermi level EFn = EFp = EF and thus:
n2i = n0 p0 = NC exp
(EF − EC
kBT
)NV exp
(−EF − EV
kBT
)= NCNV exp
(−EG
kBT
). (3.32)
The exponential dependence on EG is the reason why ni increases with decreasing bandgap. However, in a highly doped BSF where the holes becomedegenerate, the intrinsic carrier density changes to:
n2i,BSF = n0 p0 = NC exp
(EF − EC
kBT
)NV F1/2
(EV − EFkBT
). (3.33)
For high doping densities, EF < EV and the argument of the Fermi Diracintegral becomes positive. For large arguments, the Fermi function can beapproximated as a step function so that:
F1/2
(EV − EFkBT
)∼(EV − EFkBT
) 32
. (3.34)
Thus, by increasing the ptype doping, EF is shifted downward so that theelectrons are depleted exponentially in EF while the hole density only increasesproportionally to (EV−EF )3/2. Overall, this leads to a decrease in ni,BSF sincethe decreasing exponent will win over the increasing power law.
The bandgap narrowing with doping has been measured and modelled extensively, such as in the work by Yan and Cuevas [15, 16] where an easytousemodel for BGN in cSi is presented. From experiments it is know that for cSi,
98
the equilibrium minority carrier density decreases with increasing Ndop so thathighly doped contacts are always better at reducing the contact recombination.This is particularly true for the degenerately doped regime where the minoritycarrier density is more strongly depleted due to FD statistics (see Figure 3.5).Furthermore, at high doping densities the mobility µn is also reduced, whichimpedes electron transport towards the contact even more. However, there isa limit to the solubility of dopants in semiconductors (see, e.g., Jaeger [17],Kooi [18], and Vick et al. [19] for the solubility of dopants in silicon) andonce this limit has been achieved, the only design parameter that can increasethe selectivity of the homojunction is the depth of the doping profile d. Aquick backoftheenvelope calculation shows that achieving a J0 of less than10 fA cm−2 with a blockshaped doping profile requires that d > 10 µm. Thisshould be compared to typical cSi junction depths that are frequently no morethan 1 µm.
Potentially, the selectivity of the doped membrane can be made arbitrarilylarge by making it deep enough, but in practice the intrinsic recombinationinside of the membrane (e.g., Auger recombination) will impose a lower limiton the recombination current into the membrane. This is because the resistance encountered by a minority carrier to the point where it recombines issignificantly lower if that point is somewhere in the middle of the doped regionthan if the electron needs to travel all the way to the metal contact. Thus,at some critical diffusion depth, recombination inside of the doped region becomes dominant over recombination at the contact and at that point it will beno use to make the diffusion even deeper. Furthermore, it is not desirable tomake the junction arbitrarily deep for another reason, namely the fact that thedoped region has the same absorption coefficient as the bulk of the cell. Deeperdoping profiles will therefore result in more generation inside of the selectivemembranes, which should be avoided. Of course, for the selective contact atthe rear of the cell, one could also choose to make the absorber very thick sothat no light reaches the selective membrane, but this choice is at odds with theideal situation where the cell should be as thin as possible (see the discussionfollowing Eq. (3.2)).
3.5 The selectivity of heterojunctions
From the discussion of the homojunction cell and selective contacts so far, itcan be concluded that selective membranes ideally have significantly differentmaterial properties than the photon absorber:
1. The bulk of the cell needs to have a high absorption coefficient while theselective membrane should be completely transparent if possible. Alternatively, if the selective membranes are absorptive, then it is necessary
99
Figure 3.5: Equilibrium minority carrier densities in doped cSi as a function of the dopingdensity. The black line shows the minority carrier density if ni is assumed constant (at9.65 · 109 cm−3) (i.e., if the carriers are assumed to obey Boltzmann statistics and if thebandgap is assumed constant) . The deviations of the red (electron density) and blue (holedensity) lines from the black line are due to BGN and FermiDirac statistics (calculated withthe model by Yan and Cuevas [16]). Initially, the BGN opposes the decrease of the minoritycarrier density with doping density. However, at the point where FD statistics start tobecome influential, the minority carrier density decreases at an accelerated rate with doping.As shown by Eq. (3.31), it is favourable to have an equilibrium minority carrier densitythat is as low as possible. The plot shows that degenerately doped cSi is therefore the mostsuitable for making selective contacts. The arrows show the solubility limits of boron [19](red) and phosphorus [18] (blue) in cSi, demonstrating that ntype doped cSi can achieve amuch lower minority carrier density.
100
(a) (b)
Figure 3.6: Sketch of the band diagram of a selective heterojunction hole contact. Interfacedefects are assumed zero here. In (a) the ideal situation is depicted where the valence bandis continuous while the conduction band has an offset. In (b) there is also an offset in thevalence band: this leads to a larger SCR in the selective membrane, decreasing its effectivethickness deff and making it less resistive to electrons. Depending on the exact nature ofthe heterojunction, the SCR caused by the valence band offset might also pose a significantresistance to the hole current which would result in ohmic losses (i.e., FF loss) in the contact.
to direct the light inside of the cell in such a way that the selective membranes do not receive photons with energies above their bandgap.
2. The mobility of the bulk should be high for both electrons and holes, whilea hole (electron) selective membrane ideally has a high hole (electron)mobility and a very low electron (hole) mobility. In fact, it is possibleto make a working cell by having selective membranes that only differin their electron and hole mobility [2]. Typically, though, it is mostimportant that the minority carrier mobility is low since the majoritycarrier conductivity can be increased by doping if necessary.
3. The photon absorber is preferably a (defectfree) direct bandgap semiconductor since that promotes radiative recombination over other intrinsicrecombination mechanisms, making it possible to recycle the photonsemitted by recombining charge carriers. The selective membranes onthe other hand, should simply have as little recombination as possible,making indirect bandgap materials preferable.
These very different requirements suggest that for homojunction solar cellsit will always be difficult to find one material that performs well as both an
101
absorber and as a selective membrane. Heterojunctions do not have this intrinsic limitation of conflicting material properties, giving them significantlymore design freedom to achieve higher efficiencies. A frequently proposed idealheterostructure is one where the bands of the majority carriers are continuousacross the interface whereas the bands of the minority carriers have a large discontinuity. This is illustrated in Figure 3.6a for a holecollecting contact. Theheterojunction p–membrane can be analysed in the same fashion as the dopedp–membrane in Figure 3.2, namely by solving the electron transport equationunder the assumption that the source term Gnet is negligible and that EFpis flat. In fact, the former approximation is often much more accurate for aselective membrane with a high bandgap than for a homojunction. The assumption Gnet = 0 also means that interface defects are neglected. Of course,for a good selective contact it is vital to have as little recombinationactive interface defects as possible: the point of a selective membrane is to place a bufferbetween the electronhole pairs in the bulk and the recombinationactive metal,so if there are many interface defects at the absorber/selective membrane interface the purpose of the heterojunction is completely defeated. Achievinga low interface defect density is, however, a significant practical challenge inheterojunction solar cells.
To calculate Sn and Sn for the heterojunction in Figure 3.6, the interfacewith the metal at x = L is assumed free of resistance, though its resistancecan be added without difficulty as before. The heterojunction interface atx = L− d, on the other hand, is assumed to be resistive (as evident from thediscontinuity in EFn) and will be modelled using a TE model. For simplicity,the Anderson model [20] is used to describe the conduction band offset, so∆EC = ∆χ with ∆χ (defined positive in Figure 3.6) the difference betweenthe two electron affinities of the bulk and the p–membrane. Thus, JTE is givenby:
JTE =A∗T 2
e
[n−
NC− exp
(− ∆χ
kBT
)− n+
NC+
]=A∗T 2
e
n−
NC− exp
(− ∆χ
kBT
)[1− exp
(E+Fn − E
−Fn
kBT
)]. (3.35)
Here, quantities to the left (right) of the discontinuity at x = L−d are indicatedwith a superscript minus (plus) sign. Notice how, once more, the difference inEFn across the interface is the driver of the TE current.
102
With the thermionic emission given, Rn and Rn can be calculated:
Rn = kBTNC,bulk
A∗T 2n−(L− d)exp
(∆χ
kBT
)+
∫ L
0
1
µn(x)n(x)dx, (3.36)
Rn = kBTNC,bulk
A∗T 2n−(L− d)exp
(∆χ
kBT
)+
∫ L
0
1
µn(x)n(x)dx, (3.37)
∆χ = χbulk − χsel ≥ 0,
∆φbulk = φ(0)− φ(L− d) ≥ 0,
n(x) = NC(x)e−EC(x)−EFn(0)
kBT = NC(x)eEFn(0)+φ(x)+χ(x)
kBT ,
n(x) = NC(x)e−EC(x)−EFp(0)
kBT = NC(x)eEFp(0)+φ(x)+χ(x)
kBT .
Here, the subscript “bulk” indicates material properties of the photon absorberand the subscript “sel” is for material properties of the selective membrane.Thus, S, and S are the sum of bulk and interface resistances, indicating that theheterojunction interface indeed possesses a pointlike resistance. The pseudoor intrinsic interface resistance is calculated by assuming a straight EFn; thenfinding n or n in the absorber at the interface; then using that density to calculate the TE current going into the p–membrane (ignoring the reverse currentfrom the p–membrane into the semiconductor); and then finally dividing thatTE current by the thermal voltage.
The procedure for calculating the resistance of a selective membrane outlined in this section generalises to arbitrary stacks of materials in a straightforward fashion, provided that the underlying assumptions (1D charge transport;low generation and recombination rates in selective regions; TE transport atthe interfaces; and EFp constant) remain valid. The transport resistance fromthe bulk of the layers is taken into account by the integral in Eq. (3.36), whileeach interface adds an extra resistance that depends on its band offset ∆χ;effective Richardson constant A∗; and the pseudo density at the interface n.
It is possible to estimate the intrinsic resistance Rn of the selective contactin Figure 3.6 by making the assumption that the p–membrane has a uniformand high doping density so that almost all of the band bending occurs in thebulk of the cell. The resistance of the membrane is then the following sum ofthe interface and bulk contributions:
Rn = Rn,TE + Rn,sel, (3.38a)
Rn,TE =kBT
A∗T 2
Ndop,sel
NV,selexp
(EG,sel
kBT
), (3.38b)
Rn,sel =dNdop,sel
µn,sel n2i,sel
(3.38c)
Eqs. (3.38) demonstrate that the most important tuning parameter to suppress J0 is the bandgap of the selective membrane EG,sel, since ni,sel decreases
103
exponentially with EG,sel and also because EG,sel increases Rn in junctionswhere TE is the limiting transport process. As a rule of thumb it can be saidthat for solar cells limited by the selectivity of their contacts, the VOC increaseslinearly with the bandgap of the selective contact. However, it should not beoverlooked that the electron mobility in the p–membrane as well as its thickness have significant influence on the performance of the contact as well. Toput it a bit more strongly: if the membrane is not thick enough, it is unable tofunction as a sufficient resistance to minority carriers. The conduction bandoffset in Figure 3.6 should therefore not be merely considered as a barrier toelectrons, because this view leads to the incorrect conclusion that it is onlythe interface that provides the selectivity towards electrons. While it is truethat the interface also contributes to the electron resistance, Eqs. (3.38) showthat the interface is only part of the story and that the bulk of the selectivemembrane is equally or more important.
The previous discussion does not change much if there is also a valenceband offset such as shown in Figure 3.6b). In that case, the thickness of themembrane d should be replaced with the effective thickness deff (as shown inFigure 3.6b) in Eqs. (3.38) and the interface resistance Rn,TE needs to berevised because the band offset influences the electron density at the interface. Depending on the exact nature of the heterojunction, a large offset inthe valence band can also potentially give rise to a SCR (either in the bulk orin the selective membrane) that is resistive to the holes. Even though spacecharge regions usually do not have a significant resistance when it comes toreducing minority carrier contact recombination, in SCRs where the majoritycarriers are depleted there can be significant resistive losses because the majority carrier current needs to be high under operating conditions. Fortunately,a heterojunction contact generally gives the cell a high VOC, meaning that theinjection level in the bulk of the cell is also high. This high injection level, inturn, also leads to extra hole injection into the resistive SCR, increasing itsconductance. As can be seen, valence band offsets can be –but do not needto be– detrimental to the function of a holeselective contact and in the endit depends on the details of the cell whether or not they limit its efficiency.Unfortunately, band offsets for the majority carriers are often practical hindrances that are difficult to control, meaning that one has to engineer aroundthem.
It can be concluded that heterojunctions have significant advantages asselective membranes over homojunctions. First of all, heterojunctions havemore degrees of freedom than homojunctions to tune the selectivity of themembrane for one type of carrier, which makes it possible to keep the selectivemembranes very thin. Second of all, heterojunctions offer the possibility todecouple the optical and electrical optimisation of the selective membrane.By using a nonabsorbing material for the selective contacts, the problem ofparasitic absorption can, in principle, be solved completely. It is an extra
104
plus that the demands of transparency and selectivity both demand a materialwith a high bandgap. It should be emphasised, though, that absorption in awidebandgap selective membrane is always detrimental despite the fact thatthe electronhole pairs generated in such a widebandgap material have moreenergy than those that are generated in the bulk of the cell. The crucial pointis that the free energy of the electronhole pairs ∆ηeh is what really mattersand ∆ηeh is the largest in the bulk and decreases towards the metal contact. Aswas noted in the beginning of section this chapter, this is because the minoritycarrier quasi Fermi level bends most in the part of the cell where the minoritycarrier conductivity is lowest, i.e., in the selective membranes. Heterojunctionsare no exception to this.
The aSi:H/cSi heterojunction cell from Panasonic (which holds the current world record for cSi based technology [21]) is a good example to illustratethe advantages of heterojunctions. Most notably, this cell can achieve a goodVOC of 740 mV due to the higher selectivity of the aSi:H/cSi junction compared to an ordinary diffused junction. The wide bandgap and the low mobilityof the aSi:H are the crucial to the success of the aSi:H/cSi heterojunctioncell. Unfortunately, though, this cell is nonideal in one very important aspect,namely the optical properties of the materials: aSi:H is a direct bandgap semiconductor with a high absorption coefficient while cSi has an indirect bandgapand a low absorption coefficient. Even though the bandgap of aSi:H is largerthan that of cSi, it is not large enough to prevent significant parasitic absorption in the selective membranes [3]. The most successful method so far to dealwith this problem is to fabricate both the n–contact and the p–contact on therear of the cell, because only lowenergy photons (that are not absorbed by theaSi:H) can penetrate all the way through the cSi bulk.
3.6 Generation and recombination in selective membranes
At the beginning of Section 3.2 the assumption was made that there is nogeneration or recombination of carriers in the selective membrane, but thisassumption cannot always be made in practise. To see how generation andrecombination affect the discussion of selective contacts, a small modificationof the original problem is considered. Just like before, EFp is assumed to bestraight in the p–membrane and the electron transport equation is solved onthe interval 0 ≥ x ≥ L, with x = 0 a point in the bulk and x = L the metalcontact. The metal contact is assumed resistanceless, so that EFn is continuousat x = L.
This time, though, there is a pointlike source/sink of electrons somewherein this interval at x = a that generates/recombines an amount Jsource of electrons per unit of time. It is straightforward to solve the electron transport
105
equation on the subintervals [0, a] and [a, L] and then to patch those two solutions together. For notational convenience, the intrinsic resistance10 of asubinterval [x1, x2] ⊆ [0, L] will be denoted as:
Rn(x1, x2) =
∫ x2
x1
1
µnndx. (3.39)
The electron current flowing from the bulk into the selective membrane is then:
Jn(0) =VT
Rn(0, L)
[exp
(∆ηehkBT
)− 1
]− Jsource
1 + Rn(0,a)
Rn(a,L)
. (3.40)
In Eq. (3.40), the first term is simply the metal recombination current thatwould flow in the absence of a source/sink, while the second term shows howJsource affects the total current. Heuristically, Eq. (3.40) can be interpretedas an ordinary electrical circuit consisting of two series resistances R(0, a) andR(a, L) with a current source between them (see Figure 3.7a). This demonstrates that the intrinsic resistance behaves just like one would expect from areal resistance.
For a thermodynamic discussion of generation and recombination, it is alsouseful to calculate the Fermi level splitting at the source/sink:
EFn(a)− EFp = ∆ηeh + kBT ln
Rn(a,L)
Rn(0,a)+ e
−∆ηehkBT
(1 + JsourceRn(a,L)
VT
)1 + Rn(a,L)
Rn(0,a)
.(3.41)
As an example of how to interpret Eq. (3.40) and (3.41), consider the casewhere point a is deep within the selective membrane so that Rn(0, a) Rn(a, L). In this situation the source is essentially shielded from the bulkand only a small fraction of the source influences the current Jn(0) in the bulk.If Jsource = −Jrec < 0 acts as a recombination centre, this means that therecombination is not very detrimental to the operation of the cell, since thecarriers would have recombined in the metal anyway even if Jrec were zero.Thermodynamically speaking, the Fermi level splitting at x = a given by Eq.(3.41) is significantly less than ∆ηeh in this case so that the recombination doesnot generate much entropy. Conversely, if the recombination centre is close tothe bulk so that Rn(0, a) Rn(a, L), then Jrec adds directly to the total recombination current, giving it a significant impact on the cell performance. Inthat case, the recombination happens at a point with high Fermi level splitting.
As an alternative view, it is also possible to model the recombination as aparallel resistor as shown in Figure 3.7b. The recombination resistance Rn,rec
10For this discussion the intrinsic resistance will be used, though it is equally possible touse the pseudo resistance.
106
(a)
(b)
Figure 3.7: The equivalent circuit of the metal electron recombination current through aselective membrane with (a) a current source in the middle or (b) a parallel resistor thatmodels bulk recombination. If the recombination rate is proportional to the np product, thenthe parallel resistor in (b) is constant; otherwise it is nonohmic. Recall that the drivingforce V that is shown here for the equivalent circuit corresponds to the intrinsic resistanceand should therefore not be confused with EFn. For extra clarity it should be noted thatthese circuits only correspond to the minority electron current; the majority hole current isnot considered here.
107
is not constant for general recombination processes, but there is an importantclass of loss mechanisms that can be modelled by an ohmic resistance, namelythose where the recombination rate is proportional to the np product. To findRn,rec, the recombination current is first stated in its general form using itsrecombination parameter J0,rec and is then rewritten as follows:
Jrec = J0,rec
[np
n2i
− 1
]=
VT
Rn,rec
[exp
(EFn(a)− EFp
kBT
)− 1
]. (3.42)
Thus, Rn,rec = VT /J0,rec. The fact that Rn,rec is constant, is due to the exponential dependence on EFn(a)− EFp.
For generation in a p–membrane the discussion is similar as for recombination. If the generation takes place deep in the p–membrane (i.e., Jsource > 0and Rn(0, a) Rn(a, L)), then Eq. (3.40) shows that most of the electronsgenerated at x = a are not transported into the bulk but are lost in theholecollecting metal contact. In this case, the generation of carriers does notgenerate free energy due to the low Fermi level splitting at the source, leadingto parasitic absorption. If Rn(0, a) Rn(a, L), then the generated electronsare transported into the bulk and contribute to the power output of the cell.Perhaps surprisingly, the generation of carriers in the p–membrane has no influence on its selectivity towards carriers coming from the bulk, since thesecarriers still experience the same resistance regardless of the value of Jsource.This means that the selectivity of the contact can be discussed independentlyfrom its parasitic absorption. The exception to this rule is when Jsource is solarge that not only EFn but also EFp (and thereby Rn) gets affected by thegeneration. The high density of holes in the p–membrane makes that unlikely,though.
The main goal of Section 3.6 is to substantiate the intuition that a selective membrane can be considered as a series of resistances with sources/sinksbetween them and Eq. (3.40) expresses this idea quantitatively and succinctlyfor one source. The method outlined here can be extended in a straightforward fashion to include more than one sinks/sources separated by resistances.When this procedure is taken to the continuum limit, one essentially obtainsthe Green’s function formalism for solving the electron transport equation andthe mathematically inclined reader will perhaps recognise in Eq. (3.40) a disguised form of a Green’s function for the electron current. However, the Green’sfunction formalism will not be further developed here, since it will not help toclarify the message of this section. Moreover, the Green’s function formalism iscomplicated further by the fact that it can only provide an implicit solution forelectron transport if the recombination is a function of EFn, which is usually
108
the case11.
3.7 Conclusions
The most important conclusion from this chapter is that a cell can be dividedinto two parts with complementary functions: the photon absorber and theselective membranes. The absorber converts photons into free electrochemicalenergy and the selective membranes make sure that the electrons and holes exitthe cell through different leads so that a net electric current can flow. Thesetwo functions cannot be mixed: a photon absorber is necessarily not selectivewhile a selective membrane is necessarily less efficient at converting photonsinto electrochemical energy than the absorber. Because of this, the selectivemembrane model presents a meaningful way to divide a cell into functionalparts and to discuss the thermodynamic losses in each part, making it a usefullanguage for discussions about optimisation. As it turns out, not many newtools are necessary to do so: the familiar recombination parameter J0 can beinterpreted as a type of minority carrier resistance that is related to parametersof the selective membrane such as its thickness, mobility and bandgap andthe Richardson constants of interfaces. In many cases, this resistance can beestimated with relatively simple formulae. Furthermore, the thermodynamicview of solar cells puts a great importance on the quasi Fermi levels EFn,pthat represent the free energy of the electrons and holes. The most importantrealisation here is that free energy is simply more thermodynamically relevantthan total energy, since one can in general not expect to extract all energyfrom the cell: only free energy is available to generated work. It is thereforerecommended to start viewing thermalisation as free energy thermalisation asshown in Figure 3.3b.
Finally, because the photon absorber and the membranes have complementary functions it becomes natural to look for different materials to fulfil thesefunctions optimally. In short, the heterojunction cell is the way forward if wereally want to push the efficiency limit of solar cells.
11This situation is similar to the one where Green’s function formalism is used for solvingSchrodingers equation in quantum mechanics. See, for example, Chapter 11.4 on the Bornapproximation in Griffiths [22]
109
110
References Chapter 3
[1] Peter Wurfel. Physics of Solar Cells. WileyVCH Verlag GmbH & Co,Weinheim, 2005. ISBN 3527404287.
[2] Uli Wurfel, Andres Cuevas, and Peter Wurfel. Charge Carrier Separationin Solar Cells. IEEE Journal of Photovoltaics, 5(1):461–469, 2015. ISSN21563381. doi: 10.1109/JPHOTOV.2014.2363550.
[3] Stefaan De Wolf, Antoine Descoeudres, Zachary C. Holman, andChristophe Ballif. Highefficiency Silicon Heterojunction Solar Cells:A Review. green, 2(1):7–24, January 2012. ISSN 1869876X. doi:10.1515/green20110018.
[4] J.A. del Alamo and R.M. Swanson. The physics and modeling of heavilydoped emitters. IEEE Transactions on Electron Devices, 31(12):1878–1888, December 1984. ISSN 00189383. doi: 10.1109/TED.1984.21805.
[5] S.M. Sze and K. Ng Kwok. Physics of Semiconductor Devices. John Wiley& Sons, Inc., 2007. ISBN 97804710143239.
[6] Harald Ibach and Hans Luth. SolidState Physics. SpringerVerlag BerlinHeidelberg New York, Berlin, Heidelberg, 3 edition, 2003. doi: PhysRevB.83.165113.
[7] Xinming Li, Hongwei Zhu, Kunlin Wang, Anyuan Cao, Jinquan Wei,Chunyan Li, Yi Jia, Zhen Li, Xiao Li, and Dehai Wu. GrapheneonsiliconSchottky junction solar cells. Advanced materials (Deerfield Beach, Fla.),22(25):2743–8, July 2010. ISSN 15214095. doi: 10.1002/adma.200904383.
[8] Yu Ye and Lun Dai. Graphenebased Schottky junction solar cells. Journal of Materials Chemistry, 22(46):24224, 2012. ISSN 09599428. doi:10.1039/c2jm33809b.
[9] Yi Song, Xinming Li, Charles Mackin, Xu Zhang, Wenjing Fang, TomasPalacios, Hongwei Zhu, and Jing Kong. Role of Interfacial Oxide in HighEfficiency GrapheneSilicon Schottky Barrier Solar Cells. Nano Letters, 15(3):150225082743008, 2015. ISSN 15306984. doi: 10.1021/nl505011f.
111
[10] G. Dingemans and W. M. M. Kessels. Status and prospects of Al2O3basedsurface passivation schemes for silicon solar cells. Journal of Vacuum Science & Technology A: Vacuum, Surfaces, and Films, 30(4):040802, 2012.ISSN 07342101. doi: 10.1116/1.4728205.
[11] Rolf Brendel. Modeling solar cells with the dopantdiffused layers treatedas conductive boundaries. Progress in Photovoltaics: Research and Applications, 20(1):31–43, jan 2012. ISSN 10627995. doi: 10.1002/pip.954.
[12] Andreas Fell. A Free and Fast ThreeDimensional/TwoDimensional Solar Cell Simulator Featuring Conductive Boundary and QuasiNeutralityApproximations. IEEE Transactions on Electron Devices, 60(2):733–738,feb 2013. ISSN 00189383. doi: 10.1109/TED.2012.2231415.
[13] Dhiraj Sinha and Ji Ung Lee. Ideal Graphene/Silicon Schottky JunctionDiodes. Nano Letters, 14(8):4660–4664, aug 2014. ISSN 15306984. doi:10.1021/nl501735k.
[14] J Tersoff. Schottky Barrier Heights and the Continuum of Gap States.Physical Review Letters, 52(6):465–468, feb 1984. ISSN 00319007. doi:10.1103/PhysRevLett.52.465.
[15] Di Yan and Andres Cuevas. Empirical determination of the energy bandgap narrowing in highly doped n+ silicon. Journal of Applied Physics,114(4):044508, 2013. ISSN 00218979. doi: 10.1063/1.4816694.
[16] Di Yan and Andres Cuevas. Empirical determination of the energy bandgap narrowing in p+ silicon heavily doped with boron. Journal of Applied Physics, 116(19):194505, November 2014. ISSN 00218979. doi:10.1063/1.4902066.
[17] Richard C. Jaeger. Introduction to Microelectronic Fabrication: ModularSeries on Solid State Devices Volume V. Prentice Hall, 2 edition, 2001.ISBN 9780201444940.
[18] E. Kooi. Formation and Composition of Surface Layers and Solubility Limits of Phosphorus During Diffusion in Silicon. Journal of The Electrochemical Society, 111(12):1383, 1964. ISSN 00134651. doi: 10.1149/1.2426010.
[19] G. L. Vick and K. M. Whittle. Solid Solubility and Diffusion Coefficientsof Boron in Silicon. Journal of The Electrochemical Society, 116(8):1142,1969. ISSN 00134651. doi: 10.1149/1.2412239.
[20] R.L. Anderson. Experiments on GeGaAs heterojunctions. SolidState Electronics, 5(5):341–351, September 1962. ISSN 00381101. doi:10.1016/00381101(62)901156.
112
[21] Martin A. Green, Keith Emery, Yoshihiro Hishikawa, Wilhelm Warta,and Ewan D. Dunlop. Solar cell efficiency tables (version 46). Progress inPhotovoltaics: Research and Applications, 23(7):805–812, jul 2015. ISSN10627995. doi: 10.1002/pip.2637.
[22] David J Griffiths. Introduction to Quantum Mechanics. Pearson Education, Inc., 2nd edition, 2005. ISBN 0131911759.
113
114
Chapter 4
Variational method for theminimisation of entropygeneration in solar cells
Abstract
In this work a method is presented to extend traditional solar cell simulationtools to make it possible to calculate the most efficient design of practical solarcells. The method is based on the theory of nonequilibrium thermodynamics,which is used to derive an expression for the local entropy generation rate in thesolar cell, making it possible to quantify all free energy losses on the same scale.The framework of nonequilibrium thermodynamics can therefore be combinedwith the calculus of variations and existing solar cell models to minimise thetotal entropy generation rate in the cell to find the most optimal design. Thevariational method is illustrated by applying it to a homojunction solar cell.The optimisation results in a set of differential algebraic equations, which determine the optimal shape of the doping profile for given recombination andtransport models.
4.1 Introduction
Following the analysis of the efficiency potential of singlejunction solar cellsby Shockley and Queisser [1], the upper limit on the efficiency of solar cells hasbeen determined in literature under various idealised assumptions (see, e.g.,[2, 3, 4]). For many practical types of solar cells, however, it is still unclearhow to realise the highest possible efficiency because of the presence of specific(nonideal) loss mechanisms that limit the efficiency potential of the cell. Forexample, in solar cells based on crystalline silicon (cSi), Auger recombinationand surface recombination at the metal contacts limit the attainable efficiency
115
considerably, whereas in an ideal solar cell only radiative recombination wouldoccur. Furthermore, these nonideal loss mechanisms often have complex interactions in the cell design, making it difficult to find the optimal tradeoffbetween them. In homojunction cells, for example, the high doping densitiesin the emitter and back surface field (BSF) function to limit the recombinationat the metal contact, but simultaneously give rise to increased Auger recombination.
To aid in the practical design of these kinds of nonideal solar cells, detailed models have been developed to predict their efficiency. Programs likepc1d [5], aforshet [6], and asa [7] are all efficiencypredictive in this sense.Efficiencypredictive simulations are commonly used in parametric optimisation studies where the simulation results of the solar cell design are used toimprove the design iteratively and provide a cost efficient alternative for experimental trials. However, the parameter space for such optimisation problemscan become very large if many different parameters are optimised simultaneously. For example, to optimise the doping profile ρ(x) of a homojunction cellin complete generality, it is in principle possible to parametrise the functionρ(x) using a spline function with a high density of control nodes, but this willlead to an unfeasibly large parameter space.
The goal of this work is to introduce the designpredictive method of Variational Entropy Generation Minimisation (VEGM), which aims to circumventiterative optimisation altogether. The VEGM method extends the scope ofcurrent efficiencypredictive methods by making it possible to directly predictthe optimal solar cell design for a given set of physical constraints and nonideal loss mechanisms that depend on the materials used. The main differencewith efficiencypredictive methods is in the figure of merit used to optimisedthe solar cell. Iterative methods based on efficiencypredictive models optimisethe solar cell based on figures of merit such as the output power POut, opencircuit voltage VOC, and short circuit current JSC. These figures of merit aredetermined on the boundary of the solar cell and it is therefore often nontrivial to understand how changes to the design in the bulk of the cell willaffect POut, VOC and JSC on the boundary. The key point of the new approachis to deemphasise the importance the usual boundary figures of merit andinstead focus on the total rate of entropy production QS as a new bulk figureof merit. Unlike POut, VOC and JSC, the total rate of entropy production QS isan integral over the bulk of the cell and thus combines local information fromthe whole cell. Therefore, QS can be optimised using variational methods toimmediately predict the most efficient cell given a set of geometrical and physical constraints. In this work the EulerLagrange (EL) method will be usedto minimise QS , but in principle any variational optimisation method can beused.
The type of solar cell considered here is a device that converts blackbodyradiation from the sun into electrochemical energy (in the form of electron
116
hole pairs) and then into work (in the form of an electric current) [8]. Likeany other device that converts heat into work, the solar cell produces entropyunder operation and the more entropy it produces, the more energy is lostin the form of lowgrade heat. Therefore, the problem of maximising POut isequivalent to that of minimizing QS , which is an integral of the local entropyproduction rate qs over the domain of the cell Ω:
QS =
∫Ωqs dV. (4.1)
It is important to note that QS should be minimised under the constraints thatthe solar cell is operating at maximum power conditions under illumination,since the absolute minimum entropy generation rate is trivially QS = 0 in thedark at thermodynamic equilibrium.
Eq. (4.1) shows that qs is the central quantity that is required for thevariational optimisation of a solar cell. The expression for qs will be derivedin the following paragraphs using nonequilibrium thermodynamics, which is afield that has not found widespread use in the solar cell community. For thisreason the method of De Groot and Mazur [9] is used, which is conceptuallysimple and can be related to traditional semiconductor physics (as commonlypractised in the field of photovoltaics) with relatively little effort. A generalbackground of this method for nonequilibrium thermodynamics can also befound in the books of, e.g., Kuiken [10], Le Bellac [11], or Kjelstrup [12].General thermodynamic treatments of semiconductors physics can be found inthe works of, e.g., Lindefelt [13] and Parrott [14].
4.2 Entropy production in solar cells
To derive qs, three components from the theory of nonequilbrium thermodynamics are required: the first law of thermodynamics; the assumption oflocal thermodynamic equilibrium (LTE); and the continuity equations for theextensive variables. The derivation for qs presented below is based on the aforementioned literature sources and has been reduced to the essentials as muchas possible for the sake of accessibility.
For a solar cell in global equilibrium, the relevant thermodynamic quantitiesare: entropy S; internal energy U ; temperature T ; volume V ; the electron/holeelectrochemical potentials ηn,p; and finally the total number of electrons andholes Nn,p. The electrochemical potentials are defined as:
ηn = µcn − φ, (4.2a)
ηp = µcp + φ, (4.2b)
with µcn,p the chemical potentials for the electrons and holes, and φ the elec
trostatic energy. Because of the fundamental coupling between charge and
117
particle, ηn and ηp are the relevant thermodynamic potentials for the electrons and holes and there is no need to consider φ and µc
n,p separately [8].Related to ηn,p are the more commonly used quasiFermi energies EFn,p, givenby ηn = EFn and ηp = −EFp. It is assumed that pressure is not an importantthermodynamic quantity for a solar cell because the kinetic energy and momentum of the electrons/holes do not play a significant role in the operationof the device.
It should be noted that there is also entropy associated with the angulardistribution of the radiation field and the consideration of this distribution cantherefore also help to improve solar cells [15] and in principle it is possible tominimise the entropy generation rate of the total system consisting of the solarcell and the radiation field taken together. For this work, however, only theentropy balance of the solar cell itself will be considered and the radiation fieldwill be regarded as a source term for the processes in the semiconductor. Thissimplifying approximation is wellsuited for material systems where radiativerecombination is not the main loss mechanism, such as cSi [13].
With the quantities identified in the previous paragraph, the first law ofthermodynamics for a solar cell in global equilibrium can be stated in terms ofS:
dS =1
TdU +
−EFnT
dNn +EFpT
dNp. (4.3)
Observe that in this formulation, U , Nn, and Np are considered to be theindependent thermodynamic variables and S the fundamental potential, soS = S(U,Nn, Np). To generalise Eq. (4.3) to (nonequilibrium) operating conditions, LTE is assumed. Under this assumption, the system is divided intofinite volumes that are small enough to reach equilibrium with their surroundings on a macroscopic timescale, yet microscopically large so that they can beaccurately described by thermodynamic variables. It is furthermore assumedthat the functional form of Eq. (4.3) remains valid locally. The local form ofEq. (4.3) is stated using volumetric densities of the extensive variables, whichare indicated by a lower case letter: entropy density s, internal energy densityu, and the electron/hole densities n, p. These quantities are all dependent ontime t and position x, but these dependencies will not be stated explicitly inequations unless confusion can arise. The local form of Eq. (4.3) is therefore:
ds =1
Tdu+
−EFnT
dn+EFpT
dp. (4.4)
The densities s, u, n and p satisfy local continuity equations. Let qs,u,n,p andJs,u,n,p denote the local sources and currents of s, u, n, and p respectively.
118
Then:
∂s
∂t+∇ · Js = qs, (4.5a)
∂u
∂t+∇ · Ju = qu, (4.5b)
∂n
∂t+∇ · Jn = qn = G−R, (4.5c)
∂p
∂t+∇ · Jp = qp = G−R. (4.5d)
Here, G is the generation rate and R the recombination rate of electronholepairs. Note that Jn,p are defined as particle currents (unit: cm−2 s−1) andthat the currents Js,u,n,p are considered in the barycentric frame of the cell(so Js,u,n,p = 0 under global equilibrium conditions). To find qs, first the tderivative of Eq. (4.4) is taken:
∂s
∂t=
1
T
∂u
∂t+−EFnT
∂n
∂t+EFpT
∂p
∂t(4.6)
From Eqs. (4.5) and (4.6) the time derivatives can be eliminated. The entropy current Js can then be eliminated by using the following relation for thecurrents:1
Js =1
TJu +
−EFnT
Jn +EFpTJp. (4.7)
After rearranging, qs is then obtained:
qs =1
Tqu +
EFn − EFpT
(R−G)
+ Fu · Ju + Fn · Jn + Fp · Jp, (4.8)
In Eq. (4.8), the forces Fu,n,p are defined by Fu = ∇(1/T ), Fn = ∇(−EFn/T ),and Fp = ∇(EFp/T ). The expression for qs derived here agrees with expressions for power loss in solar cells derived in literature previously [16, 17], butalso includes thermal effects through the term Fu · Ju, which includes entropyproduction due to transport of heat. The heat flux JQ is given by
Ju = JQ + EFnJn − EFpJp, (4.9)
and can be used to rewrite Eq. (4.8) as:
Tqs = qu + (EFn − EFp)(R−G)
− ∇TT· JQ −∇EFn · Jn +∇EFp · Jp. (4.10)
1It should be noted that different arguments to obtain this expression for Js can be foundin literature. We adopt the view that the First Law in the form of Eq. (4.4) determines therelationship between the currents given in Eq. (4.7).
119
Figure 4.1: Schematic band diagram of an illuminated solar cell that illustrates the physicalprocesses corresponding to the terms in the entropy generation rate as given by Eq. (4.10). Itis assumed that the temperature in the cell is higher on the side facing the light, as indicatedby the color gradient.
Eq. (4.10) gives the source term for the entropy balance in the solar cell.The first two terms correspond to the transfer of entropy from the radiationfield to the solar cell; electronhole recombination; and the creation of entropydue to the nonradiative relaxation of electronhole pairs immediately afterthe absorption of a photon. The last three terms in Eq. (4.10) are entropyproduction terms that correspond to irreversible transport phenomena. Anoverview of the physical meaning of the terms in Eq. (4.10) is given in Figure4.1.
The Fu,n,p introduced in Eq. (4.8) are referred to as forces because theydrive the currents Ju,n,p. According to Onsager theory [18] the most generalrelation (for an isotropic medium and linear transport phenomena) betweenthe currents and forces takes the form: Ju
JnJp
=
Luu Lun LupLnu Lnn LnpLpu Lpn Lpp
FuFnFp
. (4.11)
The Lij in Eq. (4.11) are the transport coefficients for the solar cell. Onsagertheory states that the matrix L is symmetric (due to microscopic reversibility)and positivedefinite (due to the fact entropy cannot spontaneously decrease).
120
In traditional solar cell modeling, only the transport coefficients Lnn and Lpp(which are proportional to the electron and hole conductivities) are commonlyused, while the remaining transport coefficients are implicitly assumed to benegligible.
In most solar cells, recombination of electronhole pairs at the boundary ∂Ωof the cell will also contribute to the total rate of entropy generation. The surface entropy production rate QS,surf should be added to the bulk contributionand can be calculated by:
QS,surf =
∫∂Ω
EFn − EFpT
Rsurf dA. (4.12)
In Eq. (4.12), Rsurf is the surface recombination rate (in cm−2 s−1).
Eqs. (4.8) and (4.10) can be used directly to gain additional insight intosimulation results from common solar cell simulation tools such as aforshet.In order to plot power losses due to recombination and ohmic dissipation in asolar cell, it is useful to define the dissipative part of qs, which will be denotedby qdiss:
Tqdiss = (EFn − EFp)R
− ∇TT· JQ −∇EFn · Jn +∇EFp · Jp. (4.13)
Because qdiss is always positive, it can be conveniently plotted as a color mapon top of a band diagram calculation to show where the greatest losses offree energy are occurring. This is illustrated in Figure 4.2. However, it isimportant to remark that in order to optimise the solar cell completely, it isnecessary to not only minimise the total dissipation but to also make sure thatthe generation of electronhole pairs takes place in regions of the cell where theFermi level splitting is greatest, as can be seen from the term −(EFn−EFp)Gin Eq. (4.10).
It is interesting to note that for a 1 dimensional solar cell at constanttemperature and under steadystate operation, the relation between the totalentropy generation rate QS and output power POut can be obtained by directintegration. It is assumed that the electrons are extracted at x = 0 and theholes at x = d. Let eΦ = (EFn(0) − EFp(d)) (with e the elementary charge)be the voltage over the cell and J0 = e(Jp − Jn) be the total charge current(which is constant throughout the cell). Then POut = ΦJ0. The total solar
energy absorption in the solar cell will be denoted by QU =∫ d
0 qu dx. Therecombination rate at the electron contact equals Rsurf(0) = −Jp(0) and thatat the hole contact Rsurf(d) = Jn(d). Using Eqs. (4.5), (4.8), and (4.12), QS
121
Figure 4.2: Band diagram calculations (performed in aforshet) of a ptype cSi homojunction solar cell (a) with backside diffusion (BSF) and (b) without BSF. The entropyproduction rate is shown using a color map. The insets show magnifications near the surface of the cell. The BC EFn = EFp was realised by choosing a sufficiently high surfacerecombination velocity.
122
is then given by:
TQS =
∫ d
0Tqs dx+ TQS,surf
=
∫ d
0
(qu − EFnJ ′n + EFpJ
′p − E′FnJn + E′FpJp
)dx
+∑
x=0,d
[EFn(x)− EFp(x)]Rsurf(x)
= QU − ΦJ0 = QU − POut. (4.14)
Eq. (4.14) demonstrates that the minimisation of QS indeed leads to themaximisation of POut, provided that QU has been given (e.g., from opticalmodeling) or fixed in some other fashion. This again demonstrates that somecare should be taken when minimizing entropy production, since a cell in equilibrium in the dark trivially produces no entropy.
4.3 Variational solar cell optimisation
With Eqs. (4.8) and (4.11), the total entropy generation rate QS can nowbe considered as a functional that depends on all relevant solar cell variablessuch as n, p, φ etc: QS = QS [n(x), p(x), φ(x), ...]. This makes it possible tominimise QS using variational methods such as the EL method. There are,however, physical laws that need to be satisfied by the solution, so these lawsneed to be added as constraints to the optimisation procedure. In addition,other practical constraints can be imposed as well. Hence, the VEGM methodconsists of four steps:
1. The relevant unknowns are identified as well as the physical equationsthat need to be satisfied.
2. The Lagrange multiplier method is used to construct a functional Λwhich, when minimised, will lead to a solution that simultaneously minimises QS and satisfies all physical equations and additional constraints.
3. The EL method is used to find the set of differential equations for thestationarity of Λ.
4. The obtained set of equations is solved using a numerical method.
In the next paragraphs, the first three steps of the VEGM method will beillustrated by applying it to a homojunction solar cell to optimise the dopingprofile ρ(x) (expressed in cm−3). The solar cell will modelled under the assumptions commonly used in literature. This means that the device is consideredat constant temperature T (so Fu = 0) and under steadystate operation. It
123
is assumed that the boundary of the cell ∂Ω consists of perfectly passivatedsurface (meaning that Rsurf = 0) and metal contacts. At the metal contactsthe boundary condition (BC) EFn = EFp is assumed since Fermi level splittingis not possible in a metal. With these BCs, QS,surf = 0 in Eq. (4.12) and onlybulk contributions to QS need to be considered. This does, however, not meanthat recombination at the metal contacts does not generate entropy, but onlythat the entropy is generated in the bulk rather than at the contact (as can beseen in Figure 4.2).
To obtain a transport model equivalent to ordinary semiconductor physics,the offdiagonal transport coefficients in Eq. (4.11) Lun = Lnu = 0, Lup =Lpu = 0 and Lnp = Lpn = 0 are assumed negligible. Taken together, theseassumptions amount to neglecting the Seebeck and Peltier effects as well asoffdiagonal transport effects between electrons and holes. From a microscopicpoint of view, the assumption Lnp = 0 means that electronhole collisions areneglected [13]. The diagonal coefficients for charge transport are Lnn = Tnµn/eand Lpp = Tpµp/e (with µn,p the electron/hole mobilities). The mobilitiesµn,p = µn,p[ρ(x)] are assumed to depend on the doping density ρ. The localabsorption of solar heat qu is assumed known from optical modeling, as well asthe generation rate G = G(x). For recombination model R the general form
R = R(x, n, p, ρ), (4.15)
is used, indicating that R depends on n, p, and ρ as well as on x explicitly(due to, e.g., a positiondependent defect density). Furthermore, Boltzmannstatistics will be assumed, so EFn,p are related to n, p, and φ by:
n = NC exp
(EFn + χ+ φ
kT
), (4.16)
p = NV exp
(−EFp + χ+ EG + φ
kT
), (4.17)
with NC,V the effective densities of states for the conduction and valence bands,χ and EG the electron affinity and band gap (all assumed to be constant), andk the Boltzmann constant.
Next, the set of physical functions Y and transport equations Ξ that describe the solar cell are specified. The set of functions Y that will be used isgiven by: Y = n, p, φ, ρ. If the equations are stated as ξi = 0, the set ofequations Ξ = ξi is:
ξ1 = ∇ ·(−µnn
e∇EFn
)− (G−R) ,
ξ2 = ∇ ·(µppe∇EFp
)− (G−R) ,
ξ3 = ∇2φ+e2
ε(p− n+ ρ) .
124
Here, ξ1,2 are the driftdiffusion equations and ξ3 is the Poisson equation. Because ρ is considered to be an unknown, the set Ξ consists of three equations inthe four unknowns Y and is therefore underdetermined. However, the requirement that the solution minimises QS is used to make the problem wellposed.
To minimise QS subject to the constraints set by Eqs. Ξ, the followingfunctional Λ is minimised:
Λ[Y, λi] =
∫ (Tqs +
3∑i=1
λi(x)ξi
)dV
=
∫ (qu − (EFn − EFp) (G−R)−∇EFn · Jn
+∇EFp · Jp +
3∑i=1
λi(x)ξi
)dV (4.18)
The functional Λ depends on the four functions Y as well as the three scalarLagrange multiplier functions λi(x), which ensure that Eqs. Ξ are satisfied forall x ∈ Ω.
Because Λ depends on 7 scalar functions, there are also 7 EL equationsthat correspond to the stationarity requirement δΛ = 0. The 3 EL equationsfor the λi reproduce the 3 Eqs. Ξ, while the EL equations for the 4 functionsY generate 4 new equations. The latter set of 4 equations can be simplified bymaking the substitutions λ1 = λ1 − EFn and λ2 = λ2 + EFp. The resulting 4differential algebraic equations (DAEs) are:
∇ ·(µnn
e∇λ1
)= n
∂R
∂n
λ1 + λ2
kT− Jn · ∇λ1
kT− e2nλ3
εkT, (4.19a)
∇ ·(µppe∇λ2
)= p
∂R
∂p
λ1 + λ2
kT− Jp · ∇λ2
kT+e2pλ3
εkT, (4.19b)
∇ ·(µnn∇λ1 − µpp∇λ2 + e∇λ3
)= 0, (4.19c)
e2
ελ3 +
∂R
∂ρ(λ1 + λ2) =
Jn · ∇λ1
µn
∂µn∂ρ
+Jp · ∇λ2
µp
∂µp∂ρ
. (4.19d)
The BCs for the λ1,2,3 are obtained by considering the natural BCs that makeΛ stationary (see, e.g., Wan [19] and Appendix 4.A at the end of this chapter).The natural BCs depend on the BCs that have been imposed on the variablesY as well as on QS,surf . For example, if n and p are fixed at the boundaries(i.e., Dirichlet BCs) and QS,surf = 0 (as has been assumed here), the naturalBCs require that λ1 = λ2 = 0 on ∂Ω (note that these BCs are stated in termsof λ1,2 rather than λ1,2). The BCs for λ3 depend on those of φ: on boundarieswith a Dirichlet BC for φ the BC λ3 = 0 applies, while on boundaries with aNeumann BC on φ the BC n·∇λ3 = n·[2(Jn−Jp)+(µpp/e)∇λ2−(µnn/e)∇λ1]applies (with n the outward unit normal vector on ∂Ω).
125
There are 7 EL equations in 7 the functions Y and λ1,2,3, so the systemof DAEs can be solved by a numerical method to obtain the optimal shapefor ρ. This illustrates the tradeoff between parametric optimisation and thevariational method: in the VEGM method the set of differential equations islarger and has to be derived for each particular optimisation problem, but thenumerical solution has to be computed only once and the shape functions suchas ρ are optimised in complete generality rather than parametrically.
In conclusion, the framework of nonequilibrium thermodynamics offers auseful perspective for the analysis of local power losses in photovoltaic devices.By considering the entropy generation rate it becomes possible to take intoaccount electrical, optical and thermal losses and compare them on a uniformscale. The total entropy generation rate can be regarded as a functional, making it possible to optimise solar cells by taking advantage of the power of thecalculus of variations. The designpredictive method of Variational EntropyGeneration Minimisation can take advantage of detailed models for, e.g., chargecarrier recombination and mobility reduction due to semiconductor doping anduse these models to predict, e.g., the optimal doping profile for a homojunctionsolar cell. In short, the VEGM method should be considered as an extensionof the field of numerical solar cell modeling that makes it possible to find theoptimal tradeoff between the many complex loss mechanisms that occur inreal solar cells.
Acknowledgements
This work was financially supported by the Dutch Technology Foundation STW(Flash Perspectief Programma). The research of W.M.M. Kessels has beenmade possible by the Dutch Technology Foundation STW and the NetherlandsOrganisation for scientific Research (NWO, VICI programma). Furthermore,we would like to thank Dr. Stefan Bordihn for his constructive comments onthis work.
126
Appendix
4.A Boundary conditions for the VEGM method
Consider the homojunction solar cell in 1 dimension (1D) at constant T forsimplicity. The domain of the cell is the interval Ω = [0, d] and the boundaryof the cell consists of the two points ∂Ω = 0, d. The cell is described by theset of physical functions Y = n, p, φ, ρ and transport equations Ξ = ξi.This time the effect of the surface entropy generation will be accounted for ingenerality, so QS,surf 6= 0. The functional Λ then becomes:
Λ[Y, λi] =
∫ d
0
(Tqs +
3∑i=1
λi(x)ξi
)dx+ TQS,surf
=
∫ d
0
(qu − (EFn − EFp)(G−R)
− E′FnJn + E′FpJp +3∑i=1
λi(x)ξi
)dx
+∑x∈∂Ω
[EFn(x)− EFp(x)]Rsurf(x)
=
∫ d
0L(x) dx+
∑x∈∂Ω
LB(x). (4.20)
In Eq. (4.20) the symbols L and LB have been introduced. The part insideof the integral L is often referred to as the Lagrangian of the problem. Theboundary term LB will be called the boundary Lagrangian here, but sometimesit is also referred to as salvage value or terminal payoff (these terms are morecommon in variational problems in economics).
To obtain the proper BCs for the variational problem δΛ = 0, it is necessaryto consider both the first order variation of L as well as that of LB. Calculating
127
this variation gives:
δΛ =
∫ d
0
(∑y
∂L
∂yδy +
∂L
∂y′δy′ +
∂L
∂y′′δy′′ + ...
)dx
+∑x∈∂Ω
∑y
(∂LB∂y
δy +∂LB∂y′
δy′ +∂LB∂y′′
δy′′ + ...
).
(4.21)
The sum over y runs over all functions Y as well as the λi. Note that δ(y′) =(δy)′ = δy′ since the functional differential δ commutes with ordinary derivatives such as d/dx. The EL equations are obtained by repeated application ofpartial integration on the integral in Eq. (4.21) until no derivatives of the firstorder variations (i.e., δy′, δy′′ etc.) appear under the integral anymore:
δΛ =
∫ d
0
∑y
(∂L
∂y−(∂L
∂y′
)′+
(∂L
∂y′′
)′′− ...
)δy dx
+∑x∈∂Ω
∑y
[n
(∂L
∂y′−(∂L
∂y′′
)′)+∂LB∂y
]δy
+
[n∂L
∂y′′+∂LB∂y′
]δy′ + ...
(4.22)
Here, n is the 1D unit outward normal vector defined by n(0) = −1, n(d) = 1.Note that no assumptions have been made on the boundary values of δy andits derivatives yet. The requirement δΛ = 0 has consequence for both the partunder the integral and for the boundary terms. Under the integral, the firstorder variation δy can be any infinitesimal function, so in order for the integralto be zero, the prefactor of δy has to be zero for every point x. Assuming thatL does not depend on higher derivatives than y′′, the EL equations are:
d2
dx2
(∂L
∂y′′
)− d
dx
(∂L
∂y′
)+∂L
∂y= 0. (4.23)
The EL Eq. (4.23) is a necessary condition for the stationarity of Λ, but it isnot sufficient since the boundary terms in Eq. (4.22) must be zero as well. On∂Ω, all variations δy and δy′ are independent of each other. This means thatfor every term one has to choose between setting the variation equal to zero(i.e. picking a BC for y or y′) or setting the prefactor of that variation to zero.The latter choice results in a socalled natural BC.
To illustrate this, consider the boundary terms involving δn and δn′ onthe boundary x = d. It is assumed that this is the holecollecting boundary and therefore Rsurf(d) = nJn(d). Because the variations in n and n′ are
128
independent, each of the terms involving δn(d) and δn′(d) have to be zero, so:(E′Fn + λ′1 +
(λ1 + EFn − EFp)φ′
kT
)δn(d) = 0, (4.24a)
(λ1 + EFn − EFp) δn′(d) = 0. (4.24b)
Both Eqs. (4.24a) and (4.24b) have to be satisfied, but δn(d) and δn′(d) cannotbe zero simultaneously since the transport equation for n is second order. Thismeans that a choice has to be made between imposing either a Dirichlet BC forn (so δn(d) = 0) or a Neumann BC (δn′(d) = 0). A Dirichlet BC for n leadsto a natural BC for λ1 specified by Eq. (4.24b) while a Neumann BC leadsto a natural BC for λ1 specified by Eq. (4.24a). The BCs for λ3 are similarlyobtained by considering the boundary terms involving δφ and δφ′
In solar cell modeling it is often desirable to consider more general types ofBC than just Dirichlet and Neumann BCs. Such general BCs can be employedin the VEGM method by the use of Lagrange multipliers. For example, therecombination at the metal contact can be described by an effective surfacerecombination velocity Seff : Rsurf = Seff∆n. Here, ∆n is the injection level,which is approximately n at the holecollecting contact. The desired BC forelectron transport is therefore: Jn(d) = nSeff n(d). This mixed BC cannotbe used directly in the variational approach since it makes the variations inδn(d) and δn′(d) interdependent. To remedy this, the BC is enforced witha (scalar) Lagrange multiplier λn by adding the term λn[Jn(d) − nSeff n(d)]to the boundary Lagrangian LB. After that, Λ is minimised with respect toλn in addition to all the other variables, thus ensuring that the BC Jn(d) =nSeff n(d) is satisfied by the solution. The boundary terms for δn(d), δn′(d)and δλn are then: ([
φ′
kT− n
eSeffkTµn
]λn + E′Fn + λ′1
+(λ1 + EFn − EFp)φ′
kT
)δn(d) = 0 (4.25)
(λ1 + λn + EFn − EFp) δn′(d) = 0, (4.26)
(Jn − nSeff n) δλn = 0. (4.27)
In this case natural BCs have to be used to satisfy Eqs. (4.254.27), since δn(d),δn′(d) and δλn are all nonzero. From Eqs. (4.25) and (4.26) the multiplier λncan be eliminated to obtain the (mixed) BC for λ1.
129
130
References Chapter 4
[1] William Shockley and Hans J. Queisser. Detailed Balance Limit of Efficiency of pn Junction Solar Cells. J. Appl. Phys., 32(3):510, 1961. ISSN00218979. doi: 10.1063/1.1736034.
[2] C. H. Henry. Limiting efficiencies of ideal single and multiple energy gapterrestrial solar cells. J. Appl. Phys., 51(8):4494, 1980. ISSN 00218979.doi: 10.1063/1.328272.
[3] A. De Vos and H. Pauwels. On the thermodynamic limit of photovoltaicenergy conversion. Appl. Phys., 25(2):119–125, June 1981. ISSN 03403793. doi: 10.1007/BF00901283.
[4] Armin Richter, Martin Hermle, and Stefan W. Glunz. Reassessment ofthe Limiting Efficiency for Crystalline Silicon Solar Cells. IEEE J. Photovolt., 3(4):1184–1191, oct 2013. ISSN 21563381. doi: 10.1109/JPHOTOV.2013.2270351.
[5] D.A. Clugston and P.A. Basore. PC1D version 5: 32bit solar cell modelingon personal computers. In Conference Record of the Twenty Sixth IEEEPhotovoltaic Specialists Conference  1997, pages 207–210. IEEE, sep 1997.ISBN 0780337670. doi: 10.1109/PVSC.1997.654065.
[6] R. Stangl, C. Leendertz, and J. Haschke. Numerical Simulation of SolarCells and Solar Cell Characterization Methods: the OpenSource on Demand Program AFORSHET. In Radu D Rugescu, editor, Solar Energy,pages 319–352. InTech, 2010. ISBN 9789533070520.
[7] B. Pieters, J. Krc, and M. Zeman. Advanced Numerical Simulation Toolfor Solar Cells  ASA5. In 2006 IEEE 4th World Conference on Photovoltaic Energy Conference, pages 1513–1516. IEEE, 2006. ISBN 1424400163. doi: 10.1109/WCPEC.2006.279758.
[8] Peter Wurfel. Physics of Solar Cells. WileyVCH Verlag GmbH & Co,Weinheim, 2005. ISBN 3527404287.
131
[9] S.R. de Groot and Peter Mazur. Nonequilibrium Thermodynamics. DoverPublications, Mineola, New York, 1984. ISBN 0486647412.
[10] Gerard D.C. Kuiken. Thermodynamics of irreversible processes. JohnWiley & Sons, Ltd., Chichester, England, 1994. ISBN 0471948446.
[11] Michel Le Bellac, Fabrice Mortessagne, and G. George Batrouni. Equilibrium and NonEquilibrium Statistical Thermodynamics. Cambridge University Press, Cambridge, 2004. ISBN 0 521 82143 6.
[12] Signe Kjelstrup and Dick Bedeaux. NonEquilibrium Thermodynamics ofHeterogeneous Systems. World Scientific Publishing Co. Pte. Ltd., Singapore, 2008.
[13] U. Lindefelt. Heat generation in semiconductor devices. Journal of AppliedPhysics, 75:942–957, 1994. ISSN 00218979. doi: 10.1063/1.356450.
[14] J.E. Parrott. Thermodynamic theory of transport processes in semiconductors. IEEE Transactions on Electron Devices, 43, 1996. ISSN 00189383. doi: 10.1109/16.491259.
[15] Albert Polman and Harry A Atwater. Photonic design principles forultrahighefficiency photovoltaics. Nature Materials, 11(3):174–7, January2012. ISSN 14761122. doi: 10.1038/nmat3263.
[16] R. Brendel, S. Dreissigacker, N.P. Harder, and P. P. Altermatt. Theoryof analyzing free energy losses in solar cells. Applied Physics Letters, 93(17):173503, 2008. ISSN 00036951. doi: 10.1063/1.3006053.
[17] Johannes Greulich, Hannes Hoffler, Uli Wurfel, and Stefan Rein. Numerical power balance and free energy loss analysis for solar cells including optical, thermodynamic, and electrical aspects. Journal of Applied Physics,114(20):204504, 2013. ISSN 00218979. doi: 10.1063/1.4832777.
[18] Lars Onsager. Reciprocal Relations in Irreversible Processes. I. Physical Review, 37(4):405–426, February 1931. ISSN 0031899X. doi:10.1103/PhysRev.37.405.
[19] Frederick Y.M. Wan. Introduction to the calculus of variations and itsapplications. Chapman and Hall, 1995. ISBN 0412051419.
132
Chapter 5
Metaloxidebasedholeselective tunnellingcontacts for crystalline siliconsolar cells
Abstract
The goal of this work is to investigate selective hole contacts for crystalline silicon solar cells that are highly transparent, passivate the silicon surface and havelow contact resistance. Stacks of Al2O3 and ZnO films are suggested for thispurpose. The charge transport mechanism through these stacks is tunnellingrecombination and it is shown that such stacks can achieve a contact resistanceof ∼1.5 Ω cm2 for an Al2O3 thickness of 1 nm. Furthermore, it is demonstratedthat the surface passivation of such stacks can be greatly improved by the insertion of a 3 nm film of hydrogenated amorphous silicon (aSi:H) between theAl2O3 and the crystalline silicon, achieving an effective surface recombinationvelocity of ∼20 cm s−1. The stacks with an aSi:H layer achieve a contact resistance of ∼5 Ω cm2. Furthermore, from applying the theory of tunnel diodes tothe charge transport through the contact, three important elements have beenidentified for the reduction of the contact resistance: the negative fixed chargedensity in the Al2O3; the doping concentration in the ZnO; and the dielectricproperties of the Al2O3.
5.1 Introduction
In all solar cells that rely on the principle of generation of free electrons andholes, two key components can be identified: the photon absorber and the
133
selective contacts [1]. In the photon absorber, the energy of the light is converted into chemical energy in the form of electronhole pairs. This conversionis subject to the thermodynamic limit on efficiency, similarly to any other conversion of heat to a form of highergrade energy. Next, the selective contactsin the cell force the electrons to exit the absorber along a different path thanthe holes, converting the chemical energy into work by creating an electric current. In principle, the efficiency of this second conversion is not subjected tothermodynamic limitations because no heat is involved. It is the conversionfrom chemical energy to work that is the focus of the research described in thispaper.
The selective contacts in a traditional crystalline silicon (cSi) solar cell arethe diffused emitter and the back surface field (BSF). High n and pdopingdensities of these contacts result in an increase of the conductivity for onecarrier type while the conductivity for the other carrier type is simultaneouslyreduced.
In silicon heterojunction (SiHJT) solar cells, it is not just the doping inthe deposited hydrogenated amorphous silicon (aSi:H) layers that makes theemitter and rear of the cell selective to one type of carrier, but the bandalignment at the aSi:H/cSi interface plays a significant role as well [2]. Infact, higher selectivity can be achieved than with diffused junctions by tuningthe valence and conduction band offsets at the aSi:H/cSi interface, whichleads to the wellknown high VOC values of SiHJT cells [2]. One disadvantageof the aSi:H layer is that they absorb a portion of the light without convertingit into usable current, a phenomenon known as parasitic absorption [2].
The goal of our research is to investigate the possibility to create selectivecontacts by depositing stacks of selected materials on cSi. The general boundary conditions under consideration in this work (other than high selectivity toeither electrons or holes) are:
(a) The interfaces between the layers and the cSi should be well passivated toavoid surface recombination. An effective surface recombination velocityof 100 cm s−1 is considered the maximum feasible limit.
(b) The contacts should be highly transparent. The light absorption of thecontact should be less than the parasitic absorption in SiHJT solar cellsto be considered feasible.
(c) The contact resistance should be low enough to compete with currenttechnologies. Ultimately, the goal is to obtain a contact resistance on theorder of 50 mΩ cm2.
Other considerations are that the deposition methods used should be industrially scalable and the materials used should be abundant and preferablyenvironmentally friendly.
134
With these requirements in mind, stacks of Al2O3 and ZnO films are suggested to ultimately achieve these goals. The choice for Al2O3 is motivatedby the advances in recent years in silicon surface passivation by Al2O3 films,prepared by atomic layer deposition (ALD) or otherwise [3, 4], making Al2O3
a very promising material to fulfil requirement (a). The choice for ZnO isbased on the combination of its high bandgap (and thus high transparency),low resistivity and natural abundance.
In this work, the focus is on three points:
(i) To assess the potential of stacks of Al2O3 and ZnO films as passivating,transparent and selective contacts.
(ii) To gain a theoretical understanding of charge transport through thesestacks.
(iii) To find ways to improve their performance.
Point (i) is addressed in Sections 5.3.1 and 5.4.1. Section 5.3.1 will demonstrate how the negative fixed charge density at the Al2O3/cSi interface [4] canbe used to create a homojunction that separates electrons from holes. Section 5.4.1 will show the experimental results on the passivation of cSi by theAl2O3/ZnO stacks.
Point (ii) is addressed in Sections 5.3.1, 5.3.2 and 5.4.2. In Section 5.3.1 thecharge transport mechanism through the Al2O3/ZnO stacks will be identifiedas tunnelling recombination and will be discussed in more depth in Section5.3.2. Section 5.4.2 will show that the measured currents corroborate the theorypresented in Section 5.3.2.
Point (iii) is addressed in Sections 5.3.3 and 5.4.3. Section 5.3.3 will identifyfrom a theoretical perspective three key elements in the Al2O3/ZnO stacks thatinfluence the current through them and that can be optimised to reduce thetunnelling resistance. It will also discuss the potential of amorphous silicon interlayers to reduce tunnelling resistance and increase passivation. Section 5.4.3demonstrates that the passivation of the stacks can be significantly improvedby the insertion of an aSi:H interlayer between the cSi and Al2O3. The aSi:Hfilms that have been used are significantly thinner than those used in typicalSiHJT cells.
5.2 Materials and methods
Both the surface passivation and the tunnelling current investigations wereperformed on two types of stacks: Al2O3/ZnO:Al (type A) and aSi:H/Al2O3/ZnO:Al (type B). These stacks are shown in Figure 5.1a.
For the passivation study, low resistivity (∼3–4 Ω cm) ntype and ptypecSi wafers ((281.0± 1.3) µm thick) were used. The wafers were treated with
135
Figure 5.1: (a) The stack configurations of type A and type B. For the ZnO:Al films instacks of type A, various aluminium fractions (AF) are considered. For stacks of type B,AF = 0.10. (b) Schematic cross sectional view of the samples used for J–V measurements.
a diluted HF (1 % in DI–H2O) solution right before carrying out the first filmdeposition. The surface passivation was always investigated on samples withthe thin films deposited on both sides symmetrically.
The 1nmthick Al2O3 and 100nmthick ZnO:Al films were deposited using an ALD openload reactor (OpAL, Oxford Instruments). A plasma ALDprocess was used for the deposition of the Al2O3 films (Al(CH3)3,O2 plasma)at 200 C and a thermal ALD process was used to deposit the ZnO films(Zn(C2H5)2,H2O vapour) at 180 C. The ZnO films were doped with different Al concentrations by varying the ALD cycle ratio x (1 Al2O3 doping ALDcycle after every x ZnO ALD cycles). For stacks of type A, the Al doping concentration (represented as Aluminium fraction (AF)) was varied from AF = 0to 0.31; AF being defined as AF = [Al]/([Al] + [Zn]), with [Al] and [Zn] arethe atomic percentages of Al and Zn as measured by Xray photoelectron spectroscopy (XPS). For stacks of type B, AF = 0.10.
The aSi:H layers of different thicknesses (1.5–6.0 nm) were deposited at50 C by inductivelycoupled plasma chemical vapour deposition (ICPCVD)(PlasmalabSystem100 ICP 180, Oxford Instruments) using SiH4 gas.
The stacks of type A were annealed at 400 C for 5 min in a controlled N2
atmosphere before the ZnO:Al film deposition. For stacks of type B, the annealing was carried out at a lower temperature of 300 C for 1 min in a controlled N2
atmosphere to prevent loss of hydrogen in the aSi:H. The annealing was performed after the complete stack was deposited. The passivation performanceof the stacks was evaluated from the effective lifetime, τeff , of the minority carriers on the silicon wafers. τeff was determined with photoconductance decayin the transient mode and quasi steadystatemode (for τeff ≤ 100 µs) usinga Sinton lifetime tester (WCT 100). The upper level for the effective surface
136
Figure 5.2: Equilibrium band diagram of an Al2O3/ZnO stack deposited on 3 Ω cm ntypeSi. For the Si only the space charge region is shown. The red dotted band diagram showsthe sensitivity of the simulation to a variation of the band offsets. It has been simulatedusing different band offsets (red numbers between brackets) for the ZnO/Al2O3 interface andAl2O3/cSi interface.
recombination velocity (SRV), Seff,max, was extracted at an injection level of1 · 1015 cm−3 by the expression Seff,max = thickness Siwafer/2τeff . Spectroscopic Ellipsometry (SE) was employed to measure the thickness of each layerof the stacks. SE was also used to measure the optical bandgap (EG,opt) andthe carrier concentration (ne) of the ZnO:Al films using a Drude model [5].
Current density–voltage (J–V ) analysis was carried out to test the tunnelling behavior of stacks type A and type B. The front side of the tunnellingtest structure consisted of the stack under investigation and the rearside ofa 10nmthick Al2O3 single film. On both sides 2µmthick Al metal contactswith an area of 1.96 cm2 were deposited by physical vapour deposition (PVD).Subsequently, high quality p+doped contacts with a pitch of 200 µm were produced by laser firing [6] on the rear side. Figure 5.1b shows a schematic crosssection of the tunnelling samples and the stack configurations used.
137
5.3 Theory
5.3.1 The ZnO/Al2O3/cSi system as a selective contact
To demonstrate how a Al2O3 stack can function as a selective hole contact,Figure 5.2 shows the calculated band diagram of the ZnO/Al2O3/cSi system,which is based on AFORSHET simulations [7]. In the simulation, a negativefixed charge density (Qf ) of 5 · 1012 e cm−1 [4] (with e the elementary charge)has been assumed at the interface between Al2O3 and Si. The values for bandgaps and band offsets (eV) have been taken from the literature [4, 8, 9]. It isknown that there is also an SiOx layer between the Al2O3 and cSi at the interface [4]. This oxide is not included in the model explicitly, but its presence wastaken into account by using an effective dielectric constant k = 6. This is validbecause only the capacitance of the oxide interlayer has an influence on theequilibrium band diagram calculation. The SiOx/Al2O3 thickness in the modelis 5 nm. It should also be noted that the distance of the Fermi level in the ZnOto the conduction band is larger in reality than this simulated band diagramshows. This is due to the fact that AFORSHET is limited to MaxwellBoltzmann statistics, while FermiDirac statistics are needed to correctly determinethe Fermi level in a degenerate semiconductor.
The simulation demonstrates how the Al2O3/ZnO stack serves as a holeselective contact on the cSi. The high density of negative fixed charges at theinterface leads to accumulation of holes at the Al2O3/cSi interface. Similarlyto a diffused junction, in the inversion layer the conductivity for holes is muchhigher than for electrons, so the inversion layer serves as a homojunction.However, the doping is achieved without adding impurities to the silicon, thuskeeping the bulk recombination low.
If the film is thin enough, a tunnelling current through the Al2O3 is possibleby recombination of electrons from the ZnO and holes in the Si without asignificant voltage loss due to the alignment of the ZnO conduction band withthe cSi valence band. This is analogous to the case of ntype Si heterojunctionsolar cells where the ptype aSi:H is contacted with an ntype transparentconductive oxide (TCO) and the current is carried by tunnelling recombination[2, 10].
In a SiHJT cell, the hole contact consists of a stack of intrinsic and dopedaSi:H with a combined thickness of ∼10 nm [2] with on top a TCO of ∼75 nm.Therefore, compared to the SiHJT cell, the Al2O3/ZnO stack avoids the useof aSi:H, leading to a higher transparency.
5.3.2 Modeling of the tunnelling currents
From a theoretical perspective, it is expected that the tunnelling recombinationjunction behaves like an Esaki (or tunnel) diode (see Figure 5.3a) [11], rather
138
Figure 5.3: (a) The band diagram of an Esaki diode. An Esaki diode is a homojunctionwhich has been degenerately doped on both sides, making bandtoband tunnelling recombination possible. Two important parameters that characterise the diode, are the degeneracies(indicated by eVn and eVp) of the ntype and ptype sides of the junction. (b) Empirical J–Vcharacteristic of an Esaki diode (solid blue line) described by Eq. (5.1). The dashed blue lineis the current through the diode in absence of the tunnelling recombination transport, i.e.,the current predicted from the wellknown Shockley equation. The red line is the tangentV/Rt at V = 0 and indicates the ohmic behavior of the diode at low bias.
than an ideal resistor. To model the J–V characteristic of an Esaki diode inthe circuit, the following empirical relation was used [11]:
JEsaki(V ) =V
Rtexp
(− VV0
)+ J0,tunnel
[exp
(eV
kBT
)− 1
]. (5.1)
Here, kB is the Boltzmann constant and T the temperature. The variablesRt (the tunnel resistance under low bias), V0 (the voltage where J has a localmaximum) and J0,tunnel were used as fitting parameters. As can be seen inFigure 5.3b, an Esaki diodes behaves like an ohmic resistance under small forward bias. Under higher bias, the tunnelling recombination current decreasesbecause the conduction band of the ntype side of the junction is eventuallylocated completely above the valence band of the ptype side. This resultsin a characteristic region where the current through the diode decreases withthe bias, as illustrated in Figure 5.3b. This is known as “negative differentialresistance”. For even higher bias, the tunnel diode starts to function as anordinary diode and the second term in Eq. (5.1) starts to dominate, increasingthe current again.
The measured J–V data (to be presented in Section 5.4.2) of the tunnellingexperiments (described in Section 5.2) has been modelled using different circuits involving an Esaki diode. When fitting the data, it turned out thatthe tested circuits with the Esaki diode did not significantly improve the fitcompared to an ordinary double diode fit. This most likely means that thetunnel junction operates in its ohmic regime so that its contribution cannotbe separated from other contributions to the resistance. However, the model
139
of an Esaki diode is still useful for identifying the factors that can lead toimprovement of the tunnelling contact as will be shown in Section 5.3.3.
Because the effect of tunnelling recombination cannot be separated fromother series resistance contributions, the wellknown double diode equivalentcircuit is used to model the measured tunnelling currents and to assess thecontact resistance of the stacks. In the double diode fits, the ideality factors ofthe diodes were kept constant at 1 and 2, so the fits have four free parameters:the dark saturation currents of the diodes J01 and J02 (with idealities 1 and 2respectively), the shunt resistance Rshunt and the series resistance Rseries.
5.3.3 Considerations for improving the contact resistance andsurface passivation
As discussed in Section 5.3.3, the tunnelling recombination in an Esaki diodedecreases strongly when the electrons cannot recombine with holes at the sameenergy level. The underlying principle is that the recombination is most effective when energy is conserved without the need for involving a third particle(such as a phonon) [11]. Therefore, the alignment of the ZnO conduction bandwith respect to the cSi valence band is crucial for the charge transport throughthe tunnelling contact.
From a theoretical perspective, the following factors will be identified thathave influence on the alignment of these two bands: the degeneracies of thesemiconductors on both side of the junction; the band offsets at the ZnO/Al2O3
and Al2O3/cSi interfaces and the dielectric properties of the Al2O3.
5.3.3.1 Degeneracy of the ZnO and cSi
Assuming that the model of a tunnel diode applies to the tunnelling recombination current through the Al2O3 stacks, it is expected that the tunnel resistancedecreases with increasing degeneracy (i.e., the distance of the Fermi level abovethe conduction band, eVn in Figure 5.3a) of the ZnO, which is related to thecarrier concentration ne. Similarly, it is expected that an increase in the fixedcharge density in the Al2O3 will decrease the resistance by shifting up the valence band of the cSi with respect to the Fermi level and thus increasing thedegeneracy, eVp, in the cSi.
The effect of the doping in the ZnO on the degeneracy, eVn,can be measuredin various ways. First of all, an increase in eVn will increase the optical bandgapof the ZnO due to the Burstein–Moss effect. A second method to measure eVnis by the direct relation between the electron density ne and the Fermi level.If the bands of the ZnO are assumed to be parabolic, then eVn is proportional
to n2/3e . A more sophisticated approach would take the nonparabolicity of
the ZnO bands into account [12], but this requires the determination the nonparabolicity parameter of the ZnO, which is outside of the scope of this paper.
140
Another method to measure eVn is through the binding energy of electrons inthe ZnO, but this method will not be used in this work.
Both the optical bandgap and the electron density are measured by SE (seeSection 5.2). The determination of ne uses the effective mass (m∗) of the ZnOas input parameter. Generally, m∗ depends on the electron concentration (dueto the nonparabolicity of the bands), making it difficult to accurately calculateeVn from ne. Therefore, the optical bandgap is the preferred measure for eVnin this work. However, it should be noted that the change in optical bandgapcannot be attributed to the BursteinMoss shift alone since the bandgap narrows with increasing ne [13], so care must still be taken in interpreting thedata.
5.3.3.2 Band offsets in the ZnO/Al2O3/cSi system and the dielectric properties of the Al2O3
To investigate the role that the band offsets play in the ZnO/Al2O3/cSi system,the band diagram has been calculated for different values of the ZnO/Al2O3
and Al2O3/cSi band offsets. The red dotted band diagram in Figure 5.2 that issuperimposed on the original calculation shows how the band diagram changeswhen band offsets are used that are less favourable for the alignment of theZnO conduction band with respect to the cSi valence band. It can be observedthat the strength of the electric field in the Al2O3 changes significantly, butthe positions of the bands in the ZnO and cSi are not very sensitive to theband offsets used. At the interface, the cSi valence band is located 0.27 eVlower than in the original calculation, even though both band offsets have beenchanged by 0.5 eV. This illustrates that the Al2O3 fulfils an important third rolebesides inducing surface passivation and making the contact selective to holes:as a dielectric it can sustain a high amount of bandbending that facilitatesthe alignment of the ZnO conduction band and the cSi valence band. It isknown that Al2O3 layers prepared by plasma ALD have a significant breakdownelectric field of ∼9 MV cm−1 [14] and for ultrathin (∼1 nm) Al2O3 layers, valuesas high as high as ∼30 MV cm−1 have even been reported [15]. Assuminga breakdown field of ∼9 MV cm−1, this means that an energy difference of∼0.9 eV can exist across a 1 nm layer to accommodate for the alignment ofthe ZnO bands with the cSi bands. Therefore, it can be concluded that theexact values of the band offsets in the ZnO/Al2O3/cSi system will affect thetunnelling resistance through the stack, but that the effect of “misalignment”is diminished by the electric field in the Al2O3.
An interesting question is what factors determine the band offsets betweenmaterials. Knowing this will help in future research to identify other materialsthat have a high potential to make a good tunnelling contact. To answerthis question, the physical mechanism that causes band offsets needs to beaddressed. Often, band offsets are calculated using the Anderson model (also
141
known as the electron affinity rule) [11, 16], which assumes that the vacuumenergy levels of the two materials align across the interface. This assumptionleads to the equation ∆EC = e∆χ, with ∆EC the conduction band offset and∆χ the difference between electron affinities of the two materials.
However, the Anderson model is not always satisfactory for predicting bandoffsets and other models have been suggested, such as the Tersoff model [17].This model states that band offsets arise because allowed states in one semiconductor cause evanescent states in the forbidden gap of the other. This givesrise to a quantum dipole at the interface, which results in band offsets. TheTersoff model asserts that to a good approximation, the quantum dipole tendsto align the socalled branch point energies of the materials. Roughly speaking, the branch point energy of a material (which is a bulk property) is theenergy level (usually somewhere in the forbidden gap) where the (forbidden)states change from valance band character to conduction band character. Thismakes the branch point energy a useful material property for the selection ofmaterials in tunnelling stacks.
It should be noted that the Tersoff model has been applied to the ZnO/cSisystem [18, 19], but not to the ZnO/Al2O3/cSi system and, to the author’sknowledge, neither to these materials deposited by ALD.
It can be concluded that, when selecting materials for low resistance tunnelling stacks, both the electron affinity and the branch point energy of thematerials are relevant parameters for the optimization of the band alignmentof the stack. For an in depth analysis of the band offsets, detailed calculationsof the quantum dipole at the interface are recommended.
5.3.3.3 The effect of amorphous silicon interlayers
It is known that the chemical passivation of Al2O3 decreases with thickness forultrathin films (<5–10 nm) [4], so it is important to investigate ways to improvethe chemical passivation of the ultrathin Al2O3 that is needed to achieve agood tunnelling resistance. A material that is well known for its excellentchemical passivation, is aSi:H. It is therefore expected that an interlayer ofaSi:H between the Al2O3 and cSi can complement the surface passivation ofthe Al2O3.
There is, however, another motivation for the insertion of a conductiveamorphous interlayer. In the same way that tunnelling recombination is affected by the requirement for energy conservation, momentum should also beconsidered. In a crystalline material, momentum is a welldefined quantity thatis conserved, just like energy. However, in an amorphous material, momentumis not welldefined and it is expected that the insertion of an amorphous interlayer between the cSi and Al2O3 will relax the requirement for momentumconservation in the tunnelling recombination mechanism. This would be analogous to the observation that cSi has an indirect bandgap, while the relaxation
142
Table 5.1: Fitted double diode parameters for the JV characteristics (shownin Figure 5.5) of the Al2O3/ZnO:Al tunnelling stacks with various aluminiumfractions (AF), except for the sample with AF = 0.31.
AF EG,opt J01
(mA
cm2 s
)J02
(mA
cm2 s
)Rseries (Ω cm2) Rshunt (Ω cm2)
0 3.29 4.96 · 10−6 1.82 · 10−1 2.41 27.20.10 3.55 2.82 · 10−5 4.98 · 10−1 1.74 14.30.21 3.69 9.60 · 10−6 3.68 · 10−1 1.45 26.1
of momentum conservation makes aSi:H a direct bandgap semiconductor. Forthis reason, the hypothesis is advanced that a conductive amorphous interlayersuch as aSi:H will reduce the tunnelling resistance.
In principle, the same reduction of contact resistance could be obtainedif the conductive amorphous layer is inserted between the ZnO and Al2O3
instead of between the cSi and Al2O3. However, it should be noted that thesurface passivation of Al2O3 can be damaged by highenergy photons [20]. Thismakes it more difficult to achieve good surface passivation when plasmabasedmethods are used for the deposition of the amorphous layer.
5.4 Results and discussion
5.4.1 Passivation of cSi by Al2O3/ZnO stacks
The passivation results of the Al2O3/ZnO stacks are presented in Figure 5.4.As can be seen, the SRV of the stacks depends strongly on the thickness ofthe Al2O3 (dAlOx) which was varied between 1, 3 and 10 nm while the ZnOthickness was kept constant at 40 nm. When the SRV of the stack is comparedwith that of a single layer of Al2O3, it is observed that the stacks passivatebetter than the single layers for dAlOx > 3 nm and worse for dAlOx < 3 nm. AtdAlOx < 3 nm, the SRV of the stacks is ∼700 cm s−1, which is considered toohigh concerning the goal set in Section 5.1. Another observation is that thepassivation of Al2O3/ZnO stacks is mostly independent of the doping level ofthe ZnO.
More results on the passivation performance of the Al2O3/ZnO stacks arepresented in reference [21].
143
Figure 5.4: Passivation results of Al2O3/ZnO stacks on ntype silicon. The influence ofthe Al2O3 thickness is shown (left of the dashed line) as well as the influence of ZnO doping(right of the dashed line). Data marked with an asterisk (*) were performed on wafers froma different ingot.
144
Figure 5.5: Measured J–V characteristics of selected Al2O3/ZnO tunnelling samples. Thelegend shows the aluminium fraction (AF) in the ZnO as measured by XPS.
145
Figure 5.6: The fitted series resistance of the Al2O3/ZnO stacks that could be fitted as afunction of the optical bandgap of the ZnO. The dotted line is a linear fit through the datapoints and has a slope of −1.9 Ω cm2 eV−1
146
5.4.2 Charge transport through Al2O3/ZnO stacks
Measured JV curves1 for stacks with 1 nm Al2O3 and 100 nm ZnO are shownin Figure 5.5 and the parameters of the double diode fits of the curves shown inFig. 5 are in Table 5.1. Figure 5.6 shows the observed trend in the fitted seriesresistance as a function of the optical bandgap of the ZnO for all measuredsamples that could be fitted well. First of all, it should be noted that all of thesamples reach current densities higher than 43 mA cm−2 s−1 (i.e., the maximumpossible shortcircuit current for a single junction cSi solar cell under AM1.5illumination) at voltages lower than the operating voltage of a cSi solar cell.For completeness we mention that JV measurements have also been carriedout on samples with 2 nm of Al2O3, but none of these samples reached currentshigher than 10 mA cm−2 s−1. Two observations can be made from Figures. 5.5and 5.6.
First of all, the measured series resistance decreases with increasing ZnOdoping. Finite element calculations of the current flow through the ZnO havebeen used to investigate the influence of the lateral conductivity of the ZnO onthe fitted series resistance. It was found that the ZnO increases the effectivecontact area (assumed to be 1.96 cm in Figure 5.6) by approximately 10–20 %for all samples. It was also found that the observed trend in the tunnellingresistance shown in Figure 5.6 cannot be explained by the change in the ZnOsheet resistance. As can be seen, the decrease of the tunnelling resistance isobserved to be approximately linear with the optical bandgap of the ZnO,which corroborates the hypothesis advanced in Section 5.3.3.1 that the ZnOdoping improves the alignment between the ZnO conduction band and cSivalence band and therefore decreases the tunnelling resistance.
5.4.3 Improved cSi passivation by aSi:H/Al2O3/ZnO stacks
Figure 5.7 shows the passivation results and tunnel resistance of theaSi:H/Al2O3/ZnO stacks, where the thicknesses of the Al2O3 and ZnO werekept constant at 1 nm and 100 nm, respectively. The thickness of the aSi:Hwas varied between 1.5 nm and 6 nm. The parameters of the double diode fitare listed in Table 5.2. As predicted in Section 5.3.3.3, the surface passivationis already greatly enhanced by the insertion of only 1.5 nm of aSi:H. Thisrepresents a significant reduction in aSi:H thickness compared to ordinary SiHJT cells, which typically use ∼10 nm or more of aSi:H [2]. At the same time,the tunnel resistance increases slightly with aSi:H thickness.
The hypothesis from Section 5.3.3.3 that the insertion of an amorphoussilicon interlayer would decrease the tunnelling resistance has not been verified
1We would like to highlight that the JV characteristics of several samples were measuredshortly after deposition and 1 year later again. The results were very reproducible, andtherefore it can be concluded that the electric properties of these stacks are very stable intime.
147
Figure 5.7: The left axis shows the effective SRV of the aSi:H/Al2O3/ZnO stacks as afunction of the aSi:H thickness. The passivation has been determined from lifetime sampleson ptype silicon. The right axis shows the total series resistance of the tunnelling samples,determined by fitting the J–V characteristic with a double diode model.
Table 5.2: Fitted double diode parameters for the JV characteristics of theaSi:H/Al2O3/ZnO:Al tunnelling stacks. The aluminium fraction (AF) of theZnO:Al is 0.10.
aSi:H thickness (nm)
J01
(mA
cm2 s
)J02
(mA
cm2 s
)Rseries (Ω cm2) Rshunt (Ω cm2)
0 3.21 · 10−6 1.10 · 10−1 3.32 31.21.5 5.32 · 10−7 3.38 · 10−2 5.57 95.13.0 3.30 · 10−8 1.01 · 10−2 5.39 1836.0 8.04 · 10−8 1.13 · 10−3 30.8 180
148
by the experiments shown in Figure 5.7. Two factors can be advanced thatcould have played a role in the increased resistance of the samples with theaSi:H interlayer. First is the fact that these samples were annealed at a lowertemperature, most likely reducing the amount of fixed charges at the interface[4]. As explained in Section 5.3.3.1, a reduction of interface charges mostlikely leads to a higher tunnelling resistance. It is also possible that the SiOx
interlayer is thicker in the aSi:H/Al2O3/ZnO system due to different oxidationkinetics of aSi:H compared to cSi. More careful analysis of the Al2O3/aSi:Hinterface and oxide thicknesses is required to draw conclusions.
5.5 Conclusions and outlook
The potential of using Al2O3/ZnO stacks as contacts on cSi that are simultaneously holeselective, highly transparent and passivating has been addressedtheoretically and experimentally by selected measurements. Charge transportthrough these stacks is considered to occur by tunnelling recombination, whichcan be understood by applying the theory of Esaki diodes. This theory demonstrates that the ZnO conduction band should be at a lower energy than thecSi valence band in order to make the tunnelling recombination efficient andto obtain a low contact resistance. Three key elements have been identifiedthat can help to achieve the required band arrangement:
(i) The negative fixed charges in the Al2O3, which cause accumulation ofholes at the cSi surface, shifting up the cSi valence band.
(ii) The doping of the ZnO, which results in a high concentration of electrons,shifting down the ZnO conduction band.
(iii) The presence of the large bandgap dielectric Al2O3, which can sustaina large amount of band bending. This allows the ZnO and cSi bandsto align with more freedom than they would have been able to in theabsence of the Al2O3.
The influence of the doping of the ZnO on the resistance is demonstratedby the experimental observation that the contact resistance decreases withincreasing optical bandgap of the ZnO. It has been found that stacks with1 nm of Al2O3 on ptype cSi can give contact resistances of ∼1.5 Ω cm2. It wasverified that the electrical properties of the contacts are stable in time for atleast 1 year.
It has also been found that the passivation of Al2O3/ZnO stacks with 1 nmof Al2O3 is insufficient for application in high efficiency solar cells. Therefore,samples have been produced with an aSi:H interlayer between the Al2O3 andcSi in order to increase the chemical passivation. It has been demonstratedthat such interlayers can reduce Seff,max to a value as low as 20 cm s−1 while
149
still achieving a contact resistance of ∼5 Ω cm2. As the aSi:H in these stacksis significantly thinner than in a typical SiHJT cell, parasitic absorption isexpected to be reduced.
For future research, the following research directions are suggested. The aSi:H/Al2O3 interface needs to be better characterized. In particular, the fixedcharge density at this interface needs to be understood. It is also suggested tomake the Al2O3 layer as thin as possible to increase the tunnelling probability, while simultaneously making the density of negative fixed charges as highas possible. To achieve this, the growth of Al2O3 on aSi:H during the firstfew ALD cycles needs to be wellunderstood and the process tuned for thisapplication.
Another method to increase the tunnelling current through the Al2O3 is byengineering defects in the Al2O3 at a specific energy level to promote hoppingtransport through the oxide. Doing so will increase the holeselectivity of thecontact and will most likely also relax the thickness constraints on the Al2O3
so that better passivation can be achieved without introducing aSi:H in thestack.
The doping of the ZnO needs to be optimised to make the tunnelling contactas efficient as possible. ALD offers the prospect of using graded doping schemesto optimise the contact interface as well as other relevant parameters of theTCO, such as transparency and sheet resistance. It is also considered importantto start fabrication of real solar cells to test the holeselectivity of the contacts.
Acknowledgements
This work was financially supported by the Dutch Technology Foundation STW(Flash Perspectief Programma). The research of D.G.A. was funded by aMarie Curie IEF fellowship of the European Community’s Seventh FrameworkProgramme (ALD4PV, FP7MCIEF272444). The research of W.M.M.K.has been made possible by the Dutch Technology Foundation STW and theNetherlands Organization for scientific Research (NWO, VICI programma).We acknowledge financial support for this research from ADEM, A green Dealin Energy Materials of the Ministry of Economic Affairs of The Netherlands(www.ademinnovationlab.nl).
150
References Chapter 5
[1] Peter Wurfel. Physics of Solar Cells. WileyVCH Verlag GmbH & Co,Weinheim, 2005. ISBN 3527404287.
[2] Stefaan De Wolf, Antoine Descoeudres, Zachary C. Holman, andChristophe Ballif. Highefficiency Silicon Heterojunction Solar Cells:A Review. green, 2(1):7–24, January 2012. ISSN 1869876X. doi:10.1515/green20110018.
[3] Bram Hoex, S. B. S. Heil, E. Langereis, M. C. M. van de Sanden, andW. M. M. Kessels. Ultralow surface recombination of cSi substrates passivated by plasmaassisted atomic layer deposited Al2O3. Applied PhysicsLetters, 89(4):042112, 2006. ISSN 00036951. doi: 10.1063/1.2240736.
[4] G. Dingemans and W. M. M. Kessels. Status and prospects of Al2O3basedsurface passivation schemes for silicon solar cells. Journal of Vacuum Science & Technology A: Vacuum, Surfaces, and Films, 30(4):040802, 2012.ISSN 07342101. doi: 10.1116/1.4728205.
[5] S. J. Youn, T. H. Rho, B. I. Min, and Kwang S. Kim. Extended Drudemodel analysis of noble metals. physica status solidi (b), 244(4):1354–1362,April 2007. ISSN 03701972. doi: 10.1002/pssb.200642097.
[6] E. Schneiderlochner, R. Preu, R. Ludemann, and S. W. Glunz. Laserfiredrear contacts for crystalline silicon solar cells. Progress in Photovoltaics:Research and Applications, 10(1):29–34, January 2002. ISSN 10627995.doi: 10.1002/pip.422.
[7] R. Stangl, C. Leendertz, and J. Haschke. Numerical Simulation of SolarCells and Solar Cell Characterization Methods: the OpenSource on Demand Program AFORSHET. In Radu D Rugescu, editor, Solar Energy,pages 319–352. InTech, 2010. ISBN 9789533070520.
[8] Joost Jozef Hendrik Gielis, Bram Hoex, M. C. M. van de Sanden, andW. M. M. Kessels. Negative charge and charging dynamics in Al2O3 filmson Si characterized by secondharmonic generation. Journal of AppliedPhysics, 104(7):073701, 2008. ISSN 00218979. doi: 10.1063/1.2985906.
151
[9] J. B. You, X. W. Zhang, S. G. Zhang, H. R. Tan, J. Ying, Z. G. Yin,Q. S. Zhu, and Paul K. Chu. Electroluminescence behavior of ZnO/Siheterojunctions: Energy band alignment and interfacial microstructure.Journal of Applied Physics, 107(8):083701, April 2010. ISSN 00218979.doi: 10.1063/1.3385384.
[10] Ana Kanevce and Wyatt K. Metzger. The role of amorphous silicon andtunneling in heterojunction with intrinsic thin layer (HIT) solar cells.Journal of Applied Physics, 105(9):094507, 2009. ISSN 00218979. doi:10.1063/1.3106642.
[11] S.M. Sze and K. Ng Kwok. Physics of Semiconductor Devices. John Wiley& Sons, Inc., 2007. ISBN 97804710143239.
[12] T. Pisarkiewicz and A. Kolodziej. Nonparabolicity of the ConductionBand Structure in Degenerate Tin Dioxide. physica status solidi (b), 158(1):K5–K8, March 1990. ISSN 03701972. doi: 10.1002/pssb.2221580141.
[13] Anubha Jain, P. Sagar, and R.M. Mehra. Band gap widening andnarrowing in moderately and heavily doped nZnO films. SolidState Electronics, 50(78):1420–1424, July 2006. ISSN 00381101. doi:10.1016/j.sse.2006.07.001.
[14] K. B. Jinesh, J. L. van Hemmen, M. C. M. van de Sanden, F. Roozeboom,J. H. Klootwijk, W. F. a. Besling, and W. M. M. Kessels. Dielectric Properties of Thermal and PlasmaAssisted Atomic Layer Deposited Al2O3
Thin Films. Journal of The Electrochemical Society, 158(2):G21, 2011.ISSN 00134651. doi: 10.1149/1.3517430.
[15] H. C. Lin, P. D. Ye, and G. D. Wilk. Leakage current and breakdownelectricfield studies on ultrathin atomiclayerdeposited Al2O3 on GaAs.Applied Physics Letters, 87(18):182904, October 2005. ISSN 00036951.doi: 10.1063/1.2120904.
[16] R.L. Anderson. Experiments on GeGaAs heterojunctions. SolidState Electronics, 5(5):341–351, September 1962. ISSN 00381101. doi:10.1016/00381101(62)901156.
[17] J Tersoff. Theory of semiconductor heterojunctions: The role of quantumdipoles. Physical Review B, 30(8):4874–4877, October 1984. ISSN 01631829. doi: 10.1103/PhysRevB.30.4874.
[18] B Hoffling, A Schleife, C. Rodl, and F Bechstedt. Band discontinuitiesat SiTCO interfaces from quasiparticle calculations: Comparison of twoalignment approaches. Physical Review B, 85(3):035305, January 2012.ISSN 10980121. doi: 10.1103/PhysRevB.85.035305.
152
[19] Winfried Monch. Branchpoint energies and the bandstructure lineup atSchottky contacts and heterostrucures. Journal of Applied Physics, 109(11):113724, June 2011. ISSN 00218979. doi: 10.1063/1.3592978.
[20] H. B. Profijt, P. Kudlacek, M. C. M. van de Sanden, and W. M. M. Kessels.Ion and Photon Surface Interaction during Remote Plasma ALD of MetalOxides. Journal of The Electrochemical Society, 158(4):G88, 2011. ISSN00134651. doi: 10.1149/1.3552663.
[21] D. GarciaAlonso, S. Smit, S. Bordihn, and W. M. M. Kessels. Siliconpassivation and tunneling contact formation by atomic layer depositedAl2O3/ZnO stacks. Semiconductor Science and Technology, 28(8):082002,August 2013. ISSN 02681242. doi: 10.1088/02681242/28/8/082002.
153
154
Chapter 6
Properties of graphene and itspotential applications insilicon solar cells
Graphene is a relatively new material with unique electrical and optical properties, the most relevant of which –for the field of solar cells– are its highmobility combined with a low absorption coefficient. It is therefore frequentlymentioned in literature as a promising new material for cSi solar cells. In literature several devices can be found that use graphene to form a holeextractingselective contact for cSi (see, e.g., [1, 2, 3, 4, 5]). The most successful cellso far is the one made by Song et al. [5], which achieves a respectable 15.6 %efficiency with a VOC of 595 mV. However, most of the research into this typeof cell is done by researchers that are first and foremost involved in grapheneresearch rather than photovoltaics (PV) and a comprehensive overview of thestrengths and weaknesses of graphene as a material for cSi PV is therefore stillabsent. The goal of this work is therefore to answer two important questions:
1. Can graphene achieve a high enough conductivity and low enough absorption coefficient to act as a good transparent electrode in cSi cells?
2. Is graphene a suitable material for the formation of selective contactswith cSi?
These questions will be addressed as much as possible from a physics point ofview. This means that there will be less emphasis on the various devices andgraphene films that have been published in literature, since there are alreadycomprehensive reviews about these topics [3, 6, 7, 8, 9]. Instead, the relevantphysics of graphene will be discussed to develop a broad understanding of thepossibilities of graphene and to facilitate future research in this area. In Section6.1 its electronic properties will be reviewed and explained. The conductivity
155
and transparency of graphene are of special interest here and its potential asa selective electrode will be discussed. Then, in Section 6.2, the nature ofcSigraphene junctions will be explored to see what is necessary to make agood selective contact for a silicon solar cell that utilises graphene, as well asto provide practical tools to perform calculations about these types of cell.
6.1 The electrical and optical properties of graphene
Section 6.1 will give a brief overview of the properties of graphene that arerelevant for its application in solar cells. The theory has been adapted fromthe general theoretical papers on graphene by Falkovsky [10], Castro Neto etal. [11], and Abergel et al. [12].
6.1.1 The graphene dispersion relation and density of states
Graphene has two defining characteristics that give it its unique electrical andoptical properties. These characteristics are the twodimensional (2D) natureof the material and the unusual relation between energy E and momentum~k of electrons1 in the material (i.e., its dispersion relation). In most materials the dispersion relation is quadratic, meaning that the electrons in thosematerials obey a law of the form E = ~2k2/(2m∗), just like classical objectsin Newtonian mechanics. In graphene the dispersion relation is very different.For completeness sake, Figure 6.1a shows the energymomentum relation ofgraphene over the whole Brillouin zone, but in practice this full dispersion relations is seldom necessary since only the electrons near the Fermi energy areof interest for transport phenomena. As can be seen in the figure, the π andπ∗ bands (which are basically equivalent to the valence and conduction bandsin semiconductor) touch at specific points called the Kpoints or Dirac points.The momentum at these Kpoints is denoted by K. Around these Dirac pointsthe dispersion relation can be approximated to be two touching cones:
ε = ±~vFk = ±~vF√k2x + k2
y. (6.1)
Here, ε and k = κ−K are the energy and momentum measured from the Diracpoint (with κ the total momentum measured from the Γpoint). The constantvF ≈ 1 · 106 m s−1 is called the Fermi velocity of graphene. The shape of thedispersion relation in kspace is frequently referred to as the Dirac cone. Theenergy at the tip of the cone is called the Dirac energy EDirac and is located
1Because the symbol p is also used for hole density, it is preferable to use ~k for momentumto avoid confusion. Because of the equivalence between k and momentum, k will be calledthe momentum and wavenumber interchangeably.
156
4.5 eV under the vacuum level2 [14, 15]. The dispersion relation ε = ±~kvFis reminiscent of the energymomentum relation of photons E = ~kc. Likephotons, electrons in graphene have a constant (i.e., independent of energy)group velocity dω/dk = vF , which is why they are often referred to as beingmassless. The constant group velocity also is one of the properties that givegraphene its remarkable transport properties since even electrons with verylittle energy can travel at a high velocity. For comparison, an electron thattravels at 106 m s−1 in vacuum has an energy of 2.8 eV. Unlike photons, though,electrons in graphene are allowed to have energies ε < 0.
Just like in any other conductor, each electron occupies a certain volumeof phase space that is limited by the uncertainty relation. Since graphene is2D, the smallest phase space volume that an electron can occupy is given by(∆x∆k)2 = 1/(2π)2. The electrons have wave functions that extend over thearea A of the graphene so that (∆x)2 = A. By combining the uncertaintyrelation with the dispersion relation (6.1) it is possible to find the density ofstates (DOS, DG) of graphene. The DOS is measured in units of cm−2 eV−1
and is given by:
DG(ε) =2ε
π(~vF )2. (6.2)
This expression includes the spin degeneracy factor 2. With the DOS given byEq. (6.2) it becomes possible to relate the electron density to the Fermi energyof the graphene EFG. When the Fermi level is measured from the tip of theDirac cone, it is denoted by εFG = EFG − EDirac. For pure, uncontaminatedgraphene the charge neutrality point (CNP) of the Fermi level lies at the Diracpoint (i.e., at εFG = 0), so that the work function (WF) of intrinsic graphene isφG = 4.5 eV. In agreement with common conventions, all electrons occupyingstates with energy ε > 0 will be referred to as free electrons (or simply electronsif no confusion arises in a given context) while empty states with energy ε < 0will be called holes. The densities of free electrons and holes are denoted by
2Another frequently quoted value is EDirac = −4.6 eV (see, e.g., Zhong et al. [13]). In thiswork EDirac = −4.5 eV will be used, since this seems to be the most accurate experimentalvalue.
157
(a)
(b) (c)
Figure 6.1: (a) The full dispersion relation of graphene as calculated by Eq. (1) by Abergelet al. [12]. (b) On the left is shown the real space lattice of graphene. On the right onehexagon from the reciprocal space lattice of graphene is shown with the K and K’points;the four remaining corners or the hexagon are linear combinations of these two Kpoints. Itshould be recalled that a point in kspace represents a momentum or a motion. These motionsare drawn in the real space lattice using vectors of corresponding colours. As can be seen, themotions corresponding to the Kpoints are along the zigzags of atoms that provide the easiestroutes for electrons to follow. (c) The full dispersion shown in (a) can be approximated as acone at the Kpoints. The cone approximation is drawn as coloured surfaces while the exactdispersion relation is drawn as a wire frame. The energy range drawn here goes from −2 eVto 2 eV. As can be seen, the cone approximation starts to lose its accuracy at around ±1 eV.
158
nG and pG (in cm−2) and are given by:
nG =
∫ ∞EDirac
DG(E)fEFG(E) dE
=2
π
(kBT
~vF
)2 ∫ ∞0
x
1 + exp(x− εFG
kBT
) dx, (6.3a)
pG =
∫ EDirac
−∞DG(E)fEFG
(E) dE
=2
π
(kBT
~vF
)2 ∫ ∞0
x
1 + exp(x+ εFG
kBT
) dx, (6.3b)
with fEFG(E) the Fermi distribution function. At T = 300 K, the prefactor
has the value (2/π)(kBT )2/(~vF )2 = 9.82 · 1010 cm−2. Appendix 6.A discusseshow the integrals in Eqs. (6.3) can be approximated analytically and providesaccurate piecewise approximations for nG and pG in Eqs. (6.29). However, formany practical purposes it suffices to approximate the Fermi distribution as astep function to obtain the density of the dominant carriers. This density isdenoted by n (i.e., n = nG when εFG > 0 and n = pG when εFG < 0) and isgiven by:
n ≈ 1
π
(εFG
~vF
)2
≈ 7.35 · 1013 cm−2( εFG
1 eV
)2. (6.4)
This commonly used approximation has a relative error of < 10 % for εFG >5.5 kBT and an error of < 1 % for εFG > 18.1 kBT compared to the exactintegrals.
With εFG = 0 in Eqs. (6.3), the intrinsic carrier density ni,G of graphenecan be calculated to be:
ni,G =π
6
(kBT
~vF
)2
= 8.077 · 1010 cm−2. (6.5)
Note that the intrinsic carrier density is of much more interest to semiconductors than it is to graphene. In semiconductors it is possible that both theelectrons and holes follow Boltzmann statistics (i.e., when the Fermi level ismidgap) so that the law of massaction is valid: np = n2
i . However, this is notthe case for graphene since graphene is always degenerate for at least one ofthe two carrier types. So due to the fact that it does not have a bandgap thereexists no massaction law for graphene (see also the discussion about intrinsiccarrier density in doped semiconductors in Section 3.4).
From the DOS it can be seen that graphene has one forbidden energy levelat ε = 0, so it can be said that graphene almost has a bandgap. However, a
159
Figure 6.2: The (2D) Dirac cone compared to the (3D) parabolic dispersion relations of ametal and a semiconductor. In all 3 systems, the DOS is proportional to the width of thecone/parabola (though this is a happy coincidence for these particular systems and not a universal law). The Fermi level in the graphene shown in this figure corresponds to the intrinsiclevel where the numbers of free electrons and holes are equal. In graphene, like in metals,excited electrons can quickly relax back to the lowest available state by passing through intermediate empty states. In semiconductors, exited electrons relax relatively quickly to thebottom of the conduction band. Since the relaxation to the valance band involves a singlelarge jump in energy, this process is much slower than the intraband relaxation time. This isthe reason that Fermi level splitting is possible in semiconductors but not in graphene or inmetals.
160
proper semiconductor has a range of forbidden energies, so graphene is sometimes called a semimetal. Like a real metal, graphene cannot sustain Fermilevel splitting: any excited electron will quickly decay back through the intermediate states to its equilibrium energy level as shown in Figure 6.2 (seealso the discussion of Fermi level splitting in Section 3.2). This means thatgraphene is unsuited as an absorber material for solar cells. Unlike a metal,though, the Fermi level in graphene is not fixed. In a metal the DOS is verylarge at the CNP, meaning that a shift in the Fermi level will be accompaniedby a very large change in charge in the material. In intrinsic graphene, on theother hand, the DOS vanishes at the CNP so that εFG can change by a significant amount without adding much charge to it. Conversely, adding chargeto intrinsic graphene can shift εFG up or down by several tenths of an eV. Atroom temperature, for example, a Fermi level of εFG = ±kBT = 25.9 meV results in a charge of ∓1.44 ·1011 cm−2. At εFG = ±10kBT = 0.259 eV the chargeis about ∓5.1 · 1012 cm−2, which is comparable to the fixed charge density in atypical Al2O3 passivation film.
The act of shifting εFG away from its intrinsic level, thereby increasingthe carrier density, will be referred to as doping. Doping of graphene can beachieved in different ways and often happens unintentionally because the 2Dnature of the material makes it very sensitive to influences from its surroundings. For example, fixed charge can be added in the form of adsorbed ions tothe material, forcing εFG to shift to restore the charge balance. Nitric acidis a wellknown and commonly used adsorbate that can achieve ptype doping[16, 7], though it is difficult to keep ions adsorbed to the graphene permanentlydue to its chemical inertia, making chemical doping of graphene an active fieldof research [17]. Contaminating species from the environment (such as CO2,H2O and NO2 [18]) and the processing of the material are also known to causeintentional or unintentional doping [19]. The Fermi level in graphene can alsobe shifted by putting it on a dielectric substrate (such as a silicon wafer with athermal oxide film) and then gating it with an external voltage source. Whenthe dielectric is thick enough, the is configuration will behave like an ordinary(i.e., linear) capacitor so that the charge in the graphene can be calculatedfrom the gate voltage in a straightforward manner from the oxide’s thicknessand dielectric constant [20]. This method can be used to measure the adsorbedcharge density and mobility of the graphene [18] and provides a simple methodto dope graphene while performing optical measurements [21]. Another possible doping source is the substrate of the graphene itself as will be discussed inSection 6.2.
The question then rises what limits there are to graphene doping. Thoughthis question is difficult to answer, carrier densities over 1013 cm−2 [22, 23]and up to 5 · 1013 cm−2 have been observed in graphene [24]. The Diraccone approximation for the graphene dispersion relation breaks down at aboutεFG = 1 eV (see also Figure 6.1c)) and this corresponds to a carrier density
161
Table 6.1: Overview of relevant electrical properties of graphene, semiconductors and metals. In practice, metals tend to have a more complex dispersionrelation, but for the arguments in this work it is sufficient to regard metals asan ideal degenerate electron gas.
Material Dimension Bandgap Fermilevelsplitting
EF Dispersion
Graphene 2D Almost No Variable ~vFkSemiconductor 3D Yes Yes Variable ~2k2
2m∗
Metal 3D No No Fixed ~2k2
2m∗
of n = 7.4 · 1013 cm−2, so this number can be used as an approximate upperlimit for graphene doping.
Table 6.1 presents a brief overview of the most important electrical properties of graphene as well as the most important differences between graphene,metals and semiconductors.
6.1.2 Conduction and photon absorption in graphene
For assessing the electrical and optical losses in graphene, the main quantityof interest is the frequencydependent (dynamic) complex conductivity3 σ(ω).Just like the static (DC) conductance σDC = limω→0 σ(ω), the dynamic conductivity is the ratio between the inplane electric field E‖(ω) and the currentdensity (unit: A m−1) in the graphene J(ω):
J(ω) = σ(ω)E‖(ω). (6.6)
The real part of σ is associated with currents that are in phase with the electricfield (which are dissipative) while the imaginary part of σ is associated withoutofphase currents (which do not dissipate). The frequency dependenceof σ(ω) can be measured by spectroscopy (see, e.g., Horng et al. [21]; Yanet al. [23]; and Weber et al. [25]) and at wavelengths relevant for a siliconsolar cell, σ is a universal constant σAC = e2/(4~) = 6.09 · 10−5 Ω−1. Due tothe unique conical graphene dispersion relation, this constant is independentof ω; temperature; the graphene carrier density; and σDC [10]. The optical
3Because graphene is a 2D material, it is possible to measure the electrical conductivityand resistivity in S and Ω (i.e., the sheet conductance and sheet resistance). There is then noreal distinction between conductance and conductivity or between resistance and resistivityand the terms can then be used interchangeably. This is the convention that will be usedhere. Some authors (such as Weber et al. [25]) choose to express the conductivity of graphenein S m−1 by normalising to the graphene thickness dG = 0.335 nm.
162
conductivity σAC can be used to calculate the transmission through a sheetof graphene, but in general this transmission depends also on the design ofthe cell. Backside reflections from the rear of the cell and the presence ofan antireflective coating (either on top of or underneath the graphene) can allinfluence how much light the graphene absorbs and reflects. So while the opticalconductivity of graphene is a simple constant, its reflectance and transmittancedepend on the context and can in general only be calculated exactly by solvingthe Fresnel equations. Fortunately, for certain geometries there exist simpleapproximations. For example, for a sheet of graphene on a bare substrate thetransmission can be calculated to be approximately: [25]:
TsG
Ts≈ 1− πα
(1
2+
1
2(n2s + 1)
)= 1− 0.0229
(1
2+
1
2(n2s + 1)
). (6.7)
Here, the fraction TsG/Ts is the transmission through the substrate + graphenenormalised to the transmission through the substrate in the absence of thegraphene; ns is the substrate refractive index; and α ≈ 1/137.0 is the finestructure constant. Thus, for silicon (ns ≈ 3.44) the transmission loss in thevisible part of the spectrum due to the presence of a sheet of graphene is about1.2 %.
When looking at the dynamic conductivity in the lower part of the spectrum, it is possible that σ shows a feature that resembles a bandgap. Thishappens if the Fermi level is shifted far away from its intrinsic position (i.e.,εFG kBT ). In that case there are no allowed interband transitions at ω <2εFG due to a phenomenon called Pauli blocking (see Figure 6.3) and shouldnot be misinterpreted as evidence of an electrical bandgap in the graphene. Because the Pauli blocking bandgap is related to εFG, this effect provides a usefulmethod to independently measure the Fermi level and free carrier density inthe graphene.
6.1.2.1 The optical Drude response of graphene and DC conductivity
Going to even lower frequencies in the infrared (IR), the optical conductivity shows a pronounced Drude absorption peak due to intraband transitions.These intraband transitions are also referred to as free carrier scattering because they mainly involve energy levels close to the surface of the Fermi sea,which are also the states involved in DC conduction (see Figure 6.3). TheDrude contribution to σ (denoted by σDrude) has the following form [10, 21, 25]:
σDrude(ω) =iD
π(ω + iτ−1)=
ie2εFGπ~2(ω + iτ−1)
≈ ie2vF√n√
π~(ω + iτ−1). (6.8)
Here, e is the elementary charge; τ is the scattering time or inverse scatteringrate Γ−1 (Γ is also referred to as the Drude broadening parameter or scattering
163
Figure 6.3: Optical transitions in graphene. Interband transitions excite an electron withenergy ε < 0 to a state ε > 0 and are only likely if the k vector of the electron is conserved.Transitions that do not conserve k are only possible if the difference in momentum is compensated for by, e.g., a phonon and are therefore significantly less probable. Because of kconservation, only photons with energy > 2εFG can be absorbed in an interband transition.Thus, the absorption spectrum of graphene does show characteristics of an optical bandgap,even though it does not have an electrical bandgap. Intraband absorption in graphene is dominated by states close to the Fermi level because those transitions only require small changesin k. Intraband absorption therefore most pronounced in the IR part of the spectrum andleads to a characteristic Drudetype feature in the absorption spectrum. This Drude peakcan be used to measure the carrier density and mobility of the graphene [21].
164
width). The Drude weight D measures the strength of the interaction betweenthe light and the free carriers4. Strictly speaking, Eq. (6.8) is only true whenεFG kBT , but in literature a general Drude form can be found that is alsovalid at low doping levels [10].
In the ω → 0 limit, the Drude conductivity becomes the static conductivity (i.e., inverse sheet resistance) σDC = Dτ/π that measures how well thegraphene can be used as a transparent electrode. Horng et al. [21] showed thatthe sheet resistance of graphene can be successfully measured by either fourpoint probe measurements or by optically measuring the Drude weight D: bothmethods are equally accurate, but the optical method yields information aboutboth the free carrier density and the scattering rate (i.e., about the mobility).
The Drude absorption peak in the IR is of little consequence for the application of graphene in solar cells because the peak is so narrow (typically lessthan 0.3 eV) that it does not affect photons with energies above the bandgapof silicon. This is in stark contrast to traditional TCOs, in which the Drudefree carrier absorption and reflection near the silicon bandgap can be substantial. Traditional TCOs therefore have to compromise between a low resistivity(which requires a high free carrier density) and low absorption/reflection (whichrequires a low free carrier density). Only by lowering the scattering rate (andincreasing the mobility) is it possible to escape this compromise, though thedoping of a TCO will always result in ionised impurity scattering, which (together with phonon scattering) imposes an absolute upper limit on the mobilitya TCO can achieve. Indeed, for indium oxide, this upper limit has almost beenachieved [28, 29]. For graphene, on the other hand, free carrier absorption isof no consequence to a solar cell due to its very low intrinsic scattering rate;only the interband transitions matter.
It is interesting to note that the conductivity in graphene is not proportionalto n, like in most materials, but to εFG ∼
√n. To explain this dependence it
is necessary to take a closer look at the Drude model in general. This modelis commonly used to describe the conductivity of metals and semiconductors,both degenerate and nondegenerate) and provides an easy method to measurethe mobility and carrier density of a material [30]. In the Drude model the(free) electrons are considered to be an ideal gas so that the energy of theelectrons is assumed to be purely kinetic: E = ~2k2/(2m∗), with m∗ is theeffective mass of the electrons in the lattice of the material. If the electronshave an effective scattering rate τ , then the DC conductivity of the material
4In practice, it turns out that the measured Drude weight is lower than e2εFG/~2 [21].It would go too far to explain this phenomenon, but the basic idea is that, due to manybodyeffects, the scattering electrons experience a lower Fermi velocity (about 0.85 · 106 m s−1)than the DOS Fermi velocity [26, 27]
165
σDC is5 (see, e.g. [32]):
σDC = eµn =e2τ
m∗n. (6.9)
This result is very useful, but it gives the false impression that all free electronscontribute to conduction, which is only the case for a nondegenerate electrongas (such as the free electrons in lowly doped cSi). In a degenerate electron gas,however, only the electrons at the surface of the Fermi sea have the freedomto contribute to conduction. The reason n appears in Eq. (6.9) is becauseof two separate factors that together result in the proportionality σDC ∼ n.Heuristically, σDC is proportional to the number of electrons at the Fermisurface Nsurf and to their velocity (i.e. the Fermi velocity vF ):
σDC ∼ NsurfvF . (6.10)
By the same familiar argument that was used in Section 6.1.1, the electronsin a metal or semiconductor of volume V are completely delocalised. Theuncertainty principle then states:
(∆x)3(∆k)3 = V (∆k)3 =
(1
2π
)3
. (6.11)
For an ideal degenerate 3D electron gas with N particles at low temperature,the Fermi wave vector kF is given by the radius of the k sphere that containsN states. Using Eq. (6.11), kF can be calculated (taking into account the spindegeneracy of 2):
N = 2(4/3)πk3
F
∆k3=
1
3π2k3FV. (6.12)
Thus, the wellknown result kF =3√
3π2n is obtained. The same argumentcan be used to show that the number of electrons at the Fermi surface isproportional to the Fermi surface area 4πk2
F . The velocity of these surfaceelectrons is proportional to the Fermi wave vector, so Nsurf and vF scale as:
Nsurf ∼ k2F ∼ n2/3, (6.13)
vF =∂ω
∂k
∣∣∣∣E=EF
=~kFm∗∼ n1/3. (6.14)
Hence, σDC ∼ NsurfvF ∼ n as required by the Drude model, but not becauseall electrons contribute to conduction. To put it strongly: the proportionalityσDC ∼ n is merely a coincidence. There is therefore no apriori reason why
5More generally, the dynamic conductivity in the simple Drude model is σ(ω) = iσDC/(ω+iτ−1) [31].
166
σDC ∼ n should be true for graphene, which has a very different kind ofdispersion relation. Indeed, due to the linear dispersion relation ε = ~vFk ingraphene the Fermi velocity is constant and the number of electrons at theFermi surface (which is a circle rather than a spherical shell) go as Nsurf ∼kF ∼ εFG ∼
√n. Hence, the conductivity of graphene is also proportional
to εFG and√n. To derive Eq. (6.8), it is necessary to resort to calculations
based on, e.g., the Boltzmann transport equation such presented in Ibach andLuth [32], but this is not in the scope of the present work. What is importantto remember is that heavy doping of graphene is a somewhat inefficient methodto increase the conductivity because of the
√n law.
Even though the graphene DC conductivity is no longer proportional to n,it is still possible to define a (ndependent) mobility for graphene as σDC = enµ.This mobility is given by:
µ =σDC
en=
evF τ
~√πn
=ev2F τ
εFG. (6.15)
Mobility values for graphene are commonly quoted in literature, but unfortunately they can be difficult to compare due to the fact that µ is not constantwith doping. The scattering rate, on the other hand, is found to be constantwith εFG to a reasonable degree of accuracy [33], especially for ptype graphene[21], making it a convenient independent transport parameter.
Eq. (6.15) can also be compared with the common expression µ = eτ/m∗
to define an effective mass for graphene (mG) as:
εFG = mGv2F . (6.16)
Eq. (6.16) is remarkably simple to remember since it closely resembles therelativistic equation for the equivalence between mass and energy E = mc2.This result can thus be interpreted as if the electrons in the graphene havea mass determined by their energy. The mass relevant for Drude scatteringis therefore the mass equivalent to the Fermi energy, since the electrons atthe Fermi level are the ones responsible for transport phenomena. In fact,the graphene effective mass has other applications as well. For example, it isalso the effective mass that is measured in cyclotron measurements [27]. Oneshould, however, be careful to not overinterpret these ideas. The effective massmG has a very different meaning from the usual effective mass m∗ definedfor ordinary semiconductors, which is directly related to energymomentumdispersion relation.
6.1.2.2 Prospects of graphene as a transparent electrode for cSi
For a solar cell, the transmission losses through a sheet of graphene (calculatedearlier to be on the order of a percent) are on an acceptable level compared
167
to other available transparent conductors, but still significant enough that itquickly becomes unattractive to stack multiple sheets of graphene on top of oneanother (such as done by, e.g., Yan et al. [23]). This means that if graphene isused as a transparent electrode, no more than a few monolayers (and preferably just one) can be used to achieve the sheet resistance desired for the cell.It should also be kept in mind that graphene cannot act as a anti reflectivecoating (ARC) like a transparent conductive oxide (TCO) can, so the graphenewill have to be combined with a light trapping scheme; preferably one that isindustrially viable. Given the fact that it is no straightforward task to deposit materials on top of graphene (and even if it is possible, those films arelikely to degrade the graphene or at least change its properties), realising sucha scheme imposes significant practical design limitations. Mie resonators [34]are an attractive option to realise a light trapping scheme on top of graphene,since it does not require the silicon surface to be textured and only needs arelatively limited amount of the cell surface to be covered with extra materialto minimise the reflectance.
To assess the conductance potential of a single sheet graphene, it is instructive to compare the Drude theory for graphene with experimental data. In thework by Horng et al. [21], the scattering rate Γ = τ−1 and the Drude factorD have been measured optically. They found that the scatting rate Γ(ω) isapproximately constant for ptype doping, meaning that τ does not dependon the position of the Fermi level εFG. For ntype doping, however, it wasalso found that Γ(ω) increases significantly with the doping density, makingntype graphene less attractive as a transparent electrode. With these data itbecomes possible to address the question if graphene can be a good transparentelectrode. For cSi solar cells, a typical acceptable upper limit for σDC is about(100 Ω)−1 = 1.0 · 10−2 S [35].
From the work by Horng et al. it can be readily verified that as predictedby theory the Drude factor scales as D ∼ √p for pdoped graphene. In Figure6.4, their data have been fitted by plotting D2 against p. However, since D isnot a very practical number, it has been divided by πΓ0, where Γ0 = 105 cm−1
is approximately the broadening parameter they found. By doing so, the unitof the y axis becomes that of a squared sheet conductance that can be directlycompared to the conductance goal σ2
DC = 1 · 10−4 S2. As can be seen, the trendis linear and with the obtained fit it is possible to make an estimate for therequired hole density p needed to obtain the desired sheet conductance. Byextrapolating of the fit (and thus assuming that Γ remains constant), a valuep100 Ω = 2.5 · 1014 cm−2 is obtained. In practise, such a high doping densityhas not been achieved (as discussed previously in Section 6.1.1), so a scatteringwidth of 105 cm−1 is most likely too high to achieve the desired sheet resistance.However, it known that the substrate of the graphene can affect the scatteringof free carriers [36, 33] and SiO2 (the substrate used by Horng et al.) is farfrom ideal in this regard. Lower scattering rates have been found by, e.g., Yan
168
Figure 6.4: Fit of the square of the Drude factorD (expressed as a conductance (D/(πΓ0))2)against the hole concentration (assuming a constant scattering rate Γ0 = 105 cm−1). Datafrom the work by Horng et al. [21]. The blue crosses indicate data points that were excludedfrom the fit, because at low carrier densities σDC deviates from the
√p law [10]. The bands
indicate 99.9 % single observation prediction confidence intervals based on the quality of thefit. Note that the authors of the work report an approximate experimental uncertainty of10 % which is not incorporated into the fit.
169
et al. [23], who report a scattering rate of about 50 cm−1 for graphene on apolymer buffer layer. With this value of Γ the critical doping density comesdown to p = 5.6 · 1013 cm−2, which is a feasible yet still a significant amount.The question rises how much electron scattering can realistically be suppressed.According to Chen et al., [37], graphene could achieve a sheet resistance of 30 Ωat room temperature if all scattering mechanisms other than intrinsic phononscattering are absent. However, if also surface phonon interaction with an SiO2
substrate is included this limit shifts up to about 150 Ω, showing that the 100 Ωgoal relevant for solar cells is close to what is theoretically (let alone practically)feasible. Furthermore, the authors indicate that even for pristine exfoliatedgraphene cleaned and measured under ultra high vacuum conditions they stillfound a very significant amount of impurity scattering. They attribute thisto charged impurities inside of the SiO2 substrate, the electric fields of whichdisturb the transport in the graphene. This illustrates that even if it wouldbe possible to process very clean and defectfree graphene on an industrialscale, the substrate underneath the graphene can still substantially degradeits conductance. In other words, if graphene is to be used as a transparentelectrode, it is very likely that the rest of the cell needs to be engineeredaround this idea.
6.2 Junctions of graphene and silicon
Having established the basic properties of graphene, the next step is to reviewhow these properties come into play when a junction is made between grapheneand cSi (or another semiconductor similar to silicon). Superficially, such ajunction is similar to an ordinary Schottky junction in which a metal fixesthe Fermi level at the edge of the silicon and thereby induces a space chargeregion (SCR) near the interface. However, in graphene the Fermi level is notfixed so the graphene does not only affect the SCR in the cSi, but the latterwill, in turn, affect the former as well. Moreover, the behaviour of chargetransport between the two materials is expected to be different than in anordinary Schottky junction due to graphene’s unique dispersion relation andDOS.
The simplest way to illustrate the interaction between graphene and siliconis to first look at the equilibrium band diagram, which is the subject of Section6.2.1. After that, the discussion will be expanded to the nonequilibrium casein Section 6.2.2. Finally, the theory that has been presented will be used todiscuss the relevance of graphenesemiconductor (GS) junctions for the field ofsilicon photovoltaics in Section 6.2.3
170
6.2.1 Equilibrium conditions
To give a heuristic picture of a GS junction, it is useful to first consider thetwo systems separately from each other; particularly the positions of the Fermilevels of both systems. It was already discussed in Section 6.1.1 that for intrinsic graphene the Fermi level EFG is at −φG = −4.5 eV (measured from thevacuum level). In silicon the equilibrium Fermi level depends on the dopingtype and amount. If typical 3 Ω cm wafers are used, the Fermi levels for ntype and ptype silicon is at EF = −4.30 eV and EF = −4.95 eV respectively.The conduction and valence bands of silicon are at EC = −χSi = 4.05 eVand EV = −(χSi + EG,Si) = 5.17 eV, with χSi the silicon electron affinityand EG,Si = 1.124 eV the bandgap. Thus, when graphene is put directlyon silicon, the Dirac point is close to the midgap energy of silicon Emid,Si =−χSi−EG,Si/2 = −4.612 eV. Furthermore, the CNP of graphene is lower thanthe intrinsic Fermi level of ntype silicon, but higher than that of ptype silicon. When the silicon and the graphene are brought in contact, the differencein intrinsic EF will result in a temporary flow of electrons (holes) from high(low) EF to low (high) EF . Thus, ntype silicon will donate electrons to intrinsic graphene, while ptype silicon will donate holes. This redistribution ofelectrons and holes will charge the graphene and change its Fermi level, whilein the silicon a SCR will form and the bands will bend. Since the intrinsic graphene has a larger free carrier density after the charge redistribution,this effect is often referred to as substrate doping. Once equilibrium has beenreached, the surface charge in the graphene is mirrored by an opposite chargein the SCR and the Fermi level becomes constant throughout the whole structure so that no more charge flow is possible. For example, it can be calculatedthat intrinsic graphene on ntype and ptype 3 Ω cm silicon has a carrier densityof respectively nG = 5.8 · 1010 cm−2 (corresponding to εFG = 10.9 meV) andpG = 1.56 · 1011 cm−2 (corresponding to εFG = −27.8 meV).
As can be seen from the example in the previous paragraph, the grapheneacts like a surface charge that influences the semiconductor substrate underneath it. The semiconductor, in turn, influences the Fermi level in the grapheneand thereby the surface charge in the graphene. The equilibrium band diagramof a junction between a semiconductor and graphene can therefore be calculated by using the facts that the structure is globally charge neutral and thatthe Fermi level is straight (see also Zhong et al. [38]) throughout. The graphenecharge consists of the free carrier density QG,free = pG − nG as well as any adsorbed ionic species. These adsorbed ions will be referred to as chemical doping(as is common practise in literature6) and the doping density on the graphenewill be denoted by Ndop,G, which can be positive or negative and is expressedin units of cm−2. The total graphene charge is QG = QG,free + Ndop,G. It is
6Though this terminology is slightly misleading because chemical doping does not necessarily involve chemical bonds but can also be due to physisorption of ions.
171
assumed here that doping of the graphene is ideal, meaning that the dopantsare considered to be adsorbed ions that do not affect the system in any wayother than through their charge. It is also assumed that the charge state ofthe dopants is constant (i.e., the position of the Fermi level does not affect thecharge of the dopants).
To calculate an equilibrium band diagram for a general semiconductor device with a graphene layer, it is sufficient to treat the graphene as a variablesurface charge that depends on the surface potential and Fermi level of thedevice. Since most semiconductor modeling tools allow for the insertion ofsurface charges, this makes it possible to do these calculations without havingto model the graphene in more detail. To find the graphene charge QG, thefollowing procedure can be iterated:
1. First, a guess is made for the charge Qin and inserted into the devicesimulator.
2. To check if the guessQin is correct, the simulation result is used to read offthe Fermi level and the position of the conduction band EC at the surface.Next εFG in the graphene is calculated from these quantities (see alsoFigure 6.5) to obtain the corresponding surface charge Qout = pG(εFG)−nG(εFG) + Ndop,G. If the initial guess Qin was correct, then Qin = Qout
and the desired graphene charge QG has been found; otherwise a newguess needs to be made.
3. To find QG as quickly as possible, various root finding tricks can be used.For example, one can plot the pairs Qin,i, Qout,i (where i is the iterationnumber) in a graph and interpolate to find the best next guess for Qin.From experience it was found that iterating Qin,i+1 = Qout,i does notlead to quick convergence (or even to divergence) and is therefore notrecommended.
Alternatively, if the program does not support surface charge boundaryconditions (BCs), then one can guess the surface Schottky barrier Φin (i.e.,the value of EC − EF at the surface). From the simulation results it is thenpossible to deduce the surface charge from the electric field at the surface by:
Qout = −εrε0E · ne
, (6.17)
with E = −∇φ the electric field and φ the electrostatic potential (which isdefined as φ = −EVac, i.e, minus the vacuum energy level) at the surface; ε0and εr the vacuum permittivity and relative dielectric constant; and n the unitoutward normal vector7. From the obtained value of Qout the graphene Fermi
7On a 1D interval [0, L], n(L) = 1 and n(0) = −1
172
level and energy barrier Φout can be calculated and compared with Φin. Theprocedure is then iterated until the stabilising value Φin = Φout has been found.
Sometimes the only quantities of interest are the amount of band bendingin the substrate and the carrier density of the graphene. In those situationsthe integrated PoissonBoltzmann (PB) equation (Eq. (A.13) in AppendixA.2) provides a simple method for finding the correct charge balance in thestructure. The amount of charge in the semiconductor and the graphene canbe considered functions of the band bending ∆φ and the neutrality requirementcan then be used to find the value of ∆φ that satisfies:
QG(∆φ) +Qsubstrate(∆φ) = 0. (6.18)
This equation can, in general, only be solved approximately by a numericalroot finding algorithm, but since the value of ∆φ is usually between −1 eV and1 eV the root should be easy to find for a computer.
Examples are given in Figures 6.5 and 6.6, which show equilibrium banddiagrams of graphene on ntype silicon that were obtained using the integratedPB equation. In Figure 6.5 the graphene has been chemically doped ptypeby adsorbed negative ions (Ndop,G = −5 · 1012 cm−2), the charges of whichare mirrored by positive charges in both the graphene and the silicon. Thehole density in the graphene is pG = 4.9 · 1012 cm−2 here, so almost all of thenegative charge is mirrored in the graphene. In Figure 6.6 a thin Al2O3 film hasbeen inserted between the graphene and cSi and this material is known to havea high density of fixed negative charge Qf when deposited on silicon [39, 40].These charges can, in principle, also be used as a stable source of doping forgraphene. In Figure 6.6 the assumed charge density is Qf = −5 · 1012 cm−2,the same value as that for Ndop,G in Figure 6.5. However, the presence of thedielectric and the closer proximity of the fixed charges to the cSi result in alower doping of the graphene of pG = 4.1 · 1012 cm−2 and more mirror chargesin the cSi SCR.
One could ask how effective this fixed charge doping scheme for graphenecan be. Figure 6.7 shows a graph of the carrier density in graphene as afunction of the fixed charge in the dielectric for a similar configuration as inFigure 6.6. The silicon here is assumed to be an ntype 3 Ω cm wafer. As can beseen, the doping efficiency decreases sharply with the thickness of the dielectric(which has been expressed as equivalent SiO2 thickness or EOT) and with thefixed charge density, making it difficult to obtain carrier densities greater than5 · 1012 cm−2 for typical fixed charge densities Qf  < 1 · 1013 cm−2.
6.2.2 Nonequilibrium conditions
When nonequilibrium operating conditions are considered, there is no longera single, constant Fermi level throughout the whole device. In this situation, it
173
Figure 6.5: Equilibrium band diagram of graphene on silicon calculated using the integratedPB equation. The negative charge of the physisorbed ions (left, Ndop,G = −5 · 1012 cm−2) iscompensated by an induced positive charge in the graphene and silicon. It should be notedthat the graphene is represented by its Dirac cone in kspace; a convention often found inliterature. This makes the graphene readily identifiable and conveniently shows the locationof the Dirac point. The hole density in the graphene is pG = 4.9 · 1012 cm−2 in this situation,so the negative charge is mirrored mainly in the graphene.
174
Figure 6.6: Equilibrium band diagram of graphene on ntype silicon (3 Ω cm) with Al2O3
interlayer. In this situation, there is no negative charge present of the physisorbed ions,but now the fixed charges at the cSiAl2O3 interface (−5 · 1012 cm−2) act as doping for thegraphene. The thickness of the Al2O3 influences how the potential drop across the oxide∆φox, which in turn determines what fraction of Qf will be mirrored in the graphene andwhat fraction will be mirrored in the cSi. Generally, the thicker the oxide (and the lower itsεr), the greater the fraction of Qf that will be mirrored in the cSi. In this situation, the EOTof the oxide is 2 nm and the resulting carrier density in the graphene is pG = 3.5 · 1012 cm−2.Note how the cSi valence band has better alignment here with the graphene Fermi level thanin Figure 6.5 due to the potential drop across the oxide layer.
175
Figure 6.7: The graphene doping density due to the fixed oxide charge as a function of Qf .The oxide thickness was varied from an EOT of 0 nm to 10 nm. As can be seen, a thick oxidereduces the doping efficiency of the fixed charges. The asymmetry around Qf = 0 is due tothe fact that the Dirac point is not precisely midgap, which makes it easier to induce ptypedoping in the graphene. There is also a very minor second effect that stems from the factthat the substrate is an ntype wafer: it is easier for the fixed charges to nullify the (substrateinduced) ntype doping in the graphene than it is to increase it. It is this effect that shiftsthe minimum carrier density to a point slightly left of the yaxis.
176
is generally required to solve the complete set of coupled driftdiffusion equations (Eqs. (A.5) in Appendix A.1) in the device. The graphene can then bedescribed by applying the correct BCs for this set of equations. Here, a 1Dtransport problem on the interval [0, L] will be considered with the graphenelocated on the left boundary x = 0. Generally, the transport equations in thesemiconductor require three BCs at x = 0 to provide a unique solution: oneBC for the electrostatic potential φ and two BCs for the transport equationsof the electrons and holes. In addition, a fourth BC is required to fix the Fermilevel in the graphene EFG (or εFG = EFG + φ(0) + φG). Thus, the grapheneboundary consists of a system of four equations with four unknowns. As wasdiscussed in Section 6.2.1, the whole system should be globally charge neutral,meaning that one of the equations that should be imposed at x = 0 has to bethe following one:
−∇φ · n = −eQG(εFG)
ε0εr(6.19)
Eq. (6.19) is not an ordinary Neumann BC for φ (i.e., a BC that prescribes thenormal component of ∇φ), since it also involves the unknown εFG. Eq. (6.19)is therefore more accurately described as a nonlinear mixed BC.
A second BC is obtained by specifying the bias voltage over the device.For example, it can be assumed that the graphene is grounded while the otherterminal of the device is biased. The easiest way to implement a bias is bysetting Dirichlet BCs for φ(0) and φ(L), but it should be kept in mind that truethe bias over the device VB is determined by the Fermi level in the grapheneEFG and the Fermi level in the metal at the back contact EF (L) (i.e., VB =EF (L) − EFG). Since the charge in the graphene and εFG can change withthe voltage over the device, it is important to calculate the correct bias if thesimulation controls the voltage by varying φ(0) and φ(L). This is especially anissue for nearintrinsic graphene in which the Fermi level is very sensitive to thebias over the device. In doped graphene, the DOS is nonzero at the position ofthe Fermi level, making εFG less sensitive to changes in QG. Thus, the largerεFG, the more graphene behaves like a metal and the less the graphene Fermilevel is influenced by the operating conditions of the cell.
Two BCs remain to be specified at x = 0 and at this point different choicescan be made depending on the current transport model that is assumed at theGS interface. Here, two different models will be discussed: (a) the continuousquasi Fermi level (CQFL) model; and (b) the thermionic emission (TE) model.
In the CQFL model it is assumed that the electron and hole quasi Fermilevels merge together continuously in the graphene:
EFn(0) = EFG, (6.20)
EFp(0) = EFG. (6.21)
177
Figure 6.8: Sketch of a nonequilibrium band diagram of graphene on a semiconductor.The dashed boxed rectangle represents the transition region that connects domain whereordinary semiconductor physics apply from the graphene. In the transition region, EFn andEFp are continuous, but the transport coefficients Lnn and Lpp (see Section 2.6 in Chapter2) are in principle unknown. This makes an exact description of this region difficult, but byintroducing empirical parameters it is possible to incorporate the transition region throughmodified BCs on EFn,p, such as the TE BCs. These modified BCs will account for theresistance of the transition region and generally make EFn,p discontinuous at the grapheneinterface, but these discontinuities are understood to be artifacts of the modified descriptionof the interface rather than fundamental properties of EFn,p.
The advantage of the CQFL model is that it is straightforward to implement,but it has the drawback that it ignores the resistance associated with thegraphene/semiconductor interface (see Chapter 3, Section 3.3). This makesthe CQFL suitable to simulate cell designs in which the graphene interface isnot the (main) selective element on that side of the cell (i.e., when its primaryfunction is to act as a transparent electrode).
The TE model does not assume that EFn and EFp have to be continuous across the interface, so generally EFn 6= EFG and EFp 6= EFG. As wasdiscussed in Chapter 3, Section 3.3, the TE model can be interpreted as anextension of the CQFL model that includes an unknown transition region inbetween the graphene and the semiconductor. The transition region starts atx = 0 in the graphene and ends at x = d, as shown in Figure 6.8. In principle,
178
it would be possible to explicitly include the transition region in the transportphysics and in this case, the Fermi potentials would be continuous everywhereas shown in the figure. However, since the exact nature of the transition regionis unknown and not of great interest, it is integrated out and included onlyimplicitly by modifying the BCs. This then results in the TE model, whichuses empirical parameters to characterise the transition region.
For notational simplicity, we will only consider electron currents in the nextparagraph with the understanding that it follows the same line for holes. As wasdiscussed in Section 3.3, the TE model for an ordinary metalsemiconductor(MS) interface asserts that the TE current electron current JTE is given by:
eJM,S =4πem∗
h3(kBT )2 exp
(− ΦB
kBT
)= A∗T 2 exp
(− ΦB
kBT
), (6.22a)
eJS,M = A∗T 2 n
NC, (6.22b)
eJTE = A∗T 2
[exp
(EF,met + φ+ χ
kBT
)− exp
(EF,surf + φ+ χ
kBT
)]= A∗T 2 n
NC
(exp
(EF,met − EF,surf
kBT
)− 1
). (6.22c)
Note that here the current is defined as a particle current rather than a chargecurrent, hence appearance of the elementary charge e in front of the currents.In Eqs. (6.22), JM,S (JS,M) is the current from the metal into the semiconductor(and vice versa); ΦB = ΦM − χ is the Schottky barrier height (with ΦM themetal work function and χ the semiconductor electron affinity); n and NC arethe electron density and effective density of states in the semiconductor at theinterface; m∗ is the effective mass of the electrons in the semiconductor; EF,met
and EF,surf are the Fermi level in the metal and the electron Fermi level in thesemiconductor; and A∗ the effective Richardson constant. The (less common)form of the TE current across a MS interface in Eq. (6.22c) emphasises thatthe difference in Fermi level ∆EF = EF,met−EF,surf across the interface drivesthe current and that A∗ is a measure of the resistance of the interface.
The particular T 2 form of the TE prefactor J0 = A∗T 2 is due to the factthat in the derivation of the TE formulae (see, e.g. [32]) it is assumed that theelectrons in the metal form an ideal degenerate 3D electron gas with a quadraticdispersion relation ε = ~2k2/(2m∗). From that assumption one then calculatesthe number of electrons moving toward the interface that have enough energyto cross the barrier ΦB without tunnelling. In practice, the value of A∗ canbe different than the form derived from the ideal gas assumption (shown inEq. (6.22a)), since the dispersion relation in a metal is usually not perfectlyparabolic over the energy range that needs to be considered. In addition,quantum mechanical effects can lead to reflection of carriers that classicallywould cross the barrier (i.e. the opposite of tunnelling). For this reason A∗
179
should be considered as an empirical parameter that needs to be measured byexperiment.
It should be clear that the traditional TE model cannot be applied tographene straight away, since graphene has a linear dispersion relation ratherthan a quadratic one. Moreover, in graphene the electrons move in a 2D planeand have little tendency leave the plane by moving in the third, perpendiculardimension. It is therefore instructive to first consider thermionic emission fromgraphene in into the vacuum, as was done by Liang et al. [15]. They assumethat the electrons in the graphene are confined by a finite square quantum wellin the outofplane direction and find the following TE expression for vacuumemission:
eJTE,Vac = βT 3 exp
(− φG
kBT
)=ek3
BT3
π~3v2F
exp
(− φG
kBT
), (6.23)
βT 3 = 0.0285A0T2 = 3.078 · 105 A cm−2 (at T = 300 K).
Here, J0,Vac is the vacuum emission TE prefactor and A0 = 4πek2Bme/h
3 (withme the electron mass) is the unmodified Richardson constant. As can be seen,the exponential dependence on the work function from the usual Richardsonlaw is retained because the electrons that have sufficient energy to escape thegraphene satisfy Boltzmann statistics. However, the ∼ T 2 law has now beenreplaced by a ∼ T 3 law and there is no mention of an electron mass (as is appropriate for graphene). Furthermore, the thermionic emission from grapheneat low temperatures (i.e., room temperature and lower) is significantly reducedcompared to metals.
The next question is whether Eq. (6.23) is also valid for junctions between graphene and semiconductors. Experimental data by Sinha et al. [41]show that the TE current under forward bias can be significantly lower forgraphene/silicon Schottky junctions than for similar metalbased devices aslong as the interface is kept very clean. The authors propose their own Landauer model based on the assumption that electrons with a large enough energy will leave the graphene with a certain frequency τ−1. They performedtemperature dependent characterisation of the GS junctions in an attempt toprove their hypothesis, but unfortunately the current was found to be dominated by the temperature dependence in the exponent exp(−ΦB/(kBT )) so thattheir data could not distinguish between the Schottky model and the Landauermodel (i.e., both models could fit the data equally well). The exact form of thegraphene TE law should therefore be considered as an ongoing area of research.Regardless, at T = 300 K the authors obtain an effective Richardson constantof A∗ = 1.7 · 10−4A0 for their best device operating under forward bias (Figure1b in their article), meaning that their devices have even less thermionic emission than the vacuum TE current predicted by Liang et al. The results fromSinha et al. demonstrate that graphene/cSi junctions have significantly different characteristics compared to metal/cSi Schottky junctions in that the 2D
180
nature of the material makes it more difficult for charge carriers to cross froma semiconductor to graphene. In addition, part of the low TE current of GSjunctions might be explained by the low DOS of graphene at the cSi midgapenergy. At metalsemiconductor interfaces, the metal induced a large densityof defect states called MIGS (Metal Induced Gap States, see also Section 3.3)in the semiconductor forbidden gap. These MIGS lead to extra recombinationat the interface, which can also be regarded as modification of the interfaceresistance (as was demonstrated in Section 3.6 in Chapter 3). It is likely thatthe low DOS of graphene limits the number of induced defect states, whichwould translate to a lower effective TE current.
Thus, from a practical point of view, graphene can be considered as a metalas long as it is kept in mind that: a) the prefactor for the thermionic emissionlaw for graphene can be much lower than the one commonly used for metals(and can also follow a different temperature dependence); and b) the TE barrierheight of graphene is not constant but depends on the substrate, the graphenedoping and the bias of the device8.
6.2.3 Graphene as a carrier selective contact
As was already briefly discussed in Section 3.3, the low A∗ of GS junctionsmakes them a potential candidate for a selective contact, unlike regular metalSchottky junctions which are simply too lossy. In a GS junction, the interfaceis the primary carrier selective element, rather than the silicon SCR as is oftenbelieved. Based on the value A∗ = 1.7 · 10−4A0, a GS junction could reacha VOC of 750 mV (under AM1.5 illumination and if the GS junction is thelimiting factor of the cell) for a barrier height ΦB > 1.026 eV. Assuming thatthis value of A∗ is the same for both electrons and holes, such a barrier requiresa graphene electron density of nG > 9.29 · 1012 cm−2 (for an electronselectivecontact) or hole density of pG > 2.46 · 1013 cm−2 (for a holeselective contact).These are carrier densities that are well within the physically feasible limits,as long as a stable doping scheme for graphene can be found that is suitablefor solar cell applications.
Doping control of the graphene can be seen to be of great importance formaking a selective contact out of a GS junction. The doping of the graphenetunes the barrier height ΦB and thereby the selectivity of the GS interface toeither electrons or holes. It can be calculated that the respective graphenedoping densities that would achieve the VOC = 750 mV limit are Ndop,G >9.73 · 1012 cm−2 (electronselective contact) and Ndop,G < −2.50 · 1013 cm−2
(holeselective contact)9. The required doping densities are slightly higher
8This last effect is demonstrated convincingly by Sinha et al. for the reverse bias of theirdevices [41].
9The Landauer model proposed by Sinha et al. [41] yields slightly different values thanthe assumption A∗ = 1.7 · 10−4A0 (which is used in this work for simplicity) because in
181
than the required carrier densities because the SCR in the cSi also needs tobe compensated for by the doping.
Doping control of the graphene is also very important to effectively collectthe majority carriers. This is illustrated in Figure 6.9, where two holeselectiveGS contacts have been simulated under max power conditions. Figure 6.9ashows a band diagram of the GS contact with no graphene doping, while inFigure 6.9b the doping is Ndop,G = −2.50 · 1013 cm−2. An important differencebetween these two contacts is the position of the graphene Fermi level EFG:in the doped contact, EFG aligns neatly with EFp in the cSi, meaning thatthe holes are collected virtually without loss. This, incidentally, also showsthat the low A∗ value of the GS junction does not lead to a collection problemfor the majority carriers. On the other hand, in the undoped contact thereis a major mismatch of 0.41 eV between EFG and EFp, leading to significantcollection losses even though EFp is very straight in the cSi. In this case, thereare significant ohmic losses in the transition region between the graphene andcSi. The conclusion that should be drawn from these two diagrams is thatgraphene doping is not just important to make the graphene selective: evenif another source of selectivity is already present (say, an amorphous siliconheterojunction), then it is still important that the graphene’s Fermi level alignswith the majority carrier Fermi level in the cell to prevent collection losses.
6.3 Conclusions
In this chapter, the physics of graphene were discussed that are relevant tothe field of silicon PV. The unique transport properties of graphene stem fromits linear dispersion relation ε = ~vFk, which gives the electrons a constantgroup velocity so that even carriers with little energy can still contribute significantly to charge transport. As a transparent top electrode in cSi solar cells,graphene shows promise because in principle it should be possible to achieve asufficiently low sheet resistance with just a single sheet. However, to obtain agraphene sheet that is conductive enough, it is necessary to eliminate/minimiseas many scattering processes as possible, including substrate scattering. Doping of graphene also plays an important role in lowering its sheet resistance,but it should be kept in mind that in graphene the conductance is proportional to the square root of the carrier density, meaning that increasing thedoping density has diminishing returns. Furthermore, the optical propertiesof graphene make the material unsuited to be stacked several times since thiswill quickly lead to a prohibitive amount of parasitic absorption. On the bright
the Landauer model A∗ also depends on ΦB. Using their obtained value for the grapheneescape timescale τ = 4.62 · 10−11 s, the maximum required graphene doping density for aVOC of 750 mV becomes Ndop,G > 1.26 · 1013 cm−2 (electronselective contact) and Ndop,G <−2.93 · 1013 cm−2 (holeselective contact)
182
(a) (b)
Figure 6.9: Calculated band diagrams under maxpower conditions of holeselective GScontacts on ntype (3 Ω cm) silicon using the effective Richardson constant A∗ = 1.7 · 10−4A0.In (a) the graphene doping density Ndop,G is zero; in (b) it is Ndop,G = −2.50 · 1013 cm−2. Akeen eye can see that in (a) the graphene is slightly ntype in the situation without chemicaldoping due to the ntype silicon substrate doping. Both diagrams are zoomedin on the GSjunction: the rest of the cell is assumed ideal, meaning that there is no bulk recombinationand that the electronselective contact is perfectly insulating to holes. It should be noted thatthe cell in (b) indeed achieves a VOC of 750 mV, as predicted. Simulations were performed inCOMSOL Multiphysics®.
side, though, graphene’s very high mobility makes sure that free carrier absorption/reflection is completely negligible for solar cell applications, so one doesnot have to worry about the balance between parasitic absorption/reflectionand DC conductance like in a traditional TCO.
The electrical contact between graphene and a semiconductor is somewhatsimilar to a traditional MS Schottky contact. What makes graphene unique isthat its barrier height is variable and can depend on many different factors; themost important of which is the graphene doping density. Furthermore, the TElaw that describes charge transport between the semiconductor and grapheneis expected to have a different temperature dependence than the T 2 law thatapplies to MS junctions. The exact form of this TE law for GS junctions is stilluncertain, but experimental evidence suggests that the effective Richardsonconstant of a GS contact can be made so low that it could potentially be usedas a carrierselective contact for a highefficiency cSi solar cell. To achieve sucha selective contact, it is vital to use highly doped graphene, since the dopingwill both reduce the minority carrier leakage current as well as the majoritycarrier ohmic collection losses.
183
184
Appendix
6.A Approximate expressions for the graphene carrier densities
For some applications it is useful to have approximate expressions for the relation between the Fermi level in the graphene εFG and the carrier densities. Itis therefore useful to consider two limits for nG and pG, namely the limit whereεFG is large compared to kBT and the limit where εFG is on the same orderof magnitude (or smaller than) as kBT . First, suppose that εFG is large andpositive so the electrons dominate in the graphene. It is then possible to approximate the Fermi distribution function for the electrons 1/(1+e(ε−εFG)/kBT )by a step function, but a significantly more accurate approximation is obtainedby using the Sommerfeld expansion (see, e.g., Le Bellac [31]). This expansionis given by:∫ ∞
0
DG(ε)
1 + exp(ε−εFGkBT
) dε =
∫ εFG
0DG(ε) dε+
π2
6kBT
2D′G(εFG)
+O(
(kBT )4D(3)G (εFG)
), (6.24)
and provides an extra correction term for the thermal broadening of the Fermidistribution. In general, the Sommerfeld expansion can provide more than onecorrection terms, depending on how many times the DOS can be differentiatedat ε = εFG. However, since the DOS of graphene is linear, only one correctionterm can be obtained this way. The fact that there are no more correction termsdoes not mean that the Sommerfeld approximation is exact here. Instead,the discontinuity in the derivative of DG(ε) at ε = 0 is the reason that theSommerfeld formula cannot give more terms. Applying the expansion to nG
for the case εFG kBT gives:
nG(εFG) ≈ 2
π
(kBT
~vF
)2(
1
2
(εFG
kBT
)2
+π2
6
). (6.25)
Furthermore, for εFG kBT the distribution function for holes1/(1 + e(ε+εFG)/kBT ) can be approximated as an exponential by neglecting the
185
1 in the denominator, so that the approximation for pG becomes:
pG(εFG) ≈ 2
π
(kBT
~vF
)2
exp
(− εFG
kBT
)(6.26)
Of course, when εFG −kBT and the holes dominate, the same argument canbe used to show that:
nG(εFG) ≈ 2
π
(kBT
~vF
)2
exp
(εFG
kBT
), (6.27a)
pG(εFG) ≈ 2
π
(kBT
~vF
)2(
1
2
(εFG
kBT
)2
+π2
6
). (6.27b)
The Sommerfeld and exponential approximations have a relative error of < 1 %for εFG > 3kBT .
On the other hand, when εFG is small (i.e. on the order of a few kBT ), itis possible to expand nG and pG in a Taylor series around εFG = 0:
nG =2
π
(kBT
vF~
)2[π2
12+ ln(2)
εFG
kBT+
1
4
(εFG
kBT
)2
+1
24
(εFG
kBT
)3
− 1
960
(εFG
kBT
)5
+O
((εFG
kBT
)7)]
, (6.28a)
pG =2
π
(kBT
vF~
)2[π2
12− ln(2)
εFG
kBT+
1
4
(εFG
kBT
)2
− 1
24
(εFG
kBT
)3
+1
960
(εFG
kBT
)5
+O
((εFG
kBT
)7)]
, (6.28b)
In this expansion, all even orders > 2 are zero.
As can be seen, there are three approximations for nG and pG: the Sommerfeld expressions (6.25) and (6.27b) for large densities; the exponential expressions (6.26) and (6.27a) for small densities; and the Taylor expressions(6.28) for intermediate densities. These three approximations can be patchedtogether to obtain piecewise formulae for nG and pG. However, these piecewise functions can only be continuous if one uses a third order (rather than afifth order) Taylor series to patch the Taylor expression with the Sommerfeldexpression. Therefore, a reasonable approximation for nG and pG that works
186
for any value of x = εFG/kBT is:
nG =2
π
(kBT
vF~
)2
exp (x) x < −1.97π2
12 + x log(2) + x2
4 + x3
24 −x5
960 −1.97 ≤ x < 0π2
12 + x log(2) + x2
4 + x3
24 0 ≤ x < 2.50x2
2 + π2
6 2.50 ≤ x
, (6.29a)
pG =2
π
(kBT
vF~
)2
x2
2 + π2
6 x < −2.50π2
12 − x log(2) + x2
4 −x3
24 −2.50 ≤ x < 0π2
12 − x log(2) + x2
4 −x3
24 + x5
960 0 ≤ x < 1.97
exp (−x) 1.97 ≤ x
. (6.29b)
The relative errors of the piecewise approximations in Eqs. (6.29a) and (6.29b)have local maxima at the patching points x = ∓1.97 (3.4 % error) and x =±2.50 (1.7 % error). Asymptotically, the relative errors converge to zero inboth directions when x → ±∞. If greater accuracy is required, it is alwayspossible to include more terms in the Taylor series and recalculate the patchingpoints.
187
188
References Chapter 6
[1] Xinming Li, Hongwei Zhu, Kunlin Wang, Anyuan Cao, Jinquan Wei,Chunyan Li, Yi Jia, Zhen Li, Xiao Li, and Dehai Wu. GrapheneonsiliconSchottky junction solar cells. Advanced materials (Deerfield Beach, Fla.),22(25):2743–8, July 2010. ISSN 15214095. doi: 10.1002/adma.200904383.
[2] Xiaochang Miao, Sefaattin Tongay, Maureen K Petterson, Kara Berke,Andrew G Rinzler, Bill R Appleton, and Arthur F Hebard. High efficiencygraphene solar cells by chemical doping. Nano letters, 12(6):2745–50, jun2012. ISSN 15306992. doi: 10.1021/nl204414u.
[3] Yu Ye and Lun Dai. Graphenebased Schottky junction solar cells. Journal of Materials Chemistry, 22(46):24224, 2012. ISSN 09599428. doi:10.1039/c2jm33809b.
[4] Tongxiang Cui, Ruitao Lv, ZhengHong Huang, Shuxiao Chen, ZexiaZhang, Xin Gan, Yi Jia, Xinming Li, Kunlin Wang, Dehai Wu, and FeiyuKang. Enhanced efficiency of graphene/silicon heterojunction solar cellsby molecular doping. Journal of Materials Chemistry A, 1(18):5736, 2013.ISSN 20507488. doi: 10.1039/c3ta01634j.
[5] Yi Song, Xinming Li, Charles Mackin, Xu Zhang, Wenjing Fang, TomasPalacios, Hongwei Zhu, and Jing Kong. Role of Interfacial Oxide in HighEfficiency GrapheneSilicon Schottky Barrier Solar Cells. Nano Letters, 15(3):150225082743008, 2015. ISSN 15306984. doi: 10.1021/nl505011f.
[6] Xiao Huang, Zhiyuan Zeng, Zhanxi Fan, Juqing Liu, and HuaZhang. Graphenebased electrodes. Advanced materials (DeerfieldBeach, Fla.), 24(45):5979–6004, nov 2012. ISSN 15214095. doi:10.1002/adma.201201587.
[7] Gunho Jo, Minhyeok Choe, Sangchul Lee, Woojin Park, Yung Ho Kahng,and Takhee Lee. The application of graphene as electrodes in electrical and optical devices. Nanotechnology, 23(11):112001, mar 2012. doi:10.1088/09574484/23/11/112001.
189
[8] Nathan O Weiss, Hailong Zhou, Lei Liao, Yuan Liu, Shan Jiang,Yu Huang, and Xiangfeng Duan. Graphene: an emerging electronic material. Advanced materials (Deerfield Beach, Fla.), 24(43):5782–825, nov2012. ISSN 15214095. doi: 10.1002/adma.201201482.
[9] Xinming Li, Zheng Lv, and Hongwei Zhu. Carbon/Silicon HeterojunctionSolar Cells: State of the Art and Prospects. Advanced Materials, 27(42):6549–6574, nov 2015. ISSN 09359648. doi: 10.1002/adma.201502999.
[10] L. a. Falkovsky. Optical properties of graphene. Journal of Physics: Conference Series, 129:012004, oct 2008. ISSN 17426596. doi: 10.1088/17426596/129/1/012004.
[11] a. H. Castro Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, anda. K. Geim. The electronic properties of graphene. Reviews of ModernPhysics, 81(1):109–162, jan 2009. ISSN 00346861. doi: 10.1103/RevModPhys.81.109.
[12] D.S.L. Abergel, V. Apalkov, J. Berashevich, K. Ziegler, and TapashChakraborty. Properties of graphene: a theoretical perspective. Advances in Physics, 59(4):261–482, jul 2010. ISSN 00018732. doi:10.1080/00018732.2010.487978.
[13] Haijian Zhong, Ke Xu, Zhenghui Liu, Gengzhao Xu, Lin Shi, YingminFan, Jianfeng Wang, Guoqiang Ren, and Hui Yang. Charge transportmechanisms of graphene/semiconductor Schottky barriers: A theoreticaland experimental study. Journal of Applied Physics, 115(1):013701, January 2014. ISSN 00218979. doi: 10.1063/1.4859500.
[14] Kun Xu, Caifu Zeng, Qin Zhang, Rusen Yan, Peide Ye, Kang Wang,Alan C. Seabaugh, Huili Grace Xing, John S. Suehle, Curt A. Richter,David J. Gundlach, and N. V. Nguyen. Direct Measurement of DiracPoint Energy at the Graphene/Oxide Interface. Nano Letters, 13(1):131–136, jan 2013. ISSN 15306984. doi: 10.1021/nl303669w.
[15] Shijun Liang and L. K. Ang. Electron Thermionic Emission fromGraphene and a Thermionic Energy Converter. Physical Review Applied,3:1–8, 2015. ISSN 23317019. doi: 10.1103/PhysRevApplied.3.014002.
[16] Amal Kasry, Marcelo A. Kuroda, Glenn J. Martyna, George S. Tulevski,and Ageeth A. Bol. Chemical Doping of LargeArea Stacked GrapheneFilms for Use as Transparent, Conducting Electrodes. ACS Nano, 4(7):3839–3844, jul 2010. ISSN 19360851. doi: 10.1021/nn100508g.
[17] Qing Tang, Zhen Zhou, and Zhongfang Chen. Graphenerelated nanomaterials: tuning properties by functionalization. Nanoscale, 5(11):4541,2013. ISSN 20403364. doi: 10.1039/c3nr33218g.
190
[18] F Schedin, a K Geim, S V Morozov, E W Hill, P Blake, M I Katsnelson,K S Novoselov, and S V Morozov E W Hill P Blake M I Katsnelson & KS Novoselov F. Schedin A.K. Geim. Detection of individual gas moleculesadsorbed on graphene. Nature materials, 6(9):652–5, sep 2007. ISSN14761122. doi: 10.1038/nmat1967.
[19] Y.W. Tan, Y. Zhang, K. Bolotin, Y. Zhao, S. Adam, E. H. Hwang, S. DasSarma, H. L. Stormer, and P. Kim. Measurement of Scattering Rate andMinimum Conductivity in Graphene. Physical Review Letters, 99(24):246803, dec 2007. ISSN 00319007. doi: 10.1103/PhysRevLett.99.246803.
[20] K. S. Novoselov. Electric Field Effect in Atomically Thin Carbon Films.Science, 306(5696):666–669, oct 2004. ISSN 00368075. doi: 10.1126/science.1102896.
[21] Jason Horng, Chi Fan Chen, Baisong Geng, Caglar Girit, Yuanbo Zhang,Zhao Hao, Hans a. Bechtel, Michael Martin, Alex Zettl, Michael F.Crommie, Y. Ron Shen, and Feng Wang. Drude conductivity of Diracfermions in graphene. Physical Review B  Condensed Matter and Materials Physics, 83(16):1–5, 2011. ISSN 10980121. doi: 10.1103/PhysRevB.83.165113.
[22] Henry Medina, Yung Chang Lin, Dirk Obergfell, and Po W. Chiu. Tuning of charge densities in graphene by molecule doping. Advanced Functional Materials, 21(14):2687–2692, jul 2011. ISSN 1616301X. doi:10.1002/adfm.201100401.
[23] Hugen Yan, Xuesong Li, Bhupesh Chandra, George Tulevski, YanqingWu, Marcus Freitag, Wenjuan Zhu, Phaedon Avouris, and Fengnian Xia.Tunable infrared plasmonic devices using graphene/insulator stacks. Nature Nanotechnology, 7(5):330–334, apr 2012. ISSN 17483387. doi:10.1038/nnano.2012.59.
[24] A Das, S Pisana, B Chakraborty, S Piscanec, S K Saha, U V Waghmare,K S Novoselov, H R Krishnamurthy, a K Geim, a C Ferrari, and a KSood. Monitoring dopants by Raman scattering in an electrochemicallytopgated graphene transistor. Nature Nanotechnology, 3(4):210–215, apr2008. ISSN 17483387. doi: 10.1038/nnano.2008.67.
[25] J. W. Weber, a. a. Bol, and M. C. M. van de Sanden. An improved thinfilm approximation to accurately determine the optical conductivity ofgraphene from infrared transmittance. Applied Physics Letters, 105(1):013105, jul 2014. ISSN 00036951. doi: 10.1063/1.4889852.
[26] Saeed H. Abedinpour, G. Vignale, A. Principi, Marco Polini, WangKongTse, and A. H. MacDonald. Drude weight, plasmon dispersion, and ac
191
conductivity in doped graphene sheets. Physical Review B, 84(4):045429,jul 2011. ISSN 10980121. doi: 10.1103/PhysRevB.84.045429.
[27] M Orlita, I Crassee, C Faugeras, A B Kuzmenko, F Fromm, M Ostler,Th Seyller, G Martinez, M Polini, and M Potemski. Classical to quantumcrossover of the cyclotron resonance in graphene: a study of the strengthof intraband absorption. New Journal of Physics, 14(9):095008, sep 2012.ISSN 13672630. doi: 10.1088/13672630/14/9/095008.
[28] B. Macco, Y. Wu, D. Vanhemel, and W. M. M. Kessels. Highmobility In2O3:H transparent conductive oxides prepared by atomiclayer deposition and solid phase crystallization. physica status solidi (RRL)  Rapid Research Letters, 8(12):987–990, dec2014. ISSN 18626254. doi: 10.1002/pssr.201409426. URLhttp://doi.wiley.com/10.1002/pssr.201409426.
[29] Bart Macco, Harm C. M. Knoops, and Wilhelmus M. M. Kessels. ElectronScattering and Doping Mechanisms in SolidPhaseCrystallized In2O3:HPrepared by Atomic Layer Deposition. ACS Applied Materials & Interfaces, 7(30):16723–16729, aug 2015. ISSN 19448244. doi: 10.1021/acsami.5b04420.
[30] Harm C. M. Knoops, Bas W. H. van de Loo, Sjoerd Smit, Mikhail V. Ponomarev, JanWillem Weber, Kashish Sharma, Wilhelmus M. M. Kessels,and Mariadriana Creatore. Optical modeling of plasmadeposited ZnOfilms: Electron scattering at different length scales. Journal of VacuumScience & Technology A: Vacuum, Surfaces, and Films, 33(2):021509, mar2015. ISSN 07342101. doi: 10.1116/1.4905086.
[31] Michel Le Bellac, Fabrice Mortessagne, and G. George Batrouni. Equilibrium and NonEquilibrium Statistical Thermodynamics. Cambridge University Press, Cambridge, 2004. ISBN 0 521 82143 6.
[32] Harald Ibach and Hans Luth. SolidState Physics. SpringerVerlag BerlinHeidelberg New York, Berlin, Heidelberg, 3 edition, 2003. doi: PhysRevB.83.165113.
[33] ITan Lin and JiaMing Liu. Terahertz FrequencyDependent Carrier Scattering Rate and Mobility of Monolayer and AAStackedMultilayer Graphene. IEEE Journal of Selected Topics in Quantum Electronics, 20(1):122–129, jan 2014. ISSN 1077260X. doi:10.1109/JSTQE.2013.2263116.
[34] P Spinelli, M.A. Verschuuren, and Albert Polman. Broadband omnidirectional antireflection coating based on subwavelength surface Mie res
192
onators. Nature Communications, 3:692, feb 2012. ISSN 20411723. doi:10.1038/ncomms1691.
[35] Stefaan De Wolf, Antoine Descoeudres, Zachary C. Holman, andChristophe Ballif. Highefficiency Silicon Heterojunction Solar Cells:A Review. green, 2(1):7–24, January 2012. ISSN 1869876X. doi:10.1515/green20110018.
[36] Damon B. Farmer, HsinYing Chiu, YuMing Lin, Keith A. Jenkins,Fengnian Xia, and Phaedon Avouris. Utilization of a Buffered Dielectric to Achieve High FieldEffect Carrier Mobility in Graphene Transistors. Nano Letters, 9(12):4474–4478, dec 2009. ISSN 15306984. doi:10.1021/nl902788u.
[37] Jianhao Chen, Chaun Jang, Shudong Xiao, Masa Ishigami, and Michael SFuhrer. Intrinsic and extrinsic performance limits of graphene devices onSiO2. Nature Nanotechnology, 3(4):206–209, apr 2008. ISSN 17483387.doi: 10.1038/nnano.2008.58.
[38] Haijian Zhong, Zhenghui Liu, Gengzhao Xu, Yingmin Fan, Jianfeng Wang,Xuemin Zhang, Liwei Liu, Ke Xu, and Hui Yang. Selfadaptive electroniccontact between graphene and semiconductors. Applied Physics Letters,100(12):122108, 2012. ISSN 00036951. doi: 10.1063/1.3696671.
[39] Bram Hoex, S. B. S. Heil, E. Langereis, M. C. M. van de Sanden, andW. M. M. Kessels. Ultralow surface recombination of cSi substrates passivated by plasmaassisted atomic layer deposited Al2O3. Applied PhysicsLetters, 89(4):042112, 2006. ISSN 00036951. doi: 10.1063/1.2240736.
[40] G. Dingemans and W. M. M. Kessels. Status and prospects of Al2O3basedsurface passivation schemes for silicon solar cells. Journal of Vacuum Science & Technology A: Vacuum, Surfaces, and Films, 30(4):040802, 2012.ISSN 07342101. doi: 10.1116/1.4728205.
[41] Dhiraj Sinha and Ji Ung Lee. Ideal Graphene/Silicon Schottky JunctionDiodes. Nano Letters, 14(8):4660–4664, aug 2014. ISSN 15306984. doi:10.1021/nl501735k.
193
194
Appendix A
Mathematical formulation ofthe charge transport in solarcells
A.1 The driftdiffusion equations
The mathematical description of a cSi solar cell is based on a set of assumptions that are summarised in the points (i) till (v) below. These assumptionslead to the 7 numbered equations (A.1) till (A.4) (also below): the Poissonequation; two continuity equations; two equations about carrier statistics; andtwo currentforce relations.
(i) The operation of a solar cell can be described by considering it as a systemof positive and negative charge carriers that can move freely through asolid, while simultaneously also being confined to said solid. It is assumedthat this solid is not subjected to any net external forces or torquesand the reference frame of the solid will always be used to describe anymovement of the free carriers inside. A typical example of such a systemincludes free electrons (negative charge carriers, e−) and holes (positivecharge carriers, h+) that move freely inside of a cSi wafer, but cannotescape it except through (metal) contacts connected to the wafer.
The electrons and holes are characterized by their densities n and p,which can be dependent on position x and time t. In this work the x andt dependencies will not be written explicitly unless extra attention needsto be called to them. If electrons and/or holes (locally) exhibit concertednet motion, this motion will be called current and will be representedby a vector field Jn (for electrons) or Jp (for holes). In this work, Jn,pwill always denote particle currents (as opposed to charge currents) andare measured in units of [Length−2 · Time−1]. Note that x can refer to
195
coordinates of one, two or three dimensions: only vector fields such as Jwill be printed in bold.
(ii) Since the discussion of the solar cell focusses on charged particles, electromagnetic fields play an important role in the description. In solar cells,magnetic fields are too weak to play a role in the operation of the deviceand this makes it possible to reduce the Maxwell equations to a singleequation for the electrostatic potential φ, called the Poisson equation:
∇ · (ε∇φ) = −e2 (p− n+Ndop) = −eρnet. (A.1)
Here, ε = ε0εr is the dielectric constant and Ndop is the backgrounddoping concentration. Note that φ is taken in units of energy here, whichis more convenient in a thermodynamic context because it avoids theneed to multiply φ by e to obtain an energy. Nevertheless, φ will bereferred to as electrostatic energy or potential interchangeably.
(iii) The continuity equations for electrons and holes are given by:
∂n
∂t+∇ · Jn = G−Rn, (A.2a)
∂p
∂t+∇ · Jp = G−Rp. (A.2b)
The time derivatives in Eqs. (A.2) are important when discussing certain solar cell characterisation experiments such as transient photoconductance decay or PCD (i.e., lifetime testing). However, in this workthe main focus is on the steadystate operation of a solar cell when it isproducing net power, so then time derivatives are assumed to be zero:∂n/∂t = ∂p/∂t = 0. In the steady state it is only necessary to assumeRn 6= Rp if the trapped charges are still mobile and can hop to nearbydefects. Here, it will be assumed that trapped charges are completelyfixed, so that the simplification Rn = Rp = R can be used. The termG−R will be frequently abbreviated by Gnet.
(iv) The relation between the carrier density and the potentials, i.e., the carrier statistics. If not stated otherwise, it is assumed that Boltzmannstatistics apply, so that:
n = NC exp
(−EC − EFn
kBT
)= NC exp
(EFn + φ+ χ
kBT
)= NC eµ
cn/(kBT ), (A.3a)
p = NV exp
(−EFp − EV
kBT
)= NV exp
(−EFp + φ+ χ+ EG
kBT
)= NV eµ
cp/(kBT ), (A.3b)
196
or equivalently:
EFn = kBT ln
(n
NC
)− φ− χ,
EFp = −kBT ln
(p
NV
)− φ− χ− EG.
Here, χ is the electron affinity, EC,V the energies of the conduction/valenceband edges, and µc
n,p the chemical potentials. Sometimes the use of quasiFermi energies EFn,p causes a needless confusion of signs, in which caseit is more convenient to work with the electrochemical potentials ηn,p.These potentials measure the free energy of free electrons and holes andare given by:
ηn = EFn = µcn − φ− χ,
ηp = −EFp = µcp + φ+ χ+ EG.
Since free electrons and holes are always generated and annihilated inpairs, another frequently occurring quantity is the free energy pere−–h+ pair, ∆ηeh:
∆ηeh = ηn + ηp = EFn − EFp = EG + kBT ln
(np
NCNV
).
If FermiDirac statistic are required, the exponential functions in Eqs.(A.3) have to be replaced by the FermiDirac integral F1/2:
F1/2 (x) =2√π
∫ ∞0
√y
exp (y − x) + 1dy.
Note that the argument x is dimensionless here. The factor 2/√π is
included such that in the limit of large negative x, F1/2 (x) approachesthe exponential function and Boltzmann statistics are recovered:
limx→−∞
F1/2 (x)
exp (x)= 1.
Like the exponential function, F1/2 has an inverse, which will be denotedby F←1/2 and which can be considered to be the FermiDirac equivalent of
the logarithm. Much like the logarithm, F←1/2(x) is only welldefined for
arguments x > 0 (as long as only the real numbers are considered).
A common way to evaluate the function F1/2 is by using the AymerichHumet approximation [1]:
F1/2 (x) ≈ 1
exp (−x) + 3√
π2
[x+ 2.13 +
(x− 2.132.4 + 9.6
) 512
]− 32
.
197
The AymerichHumet approximation makes it possible to directly calculate the carrier densities from the potentials without the need to performnumerical integration. However, there is no closed form for the inverse ofthe approximation, so to calculate EFn or EFp from the carrier densitiesn and p, it is necessary to use a numerical rootfinding method to invertthe equation.
(v) The currentforce relation for Jn and Jp. The local balances for electronsand holes have been specified in Eqs. (A.2), but these are not enoughto arrive at a closed set of transport equations since they only specifythe divergence of the vectors Jn,p. Additionally, if in Eqs. (A.2) therecombination R depends on n and p (as is almost always the case), itis necessary to specify how Jn,p relate to the other variables. This is thepoint where solar cell physics become truly empirical: all of the previousequations (i.e., Eqs. (A.1)) through (A.3b) are fundamental or a limitingcase of a fundamental law. The Poisson equation follows from Maxwell’sequations (with zero magnetic field); the electron and hole balances followfrom conservation of particles and charge; and the carrier statistics canbe traced back to quantum mechanical principles.
Solar cell physics commonly only considers the diagonal elements of thetransport matrix L (see Eqs. (2.55), Section 2.6) and this convention willalso be followed here, unless stated otherwise. The transport coefficientsare expressed as a product of carrier density and mobility µn,p, thoughgenerally the mobilities are not constant but nonlinear functions of thecarrier and doping densities. Thus, Jn,p are given by:
Jn = −nµne∇EFn = −σn
e2∇EFn, (A.4a)
Jp =pµpe∇EFp =
σpe2∇EFp. (A.4b)
Here, σn,p are the electron and hole conductivities of the material expressed in Ω−1 m−1. It should be noted that the proportionality betweencarrier density and conductivity is not entirely selfevident as it may appear to be. Indeed, in the degenerate regime most carriers are too deepin the Fermi sea to contribute to conduction. For degenerate semiconductors the conductivity is only proportional to the carrier density if thebands are parabolic and demonstration of this proportionality requires amore detailed analysis based on the Boltzmann transport equation (see,e.g., Ibach & Luth [2]). For nonstandard conductors (such as graphene)it is therefore always recommended to check if it is permissible to writethe conductivity as a product of density and mobility.
Equations (A.1) through (A.4) are the seven basic physical equations forthe charge transport in a solar cell. Together, the equations can be solved to
198
obtain the seven unknowns φ, n, p, EFn, EFp, Jn and Jp. These equations haveto be supplemented with models that specify the generation and recombinationrates G and R; the mobilities µn and µp; and the band gap EG and electronaffinity χ.
It is customary to reduce the seven basic equations (A.1) through (A.4) bysubstitution. The most common way to achieve this, is by eliminating EFn,pand Jn,p, which results in:
∇ · (ε∇φ) = −e2ρnet, (A.5a)
∇ ·(−nµn
e∇[kBT F←1/2
(n
NC
)− φ− χ
])= Gnet, (A.5b)
∇ ·(pµpe∇[−kBT F←1/2
(p
NV
)− φ− χ− EG
])= Gnet. (A.5c)
Equations (A.5b) and (A.5c) can be simplified further if Boltzmann statisticsare assumed and if ∇kBT is assumed to be negligible. Then F←1/2 can bereplaced by the natural logarithm and the familiar driftdiffusion equations areobtained:
∇ ·(−Dn∇n+
nµne∇ [φ+ χ]
)= Gnet, (A.6a)
∇ ·(−Dp∇p−
pµpe∇ [φ+ χ+ EG]
)= Gnet, (A.6b)
with Dn,p = kBTµn,p/e the diffusion constants.
A.2 The PoissonBoltzmann equation
The PoissonBoltzmann (PB) equation is a useful approximation to the fullsolar cell transport equations presented in Appendix A.1. It can be used to gainquick insights into the shape of band structures without the need to calculatethe currents flowing through the device. A typical example of an applicationof the PB equation can be found in the work by Girisch [3], where it is used tocalculate the amount of induced band bending in silicon due to a fixed interfacecharge in a dielectric (SiO2 in this case) that has been grown on the silicon.
The derivation of the PB equation uses the approximation that the quasiFermi levels EFn,p are constant throughout the region of interest; it is obtainedby simply substituting the equations of the carrier statistics (Eqs. (A.3)) intothe Poisson equation (Eq. (A.1)):
φ′′ = −e2
ε
[NV F1/2
(−Φp + φ
kBT
)−NC F1/2
(Φn + φ
kBT
)+Ndop
], (A.7)
Φn = EFn + χ, (A.8)
Φp = EFp + χ+ EG. (A.9)
199
Here, the quantities Φn,p have been introduced to simplify the notation. Inequilibrium conditions where EFn = EFp = EF the PB equation is exact,making it useful for calculating equilibrium band diagrams. In nonequilibriumsituations, on the other hand, the gradients in EFn and EFp can be estimatedfrom the typical currents that run through the system and the typical electron and hole densities. For many common devices (such as a cSi solar cellsworking at maxpower point under AM1.5 illumination) it is found that thequasi Fermi levels are approximately constant, so the potential applicationsof the PB equation extend beyond simple equilibrium systems. Moreover, inmany cases it can even be used in situations where one of the quasi Fermilevels is not constant, such as in selective contacts. Consider, e.g., again thehole selective membranes from Chapter 3: in such selective membrane, EFn isnot constant (as seen in Figures 3.2 and 3.6), but since the electron densityis so low anyway, the value of EFn is immaterial when calculating the chargedensity. So for selective contacts it can safely be assumed that EFn is simplyequal to its bulk value (EFn(0) in the figures) everywhere.
Compared to the three coupled, nonlinear, driftdiffusion equations (A.5),the PB equation (A.7) provides a simpler alternative for the calculation ofband diagrams. Furthermore, in situations where it is necessary to evaluatethe full set of transport equations, the PB equation can still provide a goodinitial guess of the solution for iterative numerical solvers (such as a Newtonsolver).
If the material parameters (Ndop, χ, EG, NC,V) are constant in the interval0 ≤ x ≤ d, it is also possible to integrate the PB equation analytically. As anexample, take x = 0 as a point somewhere in the bulk of a solar cell and x = Las the edge of the cell where a fixedcharge dielectric such as Al2O3 is present.The total surface charge in the dielectric is QFixed (in cm−2). This surfacecharge induces a space charge region (SCR) in the semiconductor with an equaland opposite amount of charge QSCR = −QFixed. The boundary conditions arethen φ(0) = 0 (which is simply a choice of the reference potential) and φ′(0) = 0(meaning that in the bulk of the cell the electric field has been shielded by themobile charges). To get rid of φ′′, the PB equation is first multiplied by φ′ andthen it is integrated from 0 to L. For the left hand side this yields:∫ L
0φ′φ′′ dx =
1
2φ′(L)2 (A.10)
Since −φ′/e is the electric field, it is related to the total charge QSCR in theSCR by:
QSCR = − ε
e2φ′(L). (A.11)
Integration of the right hand side of the PB equation (after multiplication by
φ′) requires a primitive function of F1/2, which is denoted by F(1)1/2 (the (−1)
200
should be interpreted as negative differentiation):
d
dxF
(1)1/2 (x) = F1/2 (x) . (A.12)
In the regime of MaxwellBoltzmann statistics where F1/2 (x) = exp(x), the
simplest choice for F(1)1/2 (x) is, of course, the exponential function exp(x) again.
In the regime of FermiDirac statistics, the easiest way to proceed is to tabulatethe integral of F1/2 (x) for fast numerical evaluation. The integrated form ofthe PB equation is then:
Q2SCR =
2kBTε
e2
[NV
F
(1)1/2
(−Φp + φ(L)
kBT
)− F
(1)1/2
(− Φp
kBT
)
+NC
F
(1)1/2
(Φn + φ(L)
kBT
)− F
(1)1/2
(Φn
kBT
)−φ(L)Ndop
kBT
]. (A.13)
Thus, Eq. (A.13) relates the surface potential φ(L) to the total amount ofspace charge QSCR in the semiconductor. The equation cannot be analyticallyinverted (even in the MaxwellBoltzmann regime) to give φ(L) as a function ofQSCR, so a numerical rootfinding algorithm is required if the surface potentialis the unknown. Brent’s method [4] is a robust algorithm that is wellsuitedfor this task. When solving Eq. (A.13), care should be taken that the sign forφ(L) (which should be opposite of the sign of QSCR) is correct.
201
202
References for AppendicesA.1 and A.2
[1] X. AymerichHumet, F. SerraMestres, and J. Millan. A generalized approximation of the FermiDirac integrals. Journal of Applied Physics, 54(5):2850–2851, 1983. ISSN 00218979. doi: 10.1063/1.332276.
[2] Harald Ibach and Hans Luth. SolidState Physics. SpringerVerlag BerlinHeidelberg New York, Berlin, Heidelberg, 3 edition, 2003. doi: PhysRevB.83.165113.
[3] R.B.M. Girisch, R.P. Mertens, and R.F. De Keersmaecker. Determination of SiSiO2/ interface recombination parameters using a gatecontrolledpointjunction diode under illumination. IEEE Transactions on ElectronDevices, 35(2):203–222, 1988. ISSN 00189383. doi: 10.1109/16.2441.
[4] R. P. Brent. An algorithm with guaranteed convergence for finding a zeroof a function. The Computer Journal, 14(4):422–425, apr 1971. ISSN 00104620. doi: 10.1093/comjnl/14.4.422.
203
Summary
Passivating contacts for silicon photovoltaics: Solarcells designed by physics
The central theme of this dissertation is to investigate how the knowledge ofsolar cell physics can be used to contribute to the improvement of solar celldesigns. To answer this question, the traditional semiconductor physics thatare commonly used to describe photovoltaic devices have been reframed in athermodynamic language, since this makes it possible to accurately quantify allefficiency losses in a solar cell. To make a truly thermodynamic description ofsolar cells possible, the field of nonequilibrium thermodynamics was reviewedand applied to the area of solar cell physics. A discussion was presented ofthe differences and similarities between the thermodynamic approach and thetraditional semiconductor description of solar cells.
From the thermodynamic view of a solar cell, the local entropy generationemerged as a new figure of merit to assess the performance of the cell. Wheretraditional solar cell performance parameters only provide global measures,the entropy generation rate provides local information based on all internalloss mechanisms (such as recombinative and ohmic losses) and measures theireffect all on the same scale. This local information was used to develop avariational optimization method that can directly predict the most efficientcell design consistent with the physical limitations of the cell (such as therecombination mechanisms and the doping dependence of the mobility). Thevariational method was illustrated by showing how it can be used to formulatea system of differential equations that determine the optimal shape for thedoping profile in a cSi homojunction cell in complete generality.
One of the most important sources of entropy generation in cSi homojunction solar cells is the recombination at the metal contacts. This loss mechanismwas discussed in detail and several strategies to reduce contact losses were categorised and discussed. These strategies are summarised with the term selectivemembranes and selective contacts. Key features for high quality selective membranes were identified and discussed from a thermodynamic point of view.
The most successful type of selective membrane found in literature is based
204
on hydrogenated amorphous silicon (aSi:H). The main drawback of this typeof membrane is its very substantial parasitic absorption of light in the aSi:H.To reduce the parasitic absorption of aSi:H, a new type of selective contactbased on Al2O3 was introduced. The passivation and contact performanceof this contact was investigated experimentally. It was concluded that Al2O3
cannot fully replace aSi:H yet, however it does make the use of thinner aSi:Hfilms feasible to reduce the parasitic absorption.
Graphene, a material well known for its high transparency and conductivity, was also investigated for its potential as a transparent electrode and asa selective contact. The physics of graphene that are relevant for solar cellapplication were reviewed to assess its viability as a contact material cSi solarcells. It was concluded that graphene shows potential as a selective contactbecause it is significantly less recombination active than an ordinary metal.However, graphene is only usable in solar cells if a stable doping scheme canbe found to engineer its work function.
In conclusion, the work in this dissertation explores how the physics underlying the operation of solar cells can be used not just to describe the photovoltaic conversion process (which current semiconductor physics are alreadyvery successful at), but also how to predict the optimal design of solar cells.
205
List of publications
[1] R M W van Bijnen, S. Smit, K A H van Leeuwen, E J D Vredenbregt,and S J J M F Kokkelmans. Adiabatic formation of Rydberg crystals withchirped laser pulses. Journal of Physics B: Atomic, Molecular and OpticalPhysics, 44(18):184008, sep 2011. ISSN 09534075. doi: 10.1088/09534075/44/18/184008.
[2] D. GarciaAlonso, S. Smit, S. Bordihn, and W. M. M. Kessels. Siliconpassivation and tunneling contact formation by atomic layer depositedAl2O3/ZnO stacks. Semiconductor Science and Technology, 28(8):082002,August 2013. ISSN 02681242. doi: 10.1088/02681242/28/8/082002.
[3] S. Smit, D. GarciaAlonso, S. Bordihn, M. S. Hanssen, and W. M M Kessels.Metaloxidebased holeselective tunneling contacts for crystalline siliconsolar cells. Solar Energy Materials and Solar Cells, 120(PART A):376–382,January 2014. ISSN 09270248. doi: 10.1016/j.solmat.2013.06.016.
[4] Benedicte Demaurex, Johannes P. Seif, Sjoerd Smit, Bart Macco, W. M.M. Erwin Kessels, Jonas Geissbuhler, Stefaan De Wolf, and ChristopheBallif. AtomicLayerDeposited Transparent Electrodes for Silicon Heterojunction Solar Cells. IEEE Journal of Photovoltaics, 4(6):1387–1396, nov2014. ISSN 21563381. doi: 10.1109/JPHOTOV.2014.2344771.
[5] B Macco, D Deligiannis, S Smit, R a C M M van Swaaij, M Zeman, andW M M Kessels. Influence of transparent conductive oxides on passivationof aSi:H/cSi heterojunctions as studied by atomic layer deposited Aldoped ZnO. Semiconductor Science and Technology, 29(12):122001, dec2014. ISSN 02681242. doi: 10.1088/02681242/29/12/122001.
[6] Sjoerd Smit and W. M. M. Kessels. Variational method for the minimizationof entropy generation in solar cells. Journal of Applied Physics, 117(13):134504, 2015. ISSN 00218979. doi: 10.1063/1.4916787.
[7] Harm C. M. Knoops, Bas W. H. van de Loo, Sjoerd Smit, Mikhail V. Ponomarev, JanWillem Weber, Kashish Sharma, Wilhelmus M. M. Kessels, andMariadriana Creatore. Optical modeling of plasmadeposited ZnO films:
206
Electron scattering at different length scales. Journal of Vacuum Science& Technology A: Vacuum, Surfaces, and Films, 33(2):021509, mar 2015.ISSN 07342101. doi: 10.1116/1.4905086.
[8] Benjamin L. Williams, Sjoerd Smit, Bas J. Kniknie, Klaas J. Bakker, WytzeKeuning, W. M. M. Kessels, Ruud E. I. Schropp, and M. Creatore. Identifying parasitic current pathways in CIGS solar cells by modelling dark JVresponse. Progress in Photovoltaics: Research and Applications, 23(11):1516–1525, nov 2015. ISSN 10627995. doi: 10.1002/pip.2582.
207
Acknowledgements
And now for the most important part of this work, as people tend to call theacknowledgements in humorous vein. Then again: what would life be like ifno one would go through the effort to show appreciation to the people aroundthem? So in the grand scheme of things, the acknowledgements may indeedbe the most important part of the thesis when it comes right down to it. It ismy own opinion that expressing gratitude is not one of my strong points and Iprobably fell short in that particular area at various moments during my PhD(and indeed in my life in general). Hopefully the words I’m about to writedown will go some way towards correcting for that shortcoming, though onecannot shake the feeling that words on paper are ultimately little more thaninadequate substitutes for the real thing.
First and foremost I’d like to thank everyone I met during my time atPMP. I know that such a catchall phrase can come off as somewhat cheap,but PMP has been such a nice and stimulating group to work in over the lastfour years. I really mean it when I say I’d like to thank each and every one ofyou (and I’m picturing many of your faces as I write this) for your contributionto the atmosphere of the group. Hopefully I will be able to thank many of youin person when I’m back in Eindhoven for my defence, but inevitably therewill be (ex)PMP members left I will not be able to see. If you are one of thesepeople, hopefully you will read this some time in the future and know that I’mhappy that I met you and worked alongside of you.
Of course, there are some PMP members I got to know better than others.Erwin, thank you for supporting my work from the beginning to the veryend, even when I just went off on my own to chase ideas that were rather farremoved from the original definition of the project. Your confidence in myabilities helped me so much to gain that confidence for myself. I couldn’t havewished for a better mentor. Jeanne and Lianne, both of you have helpedme with so many administrative chores it would have been impossible to keepcount. Your patience often seemed unending and I can only hope that I haven’ttested it too frequently. Cristian, Wytze, Janneke, Joris, Ries, Caspar,and Bernadette (not particularly in that order): I think we can all agreethat my experimental side in physics was never as strong as my theoreticalside, but it certainly improved a lot thanks to your help and patience. Bart,
208
Bas, Jimmy, and Harm: my fellow PV friends and connoisseurs. Thank youso much for all of the discussions and fruitful cooperation. Om maar niet tespreken van het gezwam tijdens de koffiepauzes, lunch and de reizen naar deSiPV :). Door jullie was het allemaal zoveel leuker. Diana, thank you for beingsuch a nice and helpful colleague and friend and for your company during themany train rides we made together. Stefan Bordihn, I’m grateful for yourhelp in getting my first experimental results. Your input was always valuable.
Special thanks go to everyone in the FLASH project and at STW whohelped support this project. I have good memories of the cooperation with thepeople at ECN, particularly Paula and Petra for their experimental supportand Gaby for our theoretical discussions. I would also like to send my thanksto Benedicte and Johannes for their help in the joint experiments betweenPMP and EPFL.
After almost eleven years, this is (for the moment at least) my goodbyeto the Eindhoven University of Technology. I grew more attached to itthan I ever thought I would and I would like to thank everyone involved andeveryone I met for making this the great and “gezellige” university it has beenduring my time here.
Maaike, heel erg bedankt voor je steun, je liefde, en voor het nieuweavontuur in Oxford waar je me in meegetrokken hebt.
Pa, ik weet dat ik veel van mijn sterke en zwakke punten van jou heb. Zoalsje soms hopeloze pogingen om dankbaarheid naar mij te tonen en omgekeerd,maar ook de mateloze interesse in techniek die we delen. Weet alsjeblieft hoeveel het voor me betekent wat je allemaal voor me gedaan hebt. En nog veelbelangrijker: hoe belangrijk het voor me is dat je uiteindelijk ervoor hebtgekozen om je eigen leven weer op de rails te krijgen. Zelfs al gaat het nietaltijd perfect tussen ons, je bent en blijft mijn lieve onmisbare pappa.
Finally, a written work is nothing without a reader. Whoever you arereading this, I thank you for giving some of your time to the thoughts I triedto solidify in this thesis.
209
Curriculum Vitae
09101986 Born in Waalwijk, the Netherlands
19992005 Secondary education, Willem van Oranje College, Waalwijk, the Netherlands
20052009 Mixed propaedeutics in Applied Mathematics and Applied Physics, Eindhoven University of Technology, Eindhoven, the Netherlands
Bachelor of Science in Applied Physics, Eindhoven University of Technology, Eindhoven, the Netherlands
20092010 Master of Science, Education and communication (unfinished), Eindhoven University of Technology, Eindhoven,the Netherlands
Teaching internship at Koning Willem II college, Tilburg,the Netherlands
20092011 Master of Science in Applied physics, Eindhoven University of Technology, Eindhoven, the Netherlands
Traineeship at Phillips Research, Eindhoven, theNetherlands
Master thesis project at the Coherence and QuantumTechnology group, Department of Applied Physics, Eindhoven University of Technology, the Netherlands
20112016 PhD. student at the Plasma & Materials Processinggroup, Department of Applied Physics, Eindhoven University of Technology, the Netherlands
Present Technical Consultant at Wolfram Research Europe Ltd.,Long Hanborough, Oxfordshire, United Kingdom
To contact the author, feel free to send an email to [email protected]
210